Soil and Rock Construction Materials
Soil and Rock...
Soil and Rock Construction Materials
© 1998 G.H.McNally
© 1998 G.H.McNally
Soil and Rock Construction Materials
G.H.McNally BSc, BA, DIC, MAppSc, MIE Aust, CPEng Senior Lecturer in Engineering Geology Department of Applied Geology, University of New South Wales
E & FN SPON
An imprint of Routledge
London and New York © 1998 G.H.McNally
First published 1998 by E & FN Spon, an imprint of Routledge 11 New Fetter Lane, London EC4P 4EE This edition published in the Taylor & Francis e-Library, 2003. Simultaneously published in the USA and Canada by Routledge 29 West 35th Street, New York NY 10001 © 1998 G.H.McNally All rights reserved. No part of this book may be reprinted or reproduced or utilized in any form or by any electronic, mechanical, or other means, now known or hereafter invented, including photocopying and recording, or in any information storage or retrieval system, without permission in writing from the publishers. British Library Cataloguing in Publication Data A catalogue record for this book is available from the British Library ISBN 0-203-47657-3 Master e-book ISBN
ISBN 0-203-78481-2 (Adobe eReader Format) ISBN 0 419 21420 8 (Print Edition)
© 1998 G.H.McNally
Contents Preface 1
Introduction to soil and rock materials 1.1 Scope of the book 1.2 Material categories 1.3 Australian production and resources 1.4 General requirements for rock materials 1.5 The superquarry concept References and further reading
Hard rock materials 2.1 Location of quarry sites 2.2 Quarrying lithologies 2.3 Investigation techniques 2.4 Investigation aims 2.5 Case history: proposed Mount Flora quarry, New South Wales 2.6 Case history: Prospect quarry, New South Wales References and further reading
Sand and gravel 3.1 Environmental constraints 3.2 Investigation and sampling 3.3 Drilling and geophysical exploration 3.4 Friable sandstone and conglomerate: Sydney Basin 3.5 Marine aggregates: North Sea 3.6 Alluvial deposits: Brisbane, Australia 3.7 Glacial deposits: England and Wales References and further reading
Natural pavement materials 4.1 Characteristics 4.2 Strength and stiffness 4.3 Duricrust road gravels 4.4 Other road gravels 4.5 Location and sampling 4.6 Testing and evaluation 4.7 Unsealed pavement materials
© 1998 G.H.McNally
4.8 Beneficiation 4.9 Case history: calcretes, southern Africa References and further reading 5
Blasting and crushing 5.1 Quarry blasting and explosives 5.2 Blast design 5.3 Fragmentation mechanisms 5.4 Geological aspects of blast design 5.5 Primary crushing 5.6 Secondary and tertiary crushing 5.7 Geological input for crusher specification References and further reading
Sizing and processing 6.1 Extraction 6.2 Washing, scrubbing and crushing 6.3 Coarse aggregate screening 6.4 Fine aggregate classification 6.5 Dewatering, desliming and beneficiation References and further reading
Aggregate and roadbase testing 7.1 Aggregate sampling 7.2 Intact rock properties 7.3 Sizing and grading 7.4 Particle shape 7.5 Surface Properties 7.6 Soundness, durability and abradability 7.7 Strength and stiffness of particulate mixes 7.8 Testing of particulate mixes 7.9 Properties of fines 7.10 Aggregate and concrete petrography References and further reading
Concrete materials and mix design 8.1 Concrete aggregates 8.2 Fine aggregates 8.3 Fillers 8.4 Chemical admixtures 8.5 Concrete mix design 8.6 Setting and hardening 8.7 Strength of concrete 8.8 Deformability of concrete 8.9 Durability of concrete References and further reading
© 1998 G.H.McNally
Asphalt and bituminous surfacing 9.1 Sprayed seals 9.2 Asphalt 9.3 Asphalt mix design 9.4 Sealing aggregates 9.5 Stripping and polishing 9.6 Bituminous materials References and further reading
Earthfill and compaction 10.1 Developments in earthworks 10.2 Earth excavatability 10.3 Earthfill materials 10.4 Earthworks design 10.5 Compaction theory—the Proctor test 10.6 Compaction practice—rollers and vibrators 10.7 Specifying and controlling compaction 10.8 Compaction behaviour 10.9 Earthfill reinforcement, drainage and confinement References and further reading
Pavement materials and design 11.1 Pavement design factors 11.2 The pavement structure 11.3 Subgrade assessment 11.4 Moisture and drainage 11.5 Expansive subgrades 11.6 Pavement materials 11.7 Flexible pavement design 11.8 Rigid pavement design 11.9 Pavement performance and strengthening References and further reading
Rockfill and ballast 12.1 Rockfill characteristics 12.2 Rockfill in embankment dams 12.3 Testing and specification of rockfill 12.4 Rockfill in road embankments 12.5 Railway ballast 12.6 Testing and specification of ballast 12.7 Macadam pavements References and further reading
Wave protection stone 13.1 Rubble breakwater design 13.2 Durability of armourstone
© 1998 G.H.McNally
13.3 Other intact rock properties 13.4 Transition zones and core 13.5 Aggregate for marine concrete 13.6 Breakwater quarry investigations 13.7 Blasting and sizing armourstone 13.8 Quality control References and further reading 14
Dimension stone 14.1 Dimension stone petrology 14.2 Quarrying dimension stone 14.3 Stone processing 14.4 Physical properties and testing 14.5 Weathering and durability tests 14.6 Stone conservation 14.7 Case study: the Australian stone industry References and further reading
Limestone and cementitious materials 15.1 Geological exploration 15.2 Geotechnical investigations 15.3 Geomechanical properties of limestone 15.4 Limestone aggregates 15.5 Mining and beneficiation 15.6 Environmental problems 15.7 Cement manufacture 15.8 Cement types 15.9 Case history: the Victorian limestone industry References and further reading
Brick clays 16.1 Properties of fired bricks 16.2 Properties of brick and tile clays 16.3 Mineralogy 16.4 Clay preparation, forming and drying 16.5 Clay firing 16.6 Geology of Australian brick clays 16.7 Investigation and sampling 16.8 Testing References and further reading
Waste, by-product and synthetic materials 17.1 Iron- and steel-making slags 17.2 Blast furnace slag (BFS) 17.3 Steel furnace slag (SFS) 17.4 Boiler ash
© 1998 G.H.McNally
17.5 Coal-mining wastes 17.6 Sand washery rejects 17.7 Demolition wastes 17.8 Synthetic aggregates References and further reading 18
Stabilization and pavement renovation 18.1 Aims and method selection 18.2 Granular stabilization 18.3 Cement stabilization 18.4 Lime and lime-pozzolan stabilization 18.5 Bitumen stabilization 18.6 Pavement renovation 18.7 Investigations for pavement renovation References and further reading
Environmental planning and management 19.1 Environmental objections to quarrying 19.2 Remedial measures 19.3 Statutory EIS requirements 19.4 Example: Diamond Hill quarry enquiry 19.5 Example: Calga sandstone quarry EIS 19.6 Example: Mount Misery and Mount Flora quarry proposals References and further reading
Blast monitoring and control 20.1 Ground vibrations 20.2 Airblast 20.3 Statutory limits 20.4 Monitoring of blast vibration 20.5 Control of ground vibration 20.6 Trial blasts and scaled distance 20.7 Airblast control References and further reading
Quarry reclamation 21.1 End-uses and reclamation strategies 21.2 Quarry landfills 21.3 Planning, procedures and materials 21.4 Reclamation of sand and gravel pits 21.5 Reclamation of hard rock quarries 21.6 Reclamation of brick-pits References and further reading
© 1998 G.H.McNally
The origins of this book go back to 1969, to my first job as a geology graduate. I was put in charge of a laboratory that tested a variety of road construction materials, including natural gravel roadbase, aggregate, concrete and earthfill. These were topics that my university training had scarcely touched upon, yet the small amount of reference literature available at the time was aimed at people already well acquainted with testing procedures and specifications. There was little in print to inform a new practitioner as to why materials behaved in the way they did, how test results could be interpreted, why specifications were strict on particular aspects, and so on. Fortunately, my colleagues and the laboratory staff gave generously of their time and experience to bring me up to scratch, and I had the opportunity of visiting dozens of construction sites (and of learning the hard way, by making mistakes!) The second starting point towards this book came in 1990, when I was asked to prepare a short course on soil and rock materials for the Key Centre for Mines at the University of New South Wales, in conjunction with the materials branch of the NSW Roads and Traffic Authority. This one-week course has now been given five times, in Australia and Malaysia, and its content has been steadily expanded. The idea of presenting the course material in book form came about because there is still no introductory text in this field, although some topics (such as concrete materials) are the subject of many volumes. Other topics, such as pavement design and recycled materials, are dealt with extensively in journals but in few books. Although this book has been written from a geological viewpoint, it is also directed towards geotechnical engineers, environmental consultants, and land-use planners and regulators. Only an elementary knowledge of geology is presumed; indeed, most of the subject matter has been drawn from mining and civil engineering, mineral processing, soil and rock mechanics, ceramics and several other disciplines. This is not a state-of-theart volume, and I have especially avoided going into detail about testing procedures and specification requirements wherever possible, to avoid the discussion becoming tedious. What I have tried to draw out are the reasons why some material qualities are sought and how they may be modified. © 1998 G.H.McNally
One of the problems in writing about natural construction materials is that the literature is voluminous, but poorly accessible—most of it is not only unpublished, but is available only in limited-circulation reports. Furthermore, many of the comments in these pages are based on my own experience and—even more so—that of my professional colleagues. The latter are busy people, not given to writing academic papers about matters that are, in their eyes, everyday knowledge. In reaching out to an international readership, I have tried to keep in mind the difficulties of access to this literature, and differences in engineering practice and terminology. Fortunately, my own country, Australia, contains a wide variety of terrains and construction problems, from those of heavilytrafficked freeways down to unsealed rural roads. Engineering construction here is based on American, British and European practice, though some aspects are drawn from countries like South Africa, which have similar terrain and climate. In citing references I have preferred to quote books rather than journals, and journals rather than limited-circulation conference proceedings, even though the latter are often the most informative. I am grateful to many people for helping me with this book, but two deserve special thanks. The first is my good friend and long-time mentor, Jim Williams (Manager, Scientific Services for the NSW Roads and Traffic Authority), who jointly presented the short courses around which this book is based. The second is the late L.G. (Gerry) Wearne, who was my senior laboratory technician in 1969–70 and who began my education in materials technology. Others who contributed to the short courses include Joe Whitehead, Ed Haber, Greg Won, Ian Stewart and Gary Rigozzi. A number of my former students, especially Ian Wilson, contributed reference material and photographs, and are acknowledged in the text. Greg McNally Sydney, June 1997
© 1998 G.H.McNally
Introduction to soil and rock materials
This book is intended to provide an introduction to the assessment, extraction, processing and environmental management of soil and rock construction materials, from a geological perspective. These geomaterials are sometimes referred to as low-cost resources, or as a category of industrial minerals. In Australia the producers of quarried products are known collectively as the extractive industries. Geomaterials differ from other mineral commodities in many ways: their widespread, though uneven, distribution; the large volumetric demand for them, concentrated around urban areas; their low ex-pit value, because substitutes can always be found; and, consequently, their sensitivity to transport costs. Large and high-quality geomaterial deposits far from cities are worthless, while inferior materials close to customers are often upgraded. The traditional task of geologists in this industry was to locate and prove up deposits meeting specified criteria within acceptable hauling distance of the construction site. With the increasing scale of quarry operations and rising public concern over landscape degradation, this role has expanded. Geologists are now generally part of a project team, in which they may be asked to give advice on the geological aspects of product quality control, blast design, crusher selection, quarry restoration and so on. They will be expected to know enough about downstream processing to prepare a preliminary pit layout and to suggest how the properties of the raw material are likely to influence this. The geologist should certainly take these things into account when planning a quarry investigation, and attempt to map, sample and log drillholes with a wider view than simply evaluating quality and reserves. At a later stage the person responsible for laboratory testing and quality control in a large quarry is also, more often than not, likely to have been originally trained as a geologist. His or her duties may also include those of © 1998 G.H.McNally
the site environmental officer—responsible for matters such as blast vibration monitoring, dust control and pit restoration. A number of significant trends in construction-materials technology have emerged over the past 20 years or so, as outlined below: •
Fewer but larger sites The first of these is towards fewer but larger extractive sites, at the expense of many small ones. Big quarries offer economies of scale: a variety of products, more elaborate processing facilities, large reserves, continuity of operation and access to specialist skills. These operations are better equipped, financially and technically, to meet increasingly stringent environmental and specification requirements, and to accommodate fluctuating market demand. There is a price to be paid for this producer concentration, of course: big quarries are more intrusive within a landscape than small ones; haulage to distant construction sites is more expensive; and price competition is diminished. Maximum use of existing quarries The second development is towards maximum use of existing quarries, even where only inferior materials remain. The aim of this, from the regulator’s viewpoint, is to minimize further landscape degradation at replacement sites. ‘High grading’ and early abandonment of partly
Figure 1.1 Quarry reclamation, the old way. This alluvial gravel pit near Urana, New South Wales, has been simply abandoned. Note that some natural revegetation has occurred, despite a poor soil and gully erosion. On a positive note, this quarry offers a wildlife refuge in an otherwise monotonous farmland plain, and is the only surface exposure of these Late Tertiary gravels in the State. © 1998 G.H.McNally
worked resources are nowadays discouraged. From the operator’s viewpoint this makes best use of fixed capital assets, retains favourably located operating pits, and avoids expensive environmental investigations and legal disputes over new sites. Greater use of upgraded materials The third trend, which is a corollary of the above, is greater use of upgraded marginal materials (or simply non-standard materials, and even wastes) to extend the life of the limited reserves of first-class rock. This can be achieved by blending, stabilization and careful quality control. In effect, the trend is away from natural deposits that happen to have suitable properties, and towards materials that are processed or even manufactured to meet a specification. It is also desirable that a material not be overspecified, to a standard above what the end-use demands, because this is wasteful of resources. Temporary land-use Finally, it is emphasized that quarrying is only a temporary use of the land, and that reclamation of mined-out land should be planned well before abandonment (Figures 1.1 and 1.2). Because old quarries are commonly enveloped by urban growth, this may be self-financing in two ways: first, because the voids can be used as waste disposal sites; and, secondly, the land may be later
Figure 1.2 Preparing for quarry restoration in a north Queensland ferricrete (laterite) roadbase pit. At this stage the ferricrete surface has just been exposed; topsoil and vegetation mulch are stockpiled on the left, thin subsoil overburden in the other two mounds. Low soil fertility and low rainfall inhibit site rehabilitation, and the shallow depth (about 1.5 m) of the ferricrete means that a large area must be stripped to obtain the required volume of gravel. Usually the time interval between stripping and restoration is 6–12 months. © 1998 G.H.McNally
sold for industrial or other higher-value end-uses. In other cases, restoration may be paid for by a levy on existing producers, who benefit from restrictions on competitors entering the market, before being returned to public ownership as recreational facilities.
1.1 SCOPE OF THE BOOK Chapters 2–4 discuss the investigation and assessment of aggregate and roadbase deposits. Emphasis is placed on methods of evaluating rather than searching for these materials, since in most cases their general location will be known beforehand. There appears to be a worldwide trend towards increased production from hard rock quarries at the expense of sand and gravel pits, partly because these are better suited to large-scale extraction and partly because they cause less environmental damage per tonne mined. However, crushed rock sources are more likely to be weathered or altered, and hence to produce stone of suspect durability. They also require blasting, which increases extraction costs and creates vibration nuisances. Chapter 3 also discusses two important developing sources of sand and gravel—marine dredging, and weakly consolidated sandstone and conglomerate. These offer very large reserves, but present problems of salt content and fines disposal, respectively. Chapter 4 deals with natural road gravels, which are a heterogeneous collection of gravel-sand-fines mixtures, such as ‘laterite’ gravel, which are used for pavements in secondary roads. Though formerly favoured because they occurred close to construction sites and required minimal processing, their use in this form is declining. Instead, they are increasingly being upgraded by crushing and stabilization to meet heavier traffic requirements (Figure 1.3). Chapters 5 and 6 discuss the extraction and processing of hard rock and granular materials. Processing is taken to include crushing, particle shaping, screening, sizing, beneficiation and de watering. These techniques—mostly borrowed from mineral processing—are becoming more important as premium sources are exhausted and inferior deposits have to be worked. The chief technical issues here are: in blasting, the replacement of nitroglycerine-based explosives by ANFO, watergels and, most recently, emulsions; in crushing, the wider use of impact crushers, even in moderately strong and abrasive rock, and especially for product shaping; and in sand workings, more extensive application of size classification techniques (Figure 1.4). Chapter 7 describes the testing and specification of aggregate and prepared roadbase. The principal categories of laboratory test methods, and their applicability, are summarized. There have been few major changes in materials testing over the past 30 years, but one has been the introduction of repeated-load triaxial testing to simulate the fatigue effects of traffic on road © 1998 G.H.McNally
Figure 1.3 Calcrete pavement beneath a thin sprayed seal, Morgan, South Australia. This is typical of duricrust road gravels still used with minimal processing (in this case grid rolling, but elsewhere single-stage crushing) for secondary road pavements. The coarse fragments in the foreground have been moved to the edge of the road shoulder during construction, and the roadbase material beneath the seal is somewhat finer.
pavement courses. Another innovation has been the move from prescriptive specifications to ones based on quality assurance and more refined sampling techniques. The use of coarse and fine aggregate in Portland cement concrete, asphaltic concrete and bituminous surfacing—and their differing requirements—are the subject of Chapters 8 and 9. In concrete aggregates (Chapter 8), intact rock strength is now thought to be less important than the tenacity of the cement-aggregate bond, especially where tensile strength is at a premium. In concrete mix design, there is now a wider acceptance of slag and fly ash as cement extenders and fillers, and not just because they are cheap. In bituminous surfacing, asphaltic veneers are progressively displacing sprayed seals, and more emphasis is being placed on skid resistance, low tyre noise and fatigue life in mix designs. Earth embankment materials, compaction and road pavement design are discussed in Chapters 10 and 11. In Australia at least, earthfill compaction standards have not improved over the past 30 years, though lift thicknesses and roller sizes have both doubled. Embankment technology has, nevertheless, greatly profited from the application of geosynthetics, © 1998 G.H.McNally
Figure 1.4 Small sand processing plant, near Renmark, South Australia, which includes a lump breaker, screens, a spiral and bucketwheel classifier, and a hydraulic classifier. A tailings pond allows process water to clarify before discharge to the Murray River (just beyond top edge of photo). The feed is very silty but well-graded Parilla Sand (Pliocene).
particularly for tensile reinforcement (as in ‘reinforced earth’; Figure 1.5). Modern deep cuttings produce less-weathered rock and hence a requirement that rockfill, with its attendant problem of settlement, be accepted in highway embankments. This in turn has dictated that a form of fill zoning be adopted to encompass common fill, select fill, transition zones and rockfill materials. The double requirements of allowing for settlement of high fills and heavier traffic loadings have dictated that pavement thickness and stiffness be greatly increased in freeway-standard roads. This has been achieved partly by the wider use of crushed and bound roadbases, including deep lift asphalt, and partly through the re-introduction of concrete pavements. The effects of cyclic loading, especially by heavy trucks, are now fully appreciated in road design, where pavement life is expressed in equivalent standard axles (ESAs) rather than years. Analytical design methods based on triaxial testing and numerical modelling are gradually supplanting the former empirical approach. Railway ballast, rockfill and macadam pavements are discussed in Chapter 12. These are all open-graded, free-draining broken rock materials, but of different maximum particle size and durability. The chief development in this area has been the widespread adoption of weak rolled © 1998 G.H.McNally
Figure 1.5 Reinforced earth bridge abutments and underpass beneath a freeway under construction at Ourimbah, New South Wales. The solidity of the abutments is deceptive: the cladding slabs are simply slotted together and held in place by steel tendons embedded in the dune sand backfill.
rockfill for embankment dams. This replaces strong end-dumped rockfill, which was sluiced but otherwise compacted under self-weight, resulting in large and long-term settlements. Chapter 13 deals with the even coarser stone used in shoreline protection works. The main geotechnical challenge here is devising blasting procedures for generating armour blocks around 10 tonnes weight and zoning the breakwater to use this stone most effectively. Another problem lies in testing such unwieldy materials; ultrasonic velocity measurements appear to offer much potential. Rock cut and split for use as dimension stone is the topic of Chapter 14. Dimension stone is experiencing a worldwide architectural revival, and indeed it is the only extractive industry with a significant export component, though facing stone has long displaced block masonry as the dominant application. The use of stone veneers as thin as 20–40 mm in facing panels places considerable emphasis on flexural tensile strength and durability, favouring granites over sandstones or limestones. Another important development in this area has been the growth of the stonework preservation and restoration sector, and the emphasis on stone salvage and matching. Chapters 15 and 16 deal with limestone and brick clays, two commodities that are important industrial raw materials as well as © 1998 G.H.McNally
construction materials. This is especially true of limestone, which, though a versatile source of aggregate, crushed roadbase, armourstone and dimension stone, is most valuable as a raw material in cement-making and other chemical processes. Carbonate rock terrains also give rise to unique landforms, soils and faunal assemblages—and therefore to a disproportionate share of environmental opposition to quarrying (Figure 1.6). The continued use of carbonate rock for aggregates, where other rock
Figure 1.6 Quarrying heritage—a limestone kiln, now abandoned, built into a rock face near Mount Gambier, South Australia. The kiln was built out of offcuts from Gambier Limestone used primarily as sawn dimension stone. © 1998 G.H.McNally
types would do as well or better, and of high-calcium limestone for cementmaking, is not easy to defend. Brick clays (Chapter 16) nowadays serve two markets: as a raw material in the mass production of extruded bricks in tunnel kilns; and, to a much smaller extent, as an ingredient in batch-produced pressed ‘boutique bricks’ for facing and restoration. In both applications the natural materials are heavily modified and blended, becoming less dependent on the source rock mineralogy and particle composition. Environmental aspects of the construction-materials industry are the themes of the last five chapters. In Chapter 17 alternatives to traditional ‘mineral aggregates’ are discussed. These include wastes, whose exploitation can both remove landscape eyesores and reduce pressure on natural resources. However, they are not equally prized: most are inhomogeneous and therefore only usable as common fill close to the dump site. By far the most valuable are iron and steel slags, which are today classified as byproducts rather than wastes and are produced to specification. Indeed, blast furnace slag in granulated or pelletized form is more valuable as a cement extender or lightweight aggregate than as roadbase. Demolition materials (crushed bricks, concrete masonry and asphalt pavements) are now being widely recycled, partly in response to Government directives and partly as a means of avoiding tipping fees. The upgrading of inferior pavement materials by means of granular or chemical stabilization is the subject of Chapter 18. In the past, stabilization always performed better in the laboratory than on the road, but modern purpose-built equipment has improved the mixing consistency. Cement and lime-fly ash pozzolans are the most common additives, though foamed bitumen is making a comeback. One important application is the in situ renovation of over-age natural gravel pavements, which in Australia alone could be needed for thousands of lane kilometres on rural highways over the next 20 years. Chapter 19 deals with the principal environmental problems of establishing new quarries, with particular emphasis on their geological justification—to counter the argument that, although the need has been established, a better site is available elsewhere. Minimization of blasting nuisances (Chapter 20) is an important issue during the working life of a quarry, especially since statutory limits for air and ground vibration are now being set far below damaging levels, to where the blast is scarcely noticeable. Ground vibrations are satisfactorily controlled by interhole delays, but airblast suppression presents more difficulties. Face reorientation is one palliative, along with more effective stemming. Blast monitoring is now routine, and the results can be used to improve fragmentation as well as meeting regulatory conditions. The final chapter is concerned with reclamation, with the theme that quarries can no longer be simply abandoned at the end of their economic life. Nor can site rehabilitation be left until last; it must be integrated with © 1998 G.H.McNally
extraction throughout the working life of the pit. However, most pits can be profitably backfilled with waste prior to final reclamation, though this must take into account the prevailing hydrogeological conditions.
1.2 MATERIAL CATEGORIES A simple classification scheme for the construction materials discussed in this book is presented in Table 1.1. The materials are categorized in terms of product size, method of processing, end-use and whether they are soil (i.e. they can be dug without blasting) or rock in origin. Many of the material classes are produced in parallel, such as washed sand being sold for concrete fine aggregate and unwashed sand from the same pit used for
Table 1.1 Classification of construction materials
© 1998 G.H.McNally
bricklaying mortars. Specification requirements vary with the proposed end-use; hence rock crushed for use as sealing aggregate is required to meet more stringent test criteria than that accepted as road sub-base, even though both may come from the same quarry and even from the same parent rock. The amount of selection, winning, processing and quality control required to meet the specification is naturally reflected in the price demanded. Broken rock and cut stone Broken rock refers to material that has been ripped or blasted and possibly passed over a bar screen (or ‘grizzly’) to remove oversize, but which is otherwise unprocessed. In general this product is cobble-sized to bouldersized, with minimal fines. Very durable rock is preferred for breakwater stone and rip-rap, but lower-quality stone is acceptable for rubble and rockfill. Cut stone is rock that has been split, sawn, wire-cut or otherwise extracted in block form. These blocks are further sawn, dressed and finished for sale as dimension stone. Crushed rock Coarse crushed rock ballast is of similar quality to concrete aggregate, but made up of coarser particle sizes and devoid of fines. Slightly inferior source rock is acceptable for fine crushed rock roadbase, which is subjected to less intense loading and for which a proportion of void-filling fines is required to ensure high compacted density (‘dense grading’). Crusher grit and dust are by-products from aggregate production used as a source of ‘sharp’ (i.e. angular and coarse) sand in concrete and as a filler in asphalt. Sands and gravels Sands and gravels are primarily of alluvial origin, although other sources such as dunes, marine deposits and weathered sandstone are also worked. Processing includes crushing coarse gravel (to create rough-faced particles as well as to reduce their size), washing (to remove fines), screening and ‘classification’ (sand size separation by settling velocity). Granulated slag is an artificial sharp sand produced by rapid water cooling. Soil materials The soil materials listed in Table 1.1 are a diverse lot, including weathered rock and boiler ash, whose only common characteristic is that they are relatively easy to dig. Most naturally occurring roadbase materials and select fill are used with little or no processing. Brick clay, on the other hand, © 1998 G.H.McNally
is an industrial raw material and may be ground, blended, moistened and chemically modified. Between these extremes are the stabilized soils, to which sand, cement, lime or bitumen are added to improve their strength, stiffness and durability.
1.3 AUSTRALIAN PRODUCTION AND RESOURCES Production of soil and rock construction materials in Australia currently amounts to about 150 million tonnes annually, with an ex-quarry value of around A$1000 million. The uncertainty is due to different methods of reporting and categorization in different states, and to under-reporting of some materials such as unprocessed roadbase. The official figures indicate that production of crushed rock aggregate is increasing faster than that of alluvial gravel, and that aggregate prices rose 160% during the 1980s, twice the consumer price index increase. A compilation of Australia’s total resources of construction materials would be meaningless, since their location close to markets is much more important than their geological reserves. However, a brief survey of the main aggregate sources in four capital cities (Sydney, Melbourne, Adelaide and Brisbane), which account for about 70% of Australian demand, may throw some light on supply trends. •
Sydney The largest hard rock quarries in the Sydney region work basalts and dolerite for aggregate, and volcanic breccia for roadbase. The volcanic breccia is a marginal-quality material, but it is relatively abundant and closer to markets than the basalt. River gravels and coarse sand are currently extracted from the Nepean-Hawkesbury River floodplain and blended with dune sand for concrete-making. Reserves of both coarse and fine aggregate are declining, and future supplies of the former are being sought from microsyenite intrusions and basalts more than 100 km distant from the city centre (where superquarries capable of producing 5–10 million tonnes per annum (Mtpa) have been proposed). Future sources of fine aggregate are from crushed sandstone and offshore sand bodies. Melbourne About 67% of Melbourne’s aggregate and roadbase requirements are obtained from basalts, the Older Volcanics (east and north of the city) and Younger Volcanics (west and north). Although the total volume of the basalts is very much greater than that in the vicinity of Sydney or Brisbane, there are problems due to secondary mineralization (chloritized ‘green basalts’) and the tendency of glassy varieties to become polished in bituminous surfacing. Most of the non-basalt production is supplied from acid volcanic and hornfels quarries. Construction sand requirements are met mainly
© 1998 G.H.McNally
from fluviatile deposits and dunes; although these require washing, large reserves are available. Adelaide Coarse aggregate for the Adelaide metropolitan area is mostly obtained from seven quartzite and six carbonate (limestone, dolomite) quarries, which together produce about 5 Mtpa. The carbonate rocks are considered to be the best available aggregate sources here, and are mainly used for sealing and concrete batching. The quartzites, which vary between hard sandstones and true silicified arenites, are used for roadbase. Reserves are large and adequate for 70–80 years, but as in other cities these are not well distributed, with quartzite predominating to the city’s east whereas carbonate rock is more abundant to the south. Large reserves of construction sand are contained within Tertiary basins to the south and northwest. Brisbane Brisbane derives most of its aggregate from river gravels dredged from the Brisbane River and the North and South Pine Rivers, but the former is rapidly being depleted and has to be supplemented with crushed basalt, acid volcanics, granite and metamorphics. Roadbase is also obtained from the hard rock quarries. Sand comes mainly from alluvial sources, supplemented by dune mining on North Stradbroke Island.
Although Sydney is undoubtedly the worst-served in geological terms, all four cities have problems in meeting the demand for soil and rock construction materials. Much of Melbourne’s abundant basalt is weathered or altered, Adelaide lacks any igneous rock sources, and Brisbane has to depend on metamorphic rocks and some marginal acid and intermediate lavas. All have environmental problems arising from quarrying, such as the conspicuous Hills Face quarry sites in Adelaide or the presumed connection between dredging and flood damage along the Brisbane River. The expansion of each city has in the past engulfed operating or potential quarry sites, particularly sand deposits. There has been considerable concentration of ownership in the Australian quarrying industry over the past decade or so, although the trend towards very large quarries evident in the UK, where one ballast quarry and seven brick-pits supply most of the country’s needs, has not yet taken hold.
1.4 GENERAL REQUIREMENTS FOR ROCK MATERIALS These may be divided into the requirements of the rock material itself, and those of the source. Rock material Though they vary somewhat, the sought-after qualities of the rock material used for aggregate, ballast, roadbase and armourstone are as follows: © 1998 G.H.McNally
Strength Adequate strength is required to resist crushing, shearing and flexural failure. Strong rocks also tend to have very low porosity (hence superior durability), high elastic modulus (hence toughness) and high specific gravity. Although high intact strength is generally desirable in aggregates, particularly surfacing aggregates, it may result in ‘harsh’ roadbase mixtures that require the addition of fines. Durability This must be sufficient to resist breakdown during the working life of the road pavement or concrete structure. Durable rocks are generally composed of tightly interlocking grains of stable minerals (i.e. those which are unweathered, unaltered and insensitive to water) and consequently are almost devoid of porosity. Shape and size The material must possess satisfactory particle shape and size distribution. These qualities influence the workability of concrete mixes (the ease with which they can be poured, pumped and compacted), their cement demand and durability. In the case of roadbase, poor grading (i.e. an uneven mixture of particle sizes) will reduce the maximum compacted density and hence pavement strength. Unsatisfactory particle shape and grading can increase bitumen requirements for sprayed road seals and asphaltic mixtures, or cause excessive aggregate stripping under traffic. Surface properties The material must also possess satisfactory surface properties, which include bitumen and cement adhesion, chemical non-reactivity and polishing resistance. These characteristics are related to particle mineralogy, surface roughness, adhering moisture films and dust coatings. Unfortunately, good adhesion is often best displayed by porous lithologies, while wear resistance has to be sacrificed to polishing resistance. Rock material sources
The general requirements of rock material sources include the following: •
Reserves There should be adequate proven (i.e. closely drilled, sampled and tested) reserves to last through the working life of the quarry (1–100 years, though 20–30 years is usual), with allowances for wastage. Economic hauling distance The source should be located within economic hauling distance of potential users and capable of being worked without undue mining or processing costs. ‘Economic’ hauling distances are extremely variable, but 40–50 km is common in Australian and British urban areas for quality aggregates. Uniformity A source must be capable of producing a uniform product (or, better still, a range of products), which is within specification or can easily be upgraded. This is often as much a function of the processing equipment as of the in situ rock.
© 1998 G.H.McNally
Acceptability The exploitation of a source must be environmentally acceptable to prevailing community values or (more commonly) capable of meeting environmental constraints imposed by regulatory bodies.
The requirements for quarried rock products will be discussed further in subsequent chapters, but are included here to highlight differences between them. It should be emphasized that, although similar general properties (for example, strength, durability and near-cubic shaped particles) are required from most of the material categories, the specification limits imposed for these can vary with the proposed end-use and are not applied with the same rigour in all cases.
1.5 THE SUPERQUARRY CONCEPT One response to the parallel trends of rising per capita consumption of aggregates and increasing public hostility to new or expanded quarries has been the development of very large quarries capable of producing 5–10 Mtpa of high-quality crushed stone. Though these might be located at relatively isolated inland sites or in remote coastal areas, it is the latter, typified by Glensanda in western Scotland, which have received most attention. Such a pit can replace about 20 medium-sized quarries—neatly increasing production efficiency through economies of scale, while greatly decreasing the overall environmental impact. By using large self-loading bulk carriers, stone can be transported 1000 km by sea at less cost than for 50 km of road haulage, making an international trade in aggregates feasible. The geological characteristics of such a quarry site would include: •
A source of homogeneous hard rock sufficient for up to 100 years of production, say 1000 Mt of probable reserves and 100 Mt of proven (drilled) reserves. Assuming a nominal quarry depth of 100 m, a deposit of this size would occupy about 4 km2. This would most likely be a large unaltered intrusive igneous body capable of being crushed with minimum waste and fines generation. A near-shore location adjacent to deep water, preferably screened from view and with a sheltered anchorage capable of handling ocean-going ships in the 50000 to 100000 tonne class. Although remote from residences, the site would have to be easily accessible to its small workforce.
The success of such a venture would also require suitable terminal depot facilities (for unloading, temporary stockpiling and possible further processing) at coastal ports close to urban markets. The combination of © 1998 G.H.McNally
deep-draught wharves, a sufficiently large waterside storage area and good access to trunk rail and road connections might prove difficult to obtain. It could also incur opposition from nearby residents, not to mention predatory pricing from established local producers! Furthermore, the demand for first-class aggregate (for road sealing, highstrength concrete and railway ballast) is only a small proportion of the total aggregate and roadbase market, most of which would continue to be met by abundant but somewhat inferior local materials. When the superquarry concept was first mooted, it was suggested that up to 40 such pits could be developed in Scotland alone, but only one has eventuated, and more realistic projections suggest perhaps 10 worldwide by the end of the century (though the number of inland 5–10 Mtpa quarries could be much greater).
REFERENCES AND FURTHER READING The following books are general references covering much of the content of this book. More specific references on individual topics are listed at the end of each chapter. American Society for Testing Materials (ASTM) (1948) Symposium on Mineral Aggregates. ASTM Special Technical Publication No. 83. Collis, L. and Fox, R.A. (eds) (1985) Aggregates: Sand, Gravel and Crushed Rock Aggregates for Construction Purposes. Geological Society of London, Engineering Geology Special Publication No. 1. Dutton, A.H. (1993) Handbook on Quarrying, 5th edn. South Australia Department of Mines and Energy, Handbook No. 1. Fookes, P.G. (1991) Geomaterials. Quarterly Journal of Engineering Geology, 24, 3–15. [Introduction to a thematic issue dealing with many quarrying topics.] Institution of Mining and Metallurgy (IMM) (1965) Opencast Mining, Quarrying and Alluvial Mining. Institution of Mining and Metallurgy, London. Institution of Mining and Metallurgy (IMM) (1983) Surface Mining and Quarrying. Institution of Mining and Metallurgy, London. International Association of Engineering Geology (IAEG) (1984) International Symposium on Aggregates, Nice, May. IAEG Bulletin, Nos 29 and 30. Kirk, M. (1993) Coastal quarry or superquarry? A review of strategy for hard-rock coastal quarries. Quarry Management, August, pp. 19–27. Knill, J.L. (ed.) (1978) Industrial Geology. Oxford University Press, Oxford. Lay, M.G. (1990) Handbook of Road Technology, vol. I, 2nd edn, Chs 8, 11. Gordon and Breach, New York. Manning, D.A.C. (1995) Introduction to Industrial Minerals. Chapman and Hall, London. © 1998 G.H.McNally
Orchard, D.F. (1976) Concrete Technology, vol. 3: Properties and Testing of Aggregates, 3rd edn. Applied Science, London. Prentice, J.E. (1990) Geology of Construction Materials. Spon/Chapman and Hall, London. Sand and Gravel Association of Great Britain (SAGA) (1967) Pit and Quarry Textbook. MacDonald, London. Selby, J. (1984) Geology and the Adelaide Environment. South Australia Department of Mines and Energy, Handbook No. 8. Smith, M.R. and Collis, L. (eds) (1993) Aggregates: Sand, Gravel and Crushed Rock Aggregates for Construction Purposes, 2nd edn. Geological Society of London, Special Publication No. 9. Weinert, H.H. (1981) The Natural Road Construction Materials of Southern Africa. Academia, Pretoria and Cape Town. Wylde, L.J. (ed.) (1978) Workshop on the Geology of Quarries. Australian Road Research Board, Report ARR 80. Wylde, L.J. (1979) Marginal Quality Aggregates Used in Australia. Australian Road Research Board, Report ARR 97.
© 1998 G.H.McNally
Hard rock materials
The term ‘hard rock’ construction materials is used here to mean quarried or shot stone, which must be blasted, crushed and screened prior to use, as distinct from alluvial gravels (Chapter 3) or broken rock and duricrust materials (Chapter 4), which are simply ripped and blended. Though more costly to extract than the naturally occurring gravels, quarried hard rock can be processed to deliver a variety of consistent-quality products. These include breakwater stone, ballast, aggregate and roadbase. Inferior materials can also be upgraded by careful blending of screened fractions, using rock either selectively mined from different parts of the quarry or imported from distant pits. Although the geological and economic aspects of quarry site selection and evaluation are emphasized in this chapter, environmental factors are
Table 2.1 Siting criteria for hard rock quarries
© 1998 G.H.McNally
nowadays of equal or greater importance. The first two are summarized in Table 2.1, while environmental requirements are dealt with in Chapter 19. Hard rock quarry sites tend to occupy hilly land of little agricultural value— though not necessarily of low scenic value. Three common types are illustrated in Figure 2.1.
Figure 2.1 Three types of hard rock quarries. See text for explanation. © 1998 G.H.McNally
Below-ground category This is characteristic of thick basalt flows, or horizontally bedded rocks such as limestone, situated on level plains. The main problems are concealment, particularly in the early stages of development, and groundwater inflows below the water table (which may also cause nearby wells to dry up). Irregular weathering profiles and altered zones between flows also cause quality control difficulties. Furthermore, the unweathered flows themselves may vary in quality; some are glassy and some contain more deleterious secondary minerals than others. Hillside type This is cheap to develop, weathering depths are minimal and rock quality—in boldly outcropping and homogeneous intrusives—is generally very good. Blasting costs may be minimized by ‘snakeholing’ or shooting inclined holes at the base of the slope. However, this sort of quarry is most conspicuous and would rarely be approved for development these days unless the faces could be concealed behind ridges, or at least oriented away from the public gaze. Composite type This represents a quarry where extraction is confined to a particular layer; for instance, a quartzite bed, a major sill, a limestone layer, or a very wide dyke. In this situation the quarry shape is dictated by the geology to a greater degree than the previous two categories. Extraction has to be carried out along-strike, and because of the narrow pit width available careful slope design is required to ensure maximum product yield. Rock quality in layered deposits is usually variable—more so vertically than horizontally—hence different products are mined on different benches, and blending may be desirable to make best use of the deposit. With bed strike lengths of many kilometres and generally rugged surrounding topography, opportunities for concealment are good. One visual screening technique that is widely used in both composite and hillside quarries is to work downwards from the top, leaving a facade of undisturbed rock around the pit and only an inconspicuous slot for road access to the workings inside the hill.
Relative to their output of crushed stone, hard rock quarries are smaller consumers of land than sand and gravel pits, but generate the additional nuisance of blast vibration. They also tend to be longer-lived, over 100 years in some cases, and require more capital. Among the economic site selection factors listed in Table 2.1, access to trunk roads and remoteness from residents are tending to become more important, while distance to markets is becoming less so. The likelihood of consent from planning and environmental authorities also looms large in the site selection process; sites likely to be the cause of administrative delays or litigation will be discarded wherever possible. © 1998 G.H.McNally
2.1 LOCATION OF QUARRY SITES The best guide to prospective hard rock quarry sites, as indeed to all extractive mineral sites, is the nearby presence of existing or abandoned workings in similar geological formations. Old pit faces can provide a good idea of the rock types present, their structure and weathering patterns, and bulk sampling locations. Even where old workings are no longer accessible—where, for example, they have been backfilled or built over—local geological knowledge based on their records may be helpful. Background geological data The background geological data on a particular area may be published or unpublished; the more general investigations tend to be published, but more specific information usually remains in geological survey open-file reports. Construction-materials resources on the outskirts of major cities have been the subject of planning studies by public authorities worldwide over the past decades. These investigations have included geological mapping, scout drilling at selected sites and limited suites of testing. Their aims were to identify and classify the principal deposits in a region, and to preserve these as long-term extractive resources by restrictive zoning before they could be sterilized by urban expansion. The primary source in a new area will usually be the regional geological map. In Australia these are mostly at 1:250000 scale, with selected areas mapped at 1:100000; in the UK resource maps are at 1:50000 or larger scales. The larger-scale maps will not necessarily be in published form— many are available only as dyeline plans from mapping authorities. In many undeveloped areas good-quality regional geological maps are a legacy from colonial administrations keen to develop mineral resources, or from previous aid projects. Because most of these maps were not compiled with constructionmaterials exploration as their principal aim, they have to be carefully interpreted. Generally they show bedrock geology well but ignore superficial deposits unless these are thicker than (say) 3–5 m. The legend and accompanying notes (if any) can be used to identify potentially quarryable formations, but very often hard and soft units are lumped together within these formations on the basis of their stratigraphic continuity rather than their economic potential. Formations with definite quarrying potential include limestone and quartzite beds, granite stocks, lava flows and intrusions wider than (say) 50 m. Maps will probably be much less useful for pinpointing thin dykes, minor intrusions and hard quartzite beds or lava flows in otherwise non-prospective sedimentary rock formations. Even where these features are shown, they may be much more numerous than the map indicates, or areally more extensive. At the very least the map will © 1998 G.H.McNally
suggest large areas where further investigation is not warranted and a few sites worth a closer look. Topographic maps Although the regional geological map may suggest prospective hard rock formations, it will not give any indication of their state of weathering (Figure 2.2) or the extent of individual deposits. These will have to be resolved by inspection, initially by driving around the area and subsequently on foot at selected sites. At this stage medium-scale topographic maps (say 1:25000 or 1:50000) may be useful for supplementing the geological map. Orthophotomaps—cheaply prepared topographic overlays on enlarged and tilt-corrected airphotos—are likely to be even more help. These large-scale (1:2500 to 1:10000) maps, in conjunction with airphotos, are more likely to show abandoned quarries, excavations, scrapes and large outcrops—all signposts to prospective sites. Airphoto interpretation is also helpful for locating access roads, drilling water points, fence lines and other vehicular barriers and (not least important!) nearby residences that could be affected by the quarry. Airphotos are usually flown every few years, so their information is more up-to-date than maps.
2.2 QUARRYING LITHOLOGIES Almost any unweathered and unaltered igneous or high-grade metamorphic rock, plus some indurated sedimentary rocks, may be suitable as a source of crushed stone. Lithology is only a rough guide to suitability; dolomitic shale, for example, would be considered an unlikely aggregate source in Canada (where some varieties are reactive in concrete) but it supplies the best-quality stone in Adelaide. Worldwide, the most common source of aggregate is undoubtedly carbonate rock, which is discussed in Chapter 15. In the USA, the largest single market for aggregates, limestone and dolomite make up about two-thirds of the quarried stone. Basic lavas Basic lavas are probably second only to limestone as a hard rock source, owing to their wide distribution and volume (sometimes hundreds of metres thick and covering thousands of square kilometres). They can be variable in quality due to weathering along joints and flow surfaces, because of a vesiculate or brecciated fabric, and as a consequence of high olivine or secondary mineral content. The ‘green’ basalts of Melbourne are good examples of the latter problem, where a significant percentage © 1998 G.H.McNally
Figure 2.2 Cross-section through a quarry in weathered and altered hard rock, showing possible uses for the different material classes present. Note that, whereas weathering intensity decreases with depth, the alteration state may remain constant in affected rock. © 1998 G.H.McNally
Figure 2.3 Columnar structure of basalt lava distorted by flow down hill, Peats Ridge, New South Wales. Each column is about 0.2 m wide, making the rockmass easy to fragment using heave-energy explosive. Note faint bleaching due to alteration at the top of the flow.
of chloritic and smectitic alteration products cause rapid deterioration on exposure. Similar non-durable basalts are common in the northwest of the USA. Thick non-glassy basalt flows are preferred for crushing, although scoria may be useful as a low-grade sub-base. Two significant quarrying benefits found in basalt flows are their non-abrasive mineralogy and the presence of closely spaced columnar joints (Figure 2.3), which reduce crushing and blasting costs respectively. Basic intrusives Basic intrusives such as dolerite are less abundant, but are often superior in quality due to slower cooling and less severe weathering effects. However, deuteric alteration, magmatic differentiation and multiple intrusions can result in several different lithologies of varying quality within a large quarry. Gravity settling of olivine-rich phases can give rise to smectitic alteration products, rendering much of the rockmass useless for concrete aggregate and suitable only as lower-quality roadbase. Thick sills and dykes, say 20 m or more in width, can provide good quarry sites where their strike length is sufficient. Small gabbro bodies may be better still, since they are less subject © 1998 G.H.McNally
to altered or weathered margins and mineral layering. Dolerites are the most widely quarried rocks in South Africa, where their properties have been described by Weinert (1968). Granites Acid igneous rocks are generally less suitable for quarrying than basic lithologies. Granites and related plutonic rocks tend to be more pervasively weathered due to kaolinization within feldspar grains, and to be very abrasive because of their quartz content. Very small increases in porosity, say from 0.5 to 1% and presumably due to microfracturing, can result in large decreases in elastic modulus and other key quality indicators such as aggregate crushing value (ACV) and Los Angeles abrasion (LAA) loss. This is often due to hydrothermal alteration rather than weathering, and the distinction can have important practical consequences: weathered rock quality improves with depth, but altered rock remains inferior. The wide spacing between joints, compared with columnar-jointed basalt, greatly increases the required powder factor and hence blasting costs. Mica and clay liberated during crushing may coat particle surfaces and resist bitumen adhesion. Nonetheless, granites have been quarried successfully in Hong Kong, where they are the main sources of aggregate (Irfan, 1994). Porphyries and microgranites Medium-grained porphyries and microgranites (Figure 2.4) are more satisfactory as aggregate sources. This is possibly due to the presence of late-crystallizing potassic feldspars, which are more stable than early-stage calcic plagioclases, but may also be related to tighter grain-to-grain bonding than is the case with coarser-grained granite and granodiorite. Fine-grained acid extrusives (rhyolite, dacite) tend to vary in strength and durability, and are sometimes flaky due to flow banding or reactive because of the presence of glass. Good polishing resistance is a bonus in some cases. Intermediate igneous rocks (diorite, syenite, trachyte and andesite) are similar to acid rocks in their aggregate-making properties, but are less common. Metamorphic rocks Of the metamorphic rocks, the most attractive quarrying propositions are high-grade gneisses, greenstones (metabasalts) and some hornfelses. Gneiss is widely distributed in high-grade metamorphic terrains, generally Precambrian in age, and is favoured because of its relatively stable mineralogy and subdued foliation. Its geomechanical properties are similar to those of granite. Greenstones are similar, possibly less abrasive but denser. © 1998 G.H.McNally
Figure 2.4 Jointed porphyry, Canberra, ACT, Australia. This face is only about 6 m high, but the 40° forward-dipping joints would present a hazard in a higher bench; the joint set dipping at 80° to the right would be a more satisfactory face orientation.
Some varieties contain a proportion of fibrous minerals, the most objectionable of which is asbestos. Hornfels is quarried simply because of its hardness, which may be such that the crushed aggregate is too harsh for roadbase without the addition of fines. Quartzite Quartzite is widely exploited for roadbase, aggregate and breakwater stone, despite its variable properties. The degree of cementation, reflected in its particle specific gravity, can be quite inhomogeneous. Some ‘quartzites’ are really only moderately indurated sandstones. Other varieties are thinly interbedded with phyllite and metasiltstone, or are actually silicified greywackes and arkoses. Patchy silicification may be due to groundwater movement rather than metamorphism, producing silcretes rather than true quartzites. Even massive and well-cemented quartzites can be difficult to blast without generating oversize or excessive dust (which is a health hazard), and will be the cause of abrasive wear in crushers. Finally, quartzites tend to be either too brittle or too soft for surfacing aggregate, though some gritstones are very skid-resistant. Other metamorphic rocks tend to be too foliated, too micaceous or too weathered to be acceptable, though even slate has been crushed for roadbase © 1998 G.H.McNally
where no better rock was available. Apart from the obvious problem of platy particles, these rocks often contain small quantities of sulphide minerals, which oxidize to sulphuric acid (proportions as low as 0.5% can be troublesome). Indurated sedimentary rocks Some indurated sedimentary rocks are quarried for roadbase and aggregate. By far the most important of these is limestone, which is discussed in Chapter 15, and others include orthoquartzite and silicified greywackes, shales and mudstones (argillites). None is entirely satisfactory as highquality aggregate, due to variable cementation (and hence variable strength and durability), a tendency to polish, and the risk of alkali-silica reaction (ASR) in concrete. They perform better as roadbase, because more fines are produced in crushing and their lack of durability is less critical in this application.
2.3 INVESTIGATION TECHNIQUES The principal means of exploration in hard rock quarry sites is cored drilling, mostly supplemented by rotary percussion (tophammer or downhole hammer) drilling. Compared to foundation investigation and mineral exploration, the amount of drilling performed at quarry sites is remarkably small—only about one cored drillhole per million tonnes of resource in Australia. Some augering and backhoe pitting is generally carried out, mainly to probe the depth of weathered overburden and to fill in detail between outcrops. Geophysical techniques, chiefly seismic refraction and magnetometry, are occasionally used. Core drilling Core drilling is usually performed by truck-mounted wireline rigs using triple tube barrels and water flush. Skid-mounted drills are used on steep slopes and for angled holes. The largest possible core diameter is desirable, both to ensure maximum recovery and to supply the largest possible volume of rock sample per metre drilled. In Australian practice this means HQ core (62 mm diameter), but in the UK core diameters up to 110 mm (P and S sizes) may be possible in weaker and non-abrasive rock. Vertical holes are most common, except in steeply dipping beds or where joint spacing and orientation information is required. Ideally, quarry sites should be drilled on a systematic grid, at about 200 m centres. Once the overall geological structure of the deposit is established by coring, fill-in holes can be drilled by cheaper open hole methods. In the latter case the holes are chip-logged and sometimes geophysically logged (using density, sonic and gamma tools) as © 1998 G.H.McNally
well. Drilling monitors are available to record penetration rate, machine torque and thrust and hence rock hardness, but do not appear to be widely used. Core logging Core logging is based largely on visual impressions and semiquantitative test data. A checklist for quarry drillhole logging is presented in Table 2.2, showing the features to be recorded. The main purpose is to develop a Table 2.2 Checklist for quarry drillhole logging
RQD=rock quality designation.
© 1998 G.H.McNally
three-dimensional geological model of the proposed quarry site, with emphasis on the classes of rock material present and the distribution of weathering and alteration within the rockmass. Core samples will be taken for petrographic examination and for limited geomechanical testing, but the quantity of drillcore available will usually be insufficient for routine aggregate testing. Sometimes additional holes are drilled alongside the first if extra rock is needed for this purpose. In any case the laboratory-crushed samples may bear little relationship to the shape and grading of the eventual quarry product, though they should be a good indicator of its durability. Geological mapping Geological mapping, typically at 1:500 or 1:1000, may be used to supplement the drilling data, although it must be remembered that surface outcrops are likely to be both more weathered and more closely jointed than the rockmass at depth. On the other hand, the visible rock exposures may represent the only really strong and unweathered material present within the deposit! This is a common trap with interbedded limestone/shale formations and granites. Similarly, some hill-capping basalt remnants may appear to be much larger in volume than in reality because of downslope movement of their copious scree. At the reconnaissance stage this mapping may be done using airphoto and topographic map enlargements as a base, but by the time detailed drilling is under way contoured photogrammetric plans should be available. With these, plus supplementary compass-and-tape, stadia and electronic distance-measuring (EDM) surveys, the geologist can prepare a ‘mud map’ of the site. At a later stage a preliminary quarry plan showing the bench and face layout, haul roads, processing plant and stockpile locations will be drawn up. Interactive PC-based mine planning software packages allow a variety of layouts to be tried out. This computer modelling should identify possible mining and environmental problems, and help to plan further investigations to solve these. The main features that might be recorded on site investigation maps are listed in Table 2.3. Trial blasting and crushing Occasionally, trial blasting and trial crushing will be carried out as a final investigation stage. This would usually only be done—because of expense— when there is some doubt about marginal-quality material, to investigate blast vibration magnitudes, or where the quarry product has to meet a particularly strict specification. Normally production blasting patterns and loading, as well as crusher settings, are adjusted on a trial-and-error basis to
© 1998 G.H.McNally
Table 2.3 Checklist for quarry site mapping
EDM=electronic distance measuring.
suit the rock coming out of the face and to satisfy environmental regulations. 2.4 INVESTIGATION AIMS Few quarries close because they run out of rock, but many have exhausted their prime material or been forced to close prematurely because haphazard working has depleted this. Therefore the main objective of drilling and mapping at quarry sites is to determine the quantity and quality of all the rock materials present, with a view to planning © 1998 G.H.McNally
systematic extraction and correctly matching product quality to end-use. In other words, fresh rock should be used as first-class aggregate and not as rubble, and lesser rock grades designated as upper course roadbase, subbase and select fill as their quality decreases (see Figure 2.2). This not only makes economic sense, it is becoming a condition of consent by environmental regulatory authorities. Previous to drilling, the site would have been regarded as a hard rock resource, in other words an area believed on good geological evidence (such as outcrop patterns, presence of nearby quarries in the same rock formation, regional mapping and so on) to be underlain by workable rock in economical quantities. It is now necessary to quantify the resource—by drilling and detailed mapping—into reserves, of which there are three main categories: •
Proved or measured reserves are those which are either so closely drilled (at, say, 100 m centres) or so well exposed that there is no doubt about their continuity in three dimensions. At a new site reserves sufficient for 10–20 years of production will usually be proved up by drilling, although much larger indicated reserves are generally present (in some cases more than 100 years’ worth). Indicated or probable reserves are semi-proven volumes of rock whose grade and tonnage are computed from widely and/or irregularly spaced drillholes. Although these cannot be regarded with the same confidence as proved reserves, it is expected that they will be upgraded once additional drilling is carried out. Inferred or prospective reserves, or simply ‘resources’, are those presumed to exist because of favourable geology or proximity to nearby operating quarry sites, but in which little or no drilling has yet been performed.
Although the determination of rock quality and quantity will always be the principal aim of quarry exploration programmes, much additional information for pit design and for planning can be obtained at very little extra cost during site investigation. Joint orientation and spacing measured during outcrop mapping, for example, is useful for blast design and face slope stability studies (see Figure 2.4). Groundwater depth and quality measured in exploratory drillholes, and rockmass permeability estimated from falling or rising head tests in the same drillholes, can influence the choice of explosive, pump capacity required in deep pits and the likelihood of future aquifer pollution. Much of this sort of information will be required in any case as input for the Environmental Impact Statement (EIS), which must be submitted before developmental approval for the quarry can be obtained from the regulatory authorities (see also Chapter 19). In the © 1998 G.H.McNally
case of a large quarry development proposal, a Public Enquiry may be convened, at which the quarrying company will be expected to answer a wide variety of objections. To do this successfully, a large amount of geological and geotechnical information may be required, much more than would be necessary simply to prove up the quarry’s 20 year reserves. In fact, the requirements for EIS preparation have greatly increased the need for geological and engineering investigations prior to quarry opening, since a proposed operating and restoration plan is now obligatory and the old ‘suck-it-and-see’ approach to pit development is no longer acceptable.
2.5 CASE HISTORY: PROPOSED MOUNT FLORA QUARRY NEW SOUTH WALES The Mount Flora intrusion is a 2.5 km wide microsyenite and gabbro body intruding Triassic sandstone and shale of the Sydney Basin about 7 km NNE of Mittagong, New South Wales. The intrusion covers 770 ha and is one of about a dozen in the area, not all of which break the surface. It is a complex igneous body, the greater part of which consists of a microsyenite laccolith about 200 m thick. This has been intruded by gabbro plugs and faulted, and is overlain in places by extrusive basalt. At this stage only the microsyenite is proposed for quarrying, and its importance lies in the fact that it is the closest unexploited large source (more than 1000 Mt inferred reserves) of aggregate-quality hard rock for the developing southwestern fringe of Sydney. It is also located a few kilometres from a freeway and a main-line railway, and in a sparsely populated area of no particular scenic significance (though close to a proposed national park). These factors have caused it to be regarded as a potential quarry site for at least 20 years, and three phases of investigation had been completed prior to 1990, when development was finally approved. These investigations comprised the following: • Diamond drillholes—36 diamond drillholes totalling 1670 m of coring across the whole of the intrusion, to evaluate geological structure and petrological variation, and to obtain test specimens. • Seismic refraction—18.2 line kilometres of seismic refraction to assess depth of weathering and rock quality in the upper portions of the igneous body. • Percussion drilling—900 m of percussion drilling to supplement coring within the selected initial quarry area of 40 ha. • Geological mapping and airphoto interpretation of outcropping microsyenite. • Trial blasts—two trial blasts, from which 300 t and 120 t of spalls were recovered for full-scale crushing tests. © 1998 G.H.McNally
The drilling outlined 32 Mt of probable reserves within the proposed quarry area, itself divided into two pits by a faulted and weathered zone. Much larger inferred reserves, totalling about 1200 Mt, are available for future development if required. The most unusual feature of the investigation was the extensive use of seismic refraction. Although this technique only penetrates to a depth of about 10 m, it was considered cost-effective for rapidly assessing what is by quarrying standards a very large site, and for estimating depth of weathered overburden and the likely quality of the nearsurface rock. The main problem that the investigations revealed was the extent of deuteric alteration in the upper layers of the intrusion. This has caused the naturally grey microsyenite to turn first pink and then white because of the prevalence of secondary minerals, and also increased the water absorption of the crushed rock up to around 5% in places. The economic result of this is that the upper benches of the proposed quarry will be used mainly for roadbase and concrete aggregate, while better-quality sealing aggregate will be obtained at depth as the proportion of secondary minerals diminishes.
2.6 CASE HISTORY: PROSPECT QUARRY, NEW SOUTH WALES Prospect Hill is a prominent topographic feature rising about 90 m above the surrounding plain at the centre of the Sydney Basin, about 7 km west of Parramatta. The hill owes its form to the presence of a dish-shaped layered basic intrusion about 2 km long by 1 km wide and covering 280 ha. Its average thickness is about 100 m, and quarry development has been carried out down to about half this depth. The intrusion forced its way between flat-lying shales and sandstone, both uplifting and thermally metamorphosing these. A geological section through the deposit is shown in Figure 2.5. The Prospect laccolith is the largest body of igneous rock in the Sydney metropolitan area and the site of the largest hard rock quarry in the region. This location has become even more strategic to Sydney’s constructionmaterials needs over the past 20 years as the suburbs have expanded westwards and surrounded it. Indeed, though quarrying has been carried out at Prospect Hill since the 1870s, more than half the present pit—actually two quarries operated by rival companies—has been excavated since 1970. Production is now in decline due to depletion of the best materials, and Prospect quarry is due to be superseded by Mount Flora and other new hard rock sources over the next decade. In fact, this decline was one of the main arguments put forward in the Mount Flora EIS and at the environmental enquiry in order to justify approval of that project. Nonetheless, Prospect quarry is an interesting example of the effect of geology and location on the development of a hard rock site in a region © 1998 G.H.McNally
Figure 2.5 Geological section through Prospect quarry, west of Sydney, New South Wales.
© 1998 G.H.McNally
where these are few and widely spaced. Though large, about 3 km3, much of the intrusion is very poor-quality rock by aggregate standards, and almost all of the superior upper material has been extracted. Despite these limitations, the site is centrally located in a growing city of three million people, adjacent to a freeway, and has the most extensive quarrying facilities in the state. With selective mining and careful blending, a variety of roadbase mixes, sand and select fill are produced. Furthermore the alternative near-city sources, mainly volcanic breccia pipes, are smaller and also considered to be of only marginal aggregate quality. The geological section (Figure 2.5) shows the igneous layering present in simplified form. The upper 30% of the laccolith is dolerite, grading downwards through olivine dolerite to picrite, which makes up more than half the volume of the intrusion. A thin chilled margin of basalt plus small amounts of late-stage differentiates (pegmatite, aplite and syenite) are also present. The main effect of magmatic differentiation within this intrusion has been to concentrate unstable olivine at depth, where it constitutes 25– 40% of the picrite and causes that rock to disintegrate rapidly on exposure (Figure 2.6). The laccolith has also been subjected to extensive deuteric alteration, which has caused all rock types present to contain between 20
Figure 2.6 Typical bench face at Prospect quarry. The dark rock is olivine-rich picrite, which disintegrates within weeks of exposure, hence the smooth, rounded exposure. The light-coloured rock is better-quality syenitic ‘pegmatite’; note the sharper joint intersections in this more durable material. © 1998 G.H.McNally
and 70% of hydrous secondary minerals (mainly prehnite, zeolites, analcite and calcite). In practical terms, this means that much of the Prospect rock is potentially non-durable and the quality becomes worse with depth. Only small quantities of first-class aggregate are now produced from the remnants of the chilled margin basalt and the less olivine-rich dolerite. With hindsight, the quarry might have been developed in a different fashion, the betterquality rock reserved for use as aggregate and the middlings for roadbase. This would have required extensive drilling and quarry planning, which is scarcely an option in a century-old quarry that has passed through the hands of many operators.
REFERENCES AND FURTHER READING Beaumont, T.E. (1979) Remote sensing for location and mapping of engineering construction materials in developing countries. Quarterly Journal of Engineering Geology, 12, 147–58. Fookes, P.G. (1980) An introduction to the influence of natural aggregates on the performance and durability of concrete. Quarterly Journal of Engineering Geology, 13, 207–29. Haines, A. (1993) Mining geotechnical investigation in quarry design practice. Quarry Management, April, pp. 15–19. Hawkins, A.B. (1986) Site Investigation Practice. Engineering Geology Special Publication No. 2, Geological Society, London. Hoek, E. and Bray, J.W. (1977) Rock Slope Engineering, 2nd edn. Institution of Mining and Metallurgy, London. Irfan, T.Y. (1994) Aggregate properties and resources of granitic rock for use in concrete in Hong Kong. Quarterly Journal of Engineering Geology, 27, 25–38. Oberholsen, R.E. (1982) Aggregates in South Africa: production, properties and utilization. Quarry Management and Products, 9 (April), 253–6. Van Schalkwyk, A. (1981) Geology and selection of quarry sites. Quarry Management and Products, 8 (June), 414–18. Weinert, H.H. (1968) Engineering petrology for roads in South Africa. Engineering Geology, 2, 363–95. Wylde, L.J. (ed.) (1978) Workshop on the Geology of Quarries. Australian Road Research Board Report ARR 80.
© 1998 G.H.McNally
Sand and gravel Sand and gravel deposits are normally considered together as sources of naturally occurring fine and coarse aggregate found mainly in alluvial environments. In former times they constituted the largest mineral commodity extracted in developed countries, but are now being overtaken by crushed rock production. Their popularity stems from being close to users, cheap to extract and easy to process (by minimal crushing, washing and screening). They are well suited to small-scale quarrying operations, providing concrete aggregates and sealing aggregates to local markets. Their present decline in many areas is partly because the best deposits have been worked out or built over, and partly a response to environmental restrictions, which tend to bear more heavily upon sand and gravel operations than on hard rock quarries. The soundness and stable mineralogy of sand and gravel deposits result from their having been subjected to comminution and sorting by natural— mainly fluvial—processes of erosion and transportation. These selectively eliminate weak or porous lithologies and concentrate different size fractions in distinct geological locations. Alluvial sand, for example, is usually composed of more than 90% quartz grains. Gravel is more heterogeneous, but is still largely made up of siliceous metamorphic and igneous rocks. Many alluvial gravels are in fact reworked older conglomerates or terrace deposits, in which the clasts have been subjected to at least two cycles of erosion, transport and deposition. Consequently, only the hardest and most durable stone survives. The geological origins and characteristics of some of the main sources of sand and gravel are described in case-history form later in this chapter, but can be summarized as follows: • Alluvial sources include fans, terraces, channel fills (Figure 3.1) and point bars. The best deposits are usually gravel-rich remnants from pluvial stages within the Pleistocene, reworked Pleistocene glacial materials, or alluvial fans close to active faults along mountain fronts. • Glacial and fluvioglacial sources include outwash sheets, eskers, kames and some moraines. The best deposits are those laid down by meltwater streams beneath the glacier or close to the ice front (Figure 3.2). However, © 1998 G.H.McNally
Figure 3.1 Pleistocene channel fill (‘prior stream’) sand deposit, northern Victoria.
glacial drift in general, particularly the blanket moraine left by retreating ice, is too heterogeneous and clayey to be useful. Aeolian (dune) sands are composed of uniformly sized, clean and wellrounded grains that improve the workability of concrete mixes. They are often used in gap-graded mixes with crushed coarse aggregate for this purpose, or blended with crusher grit to achieve a more even fine aggregate grading. Strandline deposits of beach sand and shingle (gravel) mark higher sea and lake levels in tectonically active or formerly wetter areas. They tend to be smaller in volume and coarser in grain size than dunes, but otherwise well sorted like them. Salt and shell concentrations are sometimes a problem. Marine sources are largely drowned Pleistocene alluvial, fluvioglacial and littoral deposits (Figure 3.3) that have been variably reworked by currents. Sand and fine gravel predominate, with a considerable proportion of sand-sized shell fragments and carbonate grains. Silt and clay sizes are conspicuously deficient. Residual deposits are generally unsuitable as sources of granular material because of their unsound particles and a large excess of clay fines. Nevertheless, duricrusts (ferricrete and silcrete nodules) provide a proportion of the gravel-sized alluvium in many areas of the dry tropics. Leached sandstones and conglomerates can also be large-volume sources of relatively dirty sand and gravel.
© 1998 G.H.McNally
Figure 3.2 Fluvioglacial sand and gravel deposit, southern Norway. (Photo: J.H.Whitehead.)
Figure 3.3 Bucketwheel dredger in littoral sands, Tomago, New South Wales. Note post-like ‘spud’ anchors and floating slurry pipeline at rear of barge. © 1998 G.H.McNally
3.1 ENVIRONMENTAL CONSTRAINTS The environmental problems associated with sand and gravel mining arise from a combination of land-use conflicts and changing community values. Many of the best gravel deposits are located beneath prime floodplain agricultural land, or are within level and well-drained alluvial terraces, which provide flood-free residential land and transport corridors. Off-stream extraction Off-stream extraction of alluvial sand and gravel from abandoned channels, point bars and terraces is a heavy consumer of this land. A typical 5 m thick gravel lens produces about 8 tonnes of aggregate per square metre, while a 30 m high hard rock quarry face might yield 80 tonnes per square metre. A large off-stream operation might consist of several pits and ponds spread over many square kilometres; the Penrith Lakes scheme, west of Sydney (Chapter 21), covers 19 km2, though only about a quarter of this area is being actively mined at any one time. Although these excavations can be screened by trees at ground level, they may be startlingly obvious—as white scars against a green pattern of fields—from elevated viewpoints. On-stream extraction The older alternative of on-stream extraction is nonetheless even more in disfavour, for two reasons: • Dredging and on-stream washing cause muddy plumes to migrate downstream. This is not only visually offensive, it blankets aquatic habitats with loose silt, which furthermore is easily remobilized during subsequent floods. • Gravel removal leaves hollows in the streambed, which the river’s hydraulic processes seek to fill by erosion upstream, so as to maintain an even bed profile. This can cause scouring of bridge piers and abutments, undermining of weir and causeway foundations, and oversteepening of banks. Against these environmental liabilities, which are illustrated in Figure 3.4, on-stream workings can—with care—be made less conspicuous than land pits. They can even be designed to improve river efficiency, by deepening and straightening channels. However, the removal of gravel shoals to increase stream velocity also means that oxygenation is less effective, a particular concern where the normal low-stage river flow includes a substantial proportion of sewerage effluent. Conflict with local residents may arise where gravel mining extends © 1998 G.H.McNally
Figure 3.4 Upstream bed scouring and downstream siltation due to on-stream dredging. In many areas the dredged slurry must now be piped for treatment and muddy tailings may not be discharged back into the river.
© 1998 G.H.McNally
below the water table and pit dewatering is required, since existing users can find their wells drying up or their pumps clogging through sand entry. Aquifer recharge can also be inhibited by slime blankets on pond floors and walls. On the positive side, off-stream workings are by far the easiest of all quarrying operations to rehabilitate, generally as recreational and watersports areas (Figure 3.5).
3.2 INVESTIGATION AND SAMPLING Landforms, maps and logs Sand and gravel deposits are usually found in distinctive landforms such as dunes or alluvial terraces, and consequently a knowledge of Quaternary geology and geomorphic processes is useful in prospecting for them. Some of these landforms can be interpreted from large-scale orthophotomaps with contour intervals of 1–2 m, or from airphotos; very large deposits may be visible on satellite imagery. On the other hand, many of the best sand and gravel deposits owe their formation to higher-discharge bedload streams that were active during Pleistocene time, but which are now obscured by several metres of younger silts of no engineering use (but considerable agricultural value).
Figure 3.5 Aerial view (about 2 km across) of sand mining south of Adelaide. Note urban encroachment on left and rectangular tailings dams, which occupy half the area of some pits. The sand pit on the far left has since been rehabilitated. © 1998 G.H.McNally
Another source of information is surficial geology maps—where these exist. ‘Drift’ or Quaternary geology maps showing glacial, fluvioglacial, alluvial and other unconsolidated deposits cover much of the UK and parts of North America. Even where these surficial deposits are accurately mapped, however, they may not indicate important channel sands beneath younger floodplain silts. In poorly mapped areas, meaning most of the world, logs from water bores and bridge drillholes can be valuable sources of information, since the best alluvial aquifers are also sources of granular materials. Although these logs may not be geologically precise, most drillers can recognize and record coarse gravels, cobbles and clean ‘running’ sand. Furthermore, cable tool drilling is equally applicable to water well drilling and to gravel investigations. Problems in investigations The investigation of sand and gravel deposits presents a number of problems. In the first place, alluvial sediments are extremely variable, both vertically and horizontally. Representative samples need to be large, up to 100 kg or more where the particles are very coarse, and sampling locations need to be close together (25–50 m in many cases). Great care needs to be taken to ensure that both the oversize and fines fractions—the ‘top and tail’ of the grading curve in other words—are included. Secondly, such materials are difficult to penetrate when coarse, densely packed and even cemented. Excavation walls are prone to caving, requiring casing in boreholes and bracing in test pits. Finally, most deposits occur close to or below the water table. This magnifies the problem of excavation support and impedes sample recovery. Trial excavations Trial excavations by means of backhoe pits, hydraulic excavator trenches and bulldozer costeans can be very satisfactory for investigating shallow deposits, since they allow both for bulk sampling and for assessing the variability of the deposit. The depth limits for these excavators are approximately 3 m, 6 m and 10 m respectively (less in cobbles), with the cost increasing with depth. Even the coarsest gravels can be adequately sampled above the water table, and some recovery below it is also possible. Costeans can be deepened by hydraulic excavator pits in their floors, a ‘trench-intrench’ layout. The main problem with such excavations, apart from their depth limitations, is the surface disturbance created. This is directly proportional to their size and a major cause of compensation claims from land-owners. In particularly inaccessible sites, or where backhoes cannot penetrate, hand-dug shafts may still be useful. Mechanical winches, grabs and smallscale blasting will greatly assist progress. Very precise sampling of gravel © 1998 G.H.McNally
and removal of large bulk samples for on-site screening are possible by this method. The drawbacks are high labour costs, the need to erect timber shoring for safety and the near-impossibility of excavating below the water table. Sampling procedures Sampling procedures for both trial excavations and boreholes have to take account of the likelihood that oversize blocks will be pushed aside in smalldiameter drilling, and that fines will be either washed away completely or will be greatly underestimated. In gravels, 30–50 kg samples at 1 m intervals may be required, less in sands. Depth accuracy is not a serious problem in most cases, since samples are composited and related to layers rather than to specific levels. Once recovered, samples have to be carefully mixed and quartered prior to laboratory testing, and allowance made in the test reports for rejected oversize and lost fines. Because of the large samples required in gravel deposits, some on-site preparation and oversize scalping is often needed. A small grizzly, scales and even a small front-end loader may be required. Borehole sample collection also needs some thought. Wet bailer samples should be tipped out into steel troughs to avoid loss of fines; spiral augers should be scraped rather than simply reversed to fling off the soil; and disc augers should be emptied onto canvas or plastic sheets rather than straight onto the ground. Deleterious materials A number of deleterious materials are commonly found in sand and gravel deposits, and these can easily be missed during drillhole sampling. The most prevalent contaminant is clay, in the form of lenses, partings, matrix and coatings on gravel clasts. Many clasts themselves, particularly in torrent bedded deposits, are unsound due to rapid erosion and short transportation distance. Gravel subject to fluctuating water tables may be weathered, stained or encrusted with iron oxides, or may accumulate carbonates and salts (mainly gypsum) in low-lying arid areas where groundwater discharges. Feldspathic and calcareous sands tend to be much weaker, dustier and less durable than quartzose sand. Other deleterious matter includes charcoal, coal, peat, wood fragments, mica, shell grit and some duricrust gravels.
3.3 DRILLING AND GEOPHYSICAL EXPLORATION Sand and gravel deposits deeper than a few metres can usually only be investigated by means of auger or cable tool boreholes. Where these © 1998 G.H.McNally
deposits are predominantly sand, are located above the water table and possess even a small percentage of clay binder and/or capillary moisture, their drilling and sampling are greatly simplified. A variety of truckmounted augers are capable of drilling to depths of 10 m or more; usually the base of the deposit or the water table will be encountered within this depth range. Cable tool rigs can penetrate deeper, through much harder ground and below the water table, but are slower and the sample recovered is usually inferior. Mechanical auger boreholes Mechanical auger diameters range from about 100 mm to 1 m, and sampling accuracy is greatly improved at the larger diameters, though at the cost of much greater rig power and less vehicle mobility. Sample quality can also be improved by excluding the outer mantle of cavings. The larger rigs are capable of penetrating moderately compact fine gravels, but not densely packed or cemented cobbles or boulders. Sample recovery below the water table is close to nil, though some indication of material can be obtained from fragments jammed between cutting teeth or bound with clay to auger spirals. Three different auger designs are shown in Figure 3.6. Bucket augers can recover large and representative samples of sand and fine gravel, but cannot handle stones larger than about 100 mm. Disc augers are suitable for moist or clay-bound sands or sandy gravels, and are cheaper and more mobile than bucket auger rigs. Bucket and disc augers are primarily large piling rigs, with head diameters of 0.6–1.2 m and a depth capability of about 15–20 m in favourable ground. Continuous solid flight augers are quicker, cheaper per metre and can be mounted on lighter vehicles. They are usually only 100–200 mm in diameter, and depth capability is about 20 m. Samples are contaminated by caving and only give a rough guide to layer depths, composition and variability. Depth accuracy and sample quality can be improved by casing to the bottom of the hole and screw drilling ahead of the casing shoe. This involves augering short lengths (say 1–2 m) at a time, then withdrawing the soil core. The problem of caving is also overcome by using hollow flight augers, although much greater rig power is needed to overcome wall friction, and drilling is slower. Samples are obtained by lowering an opendrive tube sampler within the casing and pushing it into the floor of the borehole. Suction drilling techniques Suction drilling techniques are applicable to sand deposits only and include reverse-circulation (RC) rotary, vibrocoring and vibrosuction. These methods make use of the fluidity of saturated sand, negative pore pressure in © 1998 G.H.McNally
Figure 3.6 Three types of power auger used in sand and gravel sampling.
partly saturated sand and its tendency to dilate (bulk up) when disturbed. They are fast and avoid loss of fines, but even a small proportion of gravel may prevent recovery. RC uses a drill string made up of two concentric pipes, which revolve together or simply sink under their own weight. Highpressure air or water is injected down the outer annulus and returned, with the entrained sample, up the inner tube. The sand sample obtained is © 1998 G.H.McNally
Figure 3.7 Method of operation of reverse-circulation drilling, using either air or water as the drilling fluid.
© 1998 G.H.McNally
disturbed but uncontaminated, though its depth can only be estimated. Typical hole diameters are 80–100 mm, with the sample diameter about half this; hole depths can be down to about 40 m. The principles of RC drilling are illustrated in Figure 3.7. Cable tool boreholes Cable tool or cable percussion is the traditional method of drilling and sampling in gravels both above and below the water table. These may be large truck- or trailer-mounted rigs, or smaller folding-tripod ‘shell and auger’ types. The borehole is advanced by surging sediments or rock fragments at the base of the hole into a cylindrical bailer or ‘shell’ equipped with a non-return flap or clack valve (Figure 3.8). Hard bands, boulders and rock are broken down by a heavy chisel. Hence the chisel and bailer are used alternately at the end of different cables, moved up and down in short strokes to pulverize and then bail out the cuttings. Cable tool drilling can penetrate the coarsest and hardest gravels in time, but the bailer samples recovered are thoroughly fragmented and washed, and hence give only a rough indication of grain size distribution. In fine gravels and sands the sample quality is better, but some fines are still lost. In dry or clayey sands the sample can be rammed into a modified bailer without a flap valve, where it is retained by a combination of friction, negative pore pressure and cohesion. Even better sample quality is ensured by hammering or pushing thick-walled tubes into the base of the borehole. It is necessary to keep the casing flush with the base of the hole, to prevent contamination due to caving and sample disturbance due to ‘boiling’ (quicksand conditions caused by water pressure inside the casing being less than that due to depth below the water table). In dry soils water must be added to the hole to facilitate bailing and casing driveage, but fines retention is improved where this drilling water is kept to a minimum. The largestdiameter casing in common use is about 250 mm OD, but diameters up to 1 m are desirable if coarse gravel and cobbles are to be recovered. The maximum size of particle that can be recovered unbroken is about 70% of the casing diameter. Geophysical techniques A number of geophysical techniques, in particular resistivity and electromagnetic conductivity (EM), have been tried for sand and gravel prospecting. These depend on the contrast between the electrical properties of fresh groundwater (high resistivity), bedrock (intermediate resistivity) and impermeable clay (low resistivity). The main purpose of electrical geophysics is to map the course of hidden channels and to select drilling and sampling sites—generally where the buried sand appears to be thickest. Granular sediments being aquifers, the presence of abundant groundwater is © 1998 G.H.McNally
Figure 3.8 Method of sample recovery in cable tool drilling. The reciprocating motion of the bailer is imparted by alternately raising and lowering its cable.
© 1998 G.H.McNally
taken to indicate sand or gravel; the method cannot distinguish the two. Another shortcoming is that dry sands are more resistive than saturated deposits and hence appear to be a different material. EM is at present superseding resistivity because it needs no ground contact and the equipment is now portable, so measurements in the field can be greatly speeded up. Geophysical prospecting is much more important in the search for marine aggregates. The two most important techniques employed are seismic reflection and sidescan sonar. Seismic reflection uses a towed vibration source (‘fish’) to map and probe unconsolidated shelf sediments. ‘Sparker’ sources generate high frequencies and offer high resolution (±100 mm) but only a few metres of penetration, while lower-frequency ‘boomers’ can penetrate to about 30m with depth accuracies to reflectors of about 0.5 m. The sediment type and shape of these bodies can be estimated from the seismic profile and the character of the reflections. Sidescan sonar records detailed bedform information using high resolution in shallow water. This method can delineate seabed topography in some detail, and can also be used to estimate sediment type from the roughness or smoothness of the return, complementing the vertical profiling data from seismic reflection surveys.
3.4 FRIABLE SANDSTONE AND CONGLOMERATE: SYDNEY BASIN Declining reserves of accessible alluvial sand and gravel have led to quarrying of the weak and weathered sandstones and conglomerates that outcrop extensively within the Sydney Basin. Similar deposits are worked in England, from the Bunter Pebble Beds and the Folkestone Sands. The Sydney Basin deposits are weathered, or at least poorly consolidated, to depths of 20–30 m and are generally soft enough to be dug by front-end loaders. Harder layers are ripped, but crushing is avoided due to the high abrasive quartz content of these formations. Oversize slabs may be broken down beneath bulldozer tracks or by exposure to wetting and drying (slaking) on the pit floor. The final stage of lump-breaking and disaggregation is carried out in logwashers (Figure 3.9) and screw classifiers. The main products are sand and fine gravel, but the stronger sandstones yield a proportion of coarse (5–75 mm) fraction, which can be used as macadam roadbase for secondary roads. Because the disaggregated rock is poorly sorted (i.e. well graded), a variety of products including fine aggregate for concrete, mortar sand and filling sand can be generated. The angularity or ‘sharpness’ of the coarse sand particles, due to silica overgrowths, is advantageous in producing high-strength concrete for thinwalled castings and for skid-resistant asphalt surfacing. However, in © 1998 G.H.McNally
Figure 3.9 Weakly cemented sandstone being disaggregated in a logwasher (note contra-rotating paddles), Kangaloon, New South Wales.
pumped concrete the same characteristic may cause excessive pipe and pump wear. From an environmental planning viewpoint these formations represent practically unlimited resources, in which extractive sites can be chosen so as to minimize their impact on the landscape and to relieve demand on premium aggregate sources. Present output of sand, pebbles and roadbase from friable sandstones in the Sydney region is about 5 Mtpa. Pits can be excavated so that their final shape is compatible with the adjacent topography, or they can be shaped to a specific end-use, such as residential or industrial subdivisions. Quarrying followed by landfilling is a particularly attractive proposition in the Sydney area, where sites are more valuable per cubic metre of dumping space than for the aggregate product. Sandstone landfill sites can be located in areas of low scenic and agricultural value, and can be easily screened by natural forest and topography. The main shortcoming of friable sandstone is that it contains 10–30% of clay and silt matrix, mainly kaolinite, which must be washed out and disposed of in tailings dams. These lagoons occupy large areas of land, usually along drainage lines since the sandstone terrain is hilly. Some have been overtopped during heavy rain, resulting in downstream siltation and turbidity. Careful design of flow diversion banks and bypass spillways will reduce this risk, though off-stream tailings disposal is preferable. © 1998 G.H.McNally
The necessity for washing and sizing friable sandstone has three positive benefits: • A number of higher-value products such as glass sand, foundry sand, granular filters and silica can be obtained in addition to fine aggregate. • Well-crystallized kaolinite, currently discarded into tailings dams, has potential uses as a brick-making blend clay and as an industrial raw material. Brick-making requires only dewatering of the clay tailings, but higher-value end-uses necessitate further beneficiation. • The tailings can be mixed with other discards and used for pit reshaping and as a base for topsoiling, or even as a topsoil extender where no better material is available.
3.5 MARINE AGGREGATES: NORTH SEA Offshore sand and gravel deposits laid down on the continental shelf during Pleistocene low sea levels supply about 13% of British requirements, or about 20 Mtpa, mainly to London and southeast England. However, Japanese consumption of marine aggregates is the world’s largest, at about 80 Mtpa. Marine gravels are cleaner, more rounded and more uniformly graded than their onshore equivalents; this produces concrete with improved workability and reduced water/cement ratio for the same strength. The smooth surface texture of marine aggregates means, however, that they are unsuited to high-strength concrete or wearing-course asphalt. Although these deposits present both practical and environmental problems, and have large capital requirements in terms of sea-going dredgers and onshore terminal facilities, the availability of reserves close to urban markets is most attractive. These aggregate bodies include drowned beaches and beach ridges, buried alluvial fills, erosional lags and shelf sand bodies. The best prospecting targets appear to be adjacent to major river valleys extending out onto the continental shelf. In the UK extraction of marine aggregates is carried out using trailing suction or—less commonly these days—forward suction (anchor) dredgers of up to 10000 tonnes capacity (Figure 3.10). A typical British dredger has a capacity of 4500 tonnes, can fill in 2–3 hours at a rate of 9000 m3/h (20% solids content) and discharge in 3 hours—the latter being more critical to profitability. The older ships equipped with onboard pumps work to depths of about 25 m, but newer dredgers with submerged pumps can operate down to 45 m. Sizing and washing of the sand onboard is possible, though it may be prohibited because of the resulting silt discharge. Trailing dredgers (Figure 3.10) are best suited to extensive but thin sand sheets, while anchor dredgers work over smaller areas but dig deeper—several metres instead of only 25 mm or so—and can lift gravel-sized particles. © 1998 G.H.McNally
Figure 3.10 Two types of marine sand dredger. The trailing suction head skims sand along parallel strips of the seabed, while the forward suction type excavates a pit or trench while swinging at anchor.
Practical problems The practical problems associated with marine aggregates are mainly due to their salt content, or rather their chloride-ion content, which can corrode steel reinforcing rods and react with cement paste. Finished concrete surfaces may exhibit white efflorescence due to salt leaching out. Freshwater washing can easily reduce chloride content from 1–2% asdredged to 0.1% or less, but 0.6% is usually considered satisfactory. Some authorities claim that in most cases the effects of salt in the aggregate and even of mixing concrete with saltwater are not significant, but care has to be taken against unusual concentrations in particular size ranges. Stockpiled sand will increase in salt content due to evaporation in hot weather, and may reach high concentrations if wet sand is repeatedly added to the pile. A high proportion of shell fragments and unsound calcareous sand grains will also reduce the value of marine sands, to the point where they can only be used as hydraulic fill for land reclamation. © 1998 G.H.McNally
Moderate amounts of shell reduce concrete workability, but have little effect on strength or other properties. Environmental problems The environmental problems of marine aggregate extraction are related to disturbance of underwater habitats and to the erosion/deposition balance in offshore sand bodies. Dredging may induce beach erosion downcurrent by intercepting sand, or it may kill marine grass by silt deposition. Detailed studies of seafloor morphology and of wave, tide and current interaction may be required before large-scale exploitation of marine sand and gravel resources is permitted. However, dredging is now technically feasible in water depths of 50 m, and deeper extraction may be possible in the future. This means that sand beds far offshore can be worked, well beyond the likely influence of beach erosion processes.
3.6 ALLUVIAL DEPOSITS: BRISBANE, AUSTRALIA The principal source of aggregate for the Brisbane metropolitan area over most of the past century has been gravel and sand dredged from the bed of the Brisbane River, which meanders through the centre of the city and its suburbs. During this time about 40 Mt has been extracted, from a total resource of perhaps 100 Mt (Malempre, 1990). These gravels were eroded during the Tertiary from nearby fault-uplifted blocks of igneous and metamorphic rocks, by streams that were rejuvenated by sea-level fluctuations of more than 100 m during the Pleistocene. Originally the gravel/sand ratio averaged 65/35, a high proportion for a non-glaciated terrain, in deposits up to 30 m thick. The gravel content is greatest upstream, close to the source rocks, and sand predominates in the lower reaches. In the currently worked reaches, gravel constitutes only about 10% of the dredged product. Production fell by about half, from 3 Mtpa to 1.5 Mtpa, following a disastrous flood in 1974. The severity of the damage was partly due to riverbank collapse, which carried away many new and expensive houses. This was blamed by the public on channel overdeepening; the gravel dredgers claimed in reply that their activities had prevented many previous floods by allowing quicker passage of peak flows. Restrictions subsequently placed on depth of dredging lost the industry 30 Mt of reserves. During the 1980s the dredging companies were subjected to further criticism from riverside residents because of noise, although in this instance the operators accepted a code of self-regulation to minimize the nuisance. Nevertheless, it had become obvious that the industry would have to move, and the North Pine and South Pine Rivers, located about 30 km north © 1998 G.H.McNally
of central Brisbane, offered one suitable replacement area. Terrace, channel and point bar deposits of Pleistocene (Last Interglacial) age occur along about 10 km of the South Pine River and 7 km of the North Pine River. Deposits within this 30 km2 area are being developed to meet strong local demand, as well as to make good declining yields from the Brisbane River. The deposits and their investigation are described by Hofmann (1980). The project is similar, but on a smaller scale, to the Penrith Lakes scheme, west of Sydney. In both cases the geological and environmental investigations were largely carried out by third parties, to ensure that the whole resource was properly assessed and managed. This means that the deposits will be systematically and fully mined and not just ‘high-graded’, that mistakes made with extraction along the Brisbane River will not be repeated, and that progressive restoration will take place. Extraction remains in the hands of quarry operators working individual leases within the overall development area. The exploration programme for the Pine Rivers project included mapping of surface geology on 1:5000 and 1:10000 orthophotomaps, airphoto interpretation, resistivity depth probing (unsuccessful) and, most important, stratigraphic drilling. The aim of this was to delineate the total resource and its quality variations, using a total of 83 holes, which were drilled to an average depth of 10 m. Half of these were put down by 108 mm diameter continuous flight auger, 13 by a 900 mm bucket auger and the rest by reverse-circulation vibrosuction and non-core rotary drilling. From these holes 120 bulk samples were submitted for testing, mainly for particle size distributions; however, a few particle shape, sulphate soundness and alkali reactivity tests were performed. The investigators concluded that about 70 Mt of the in situ resource was currently extractable in 25 deposits, within a maximum overburden/product ratio of 1/1 and maximum cover depth of 10 m. While this was regarded as a satisfactory result, some problems were highlighted and their solutions outlined: • Coarse aggregate The average proportion of coarse aggregate (+5 mm)* was only 40%, where 60% would have been preferable; this deficiency will have to be made up from hard rock quarries. Oversize (+37.5 mm) averaged 10% and fines (-75 µm)* were 5–40%. • Off-stream pondages Extraction by channel dredging in the past has caused erosion of nearby bridge abutments and has possibly aggravated bank collapse after floods. Future exploitation will be restricted to offstream pondages, which can also confine turbid wash water and are suitable for restoration as ornamental lakes. * Note that throughout this text we use the notation +5 mm and -75 µm, for example, to indicate material of size greater than 5 mm and material of size less than 75 µm, respectively. Also, we use micrometres (µm; 1 µm=0.001 mm) where appropriate. © 1998 G.H.McNally
• Dragline mining Most of the resource, particularly the coarsest fraction, occurs below the water table. This will necessitate dragline mining, a method that has in the past been hindered by the presence of a persistent tough clay band within the gravel. Clamshell dredges will be needed to extract below this horizon, where it is present. • Land ownership In this area land ownership is fragmented and some deposits are already being threatened by suburban encroachment. Many land-owners were unwilling to allow drilling on their property, fearing that it might be a prelude to resumption of mining. Control over exploitation is divided, in Queensland as elsewhere, between several state and local government authorities. Potential conflicts here are being overcome by adoption of a joint extraction and land rehabilitation strategy.
3.7 GLACIAL DEPOSITS: ENGLAND AND WALES For much of the world, especially the industrialized countries of North America and northwestern Europe, sand and gravel deposits are largely synonymous with glacial and, even more so, fluvioglacial deposits. The British literature is dominated by the topic of ‘drift’ deposits rather than hard rock quarrying (see, for example, Smith and Collis, 1993; Merritt, 1992; Crimes et al., 1994). There are several possible reasons for this interest. First, though sand and gravel now supply less than half the UK production of aggregate, they are still the preferred choice for concretemaking. Secondly, these deposits are widespread but extremely variable in size and quality, and therefore their location and evaluation are more challenging than exploration for hard rock quarries. One measure of this is the systematic evaluation carried out over 30 years by the British Geological Survey, which up to 1990 had produced about 140 reports covering perhaps one-tenth the area of Great Britain. Finally, their production costs are still relatively low, relative to marine aggregate and hard rock sources, while haulage costs are kept down by the wide distribution of the pits. The term ‘glacial deposits’ includes subglacier, ice contact, fluvioglacial, glaciolacustrine and periglacial deposits, reflecting the complex history and distribution of these materials. This complexity results from multiple advances and retreats of the ice front, even within a single glacial stage, excavation and burying of older deposits, and postglacial modification by mass movement and alluvial reworking. Merritt (1992) draws a distinction between areas of northern England and Wales affected by the Last Glacial, which climaxed about 18000 BP, and the Midlands where much older (around 450000 BP) deposits are exposed at the surface. In the first case the glacial landforms, being younger, are more sharply defined and often easily recognizable on airphotos. They are also attractive materials sources in © 1998 G.H.McNally
being less affected by post-depositional frost heaving, ice shoving and mixing. Conversely, the older deposits have been reshaped and degraded by subsequent periglacial climates and fluvial action. Though considerable resources of sand and gravel may be present, they are concealed beneath relatively featureless clay till. The most useful sources of granular materials are eskers, sinuous ridges of relatively clean, coarse sand and gravel laid down by meltwater streams flowing beneath the ice. Kames (ice-contact deltas and terraces) also show much potential, though they include more fines. Outwash fans and terminal moraines are more extensive, but are also more variable in grain size, fining rapidly away from the ice front. Glacial debris derived from areas of sedimentary rocks is also likely to be deficient in gravel compared with that gouged from hard rock terrain. The methods of materials investigation in this geological environment are reviewed by Crimes et al. (1994). They comprise: • Archival databases, built up from borehole and pit logs, quarry records and test results (mainly particle size distributions). Though the volume of this information is huge, running to tens of thousands of data points for some projects, its quality is variable and the coverage very uneven. For example, most boreholes are shallow site investigation holes concentrated in urban areas. The information has to be filtered by an experienced geologist to identify the 10 or 20% that is useful. • Geomorphological mapping, based largely on airphoto interpretation and walkover surveys, supported by satellite imagery. The aim is to build up a terrain model, on the assumption that the visible landform reflects the geological materials beneath/Certain areas, such as former ice sheet edges and meltwater channels, become targets for follow-up work, especially drilling and pit excavation. About 5 km2 can be mapped per day for compilation at 1:50000. • Shell and auger drilling, which was the most successful exploration technique used once a potential deposit had been identified by mapping. A typical coverage is about one borehole per square kilometre, but irregularly spaced. Satisfactory samples were obtained drilling ‘dry’ at 200–250 mm diameter, though progress was slow in dense sands and coarse gravels.
REFERENCES AND FURTHER READING Brown, B.V. (1990) Marine aggregates, in Standards for Aggregates, ed. D.C.Pike, pp. 64–91. Ellis Horwood, London. Crimes, T.P., et al. (1994) Techniques used in aggregate resource analysis in four areas in the UK. Quarterly Journal of Engineering Geology, 27, 165–92. © 1998 G.H.McNally
Dixon, A.J. (1988) Sampling sand and gravel deposits. Quarry Management, October, pp. 45–52. Fookes, P.G. and Higginbotham, I.E. (1980) Some problems of construction aggregate in desert areas (parts I and II). Proceedings, Institution of Civil Engineers, 68 (i), 39–90. Hofmann, G.W. (1980) Aggregate Resources of the Pine Rivers Area. Geological Survey of Queensland, Publication 375. Malempre, J.L. (1990) Gravel dredging in the Brisbane River. Quarry Management, January, pp. 33–7. Merritt, J.W. (1992) A critical review of methods used in the appraisal of onshore sand and gravel resources in Britain. Engineering Geology, 32, 1–9. Sinclair, J. (1969) Quarrying, Opencast and Alluvial Mining. Elsevier, Amsterdam. Smith, M.R. and Collis, L. (1993) Aggregates—Sand, Gravel and Crushed Rock for Construction Purposes, 2nd edn. Geological Society, Engineering Geology Special Publication No. 9. Thurrell, R.G. (1971) The assessment of mineral resources, with particular reference to sand and gravel. Quarry Managers Journal, 55 (1), 19–28. Thurrell, R.G. (1981) The identification of bulk mineral resources: the contribution of the Institute of Geological Sciences. Quarry Management and Products, 8 (March), 181–93. US Bureau of Reclamation (USBR) (1975) Concrete Manual, 8th edn, Ch. 2. US Bureau of Reclamation, Department of the Interior, Washington, DC.
© 1998 G.H.McNally
Natural pavement materials These materials comprise a diverse range of naturally occurring granular soils, dirty gravels and weathered rock, which are used in relatively unprocessed form as flexible pavements for secondary roads. Roads of this type are common in rural and developing areas around the world, typically carrying 100–500 heavy vehicles per day. They are designed as two-lane, single carriageways with priority given to all-weather operation and lowcost construction over speed. The usual surface treatment is a sprayed bitumen seal topped with stone chips. Such pavement materials are variously known as natural gravel, road gravel or soil aggregate. Though called ‘gravels’ for convenience, they are in fact gravel-sand-silt mixtures with a small proportion of clay binder. Furthermore, ‘gravel’ is used in the general sense of any particles coarser than 2–3 mm, including rock fragments, concretions and water-worn pebbles. Natural gravels are usually of marginal quality in terms of pavement material specifications for urban roads, where they might at best be acceptable as sub-base. Nonetheless they can perform satisfactorily in lightly trafficked rural highways and local roads, especially where well compacted and well drained. They are the most widely used road-making materials in the world because they are the most economical. First, they require only rudimentary processing (such as in-pit mixing), but generally no blasting, crushing or screening. Secondly, being locally available, they incur minimal haulage charges. Thirdly, they can be worked by simple equipment and are well suited to the dry tropics and to expansive clay subgrades (since they are more flexible than crushed rock pavements). In areas like southern Africa and outback Australia, production of natural road-making gravels far exceeds that of quarried basecourse materials. However, the distinction between natural gravel and prepared roadbase is fading, as more of the former is upgraded by chemical or mechanical stabilization (see Chapter 18), or by in-pit or on-road processing.
4.1 CHARACTERISTICS Although it is difficult to generalize about such varied and widespread deposits (Figure 4.1), natural pavement materials tend to have the following characteristics: © 1998 G.H.McNally
Figure 4.1 A comparison of particle size distributions for various naturally occuring road gravels with dense-graded fine crushed rock (FCR) roadbase. © 1998 G.H.McNally
• Coarse-grained They are often very coarse-grained (have an excess of gravel and rock fragments) and are gap-graded, due to a deficiency in medium to coarse sand (roughly 0.3–3 mm). In other words, the soil aggregate component is large relative to the percentage of sand-silt-clay fines. • Weak and unsound The coarse particles are weak and unsound by concrete aggregate standards, often angular or ragged in shape, and may be quite porous and absorbent due to weathering. At the other end of the size range, the clay particles are often weakly cemented by soil-forming processes. • Moisture-sensitive Both the soil aggregate and the fines fraction are more moisture sensitive than those in crushed rock roadbase. The coarse particles absorb water, reducing their effective strength, while the natural clay binders swell on wetting and shrink on drying. • Self-cementing A self-cementing action is common and may significantly increase the strength of the pavement with time. Another strength increment comes from soil suction, negative pore pressure generated as the pavement material dries out. • Inhomogeneous deposits These deposits tend to be very inhomogeneous, owing to their dependence on soil-forming processes of mineral solution, leaching and replacement. Clay content generally increases sharply with depth, and the proportion of gravel-sized particles may vary greatly. • Shallow and broad deposits Deposits tend to be shallow and broad, typically 1–3 m deep, and pit workings are therefore laterally extensive in relation to the volume of material produced (Figure 4.2). This type of gravel pit therefore has significant environmental impact, with high restoration costs per tonne extracted.
4.2 STRENGTH AND STIFFNESS The shear strength and resistance to deformation (stiffness) of a road pavement, and hence its load-carrying capacity, are derived from a number of factors (Figure 4.3). These include the following: • Tight packing, which is achieved by having an even (‘dense-graded’) mixture of gravel-, sand- and silt-sized particles, and by vibratory compaction. This causes the finer grains to fill voids between coarser ones, imparting dry densities of up to 1.8–2.1 t/m3. • Mechanical interlock between coarse particles, as exemplified by macadam pavements and railway ballast. These ‘open-graded’ mixtures contain few fines and hence their compacted densities are relatively low, but high shearing resistance is generated by interparticle friction. © 1998 G.H.McNally
Figure 4.2 Typical road gravel pit, western New South Wales. This scrape is deeper and narrower than most, and overburden has been stockpiled at the edges for site rehabilitation.
• Confinement by wide shoulders or rigid kerbs, and especially by soil suction. The pavement can also be reinforced by geosynthetic membranes. • Cementation, provided by natural ‘petrifaction’ or artificially by cement, lime or bituminous binders. • Effective sealing to prevent moisture infiltration through the road surface into the pavement courses. • Hard foundation, provided by a dry, well-compacted subgrade located far above the water table. These attributes are sought in all pavements, but the particle soundness and grading deficiencies of natural gravels mean that seal integrity, subgrade strength, soil suction and self-cementation must compensate. A summary of the differences between crushed rock and natural gravel roadbases is given in Table 4.1. The strength of gravel pavements is derived from a combination of the above factors, though the balance between these varies with the material. For example, in Figure 4.1 the graded macadam draws its strength chiefly from particle interlock, whereas suction is the significant factor in the strength of the sandy loam. Nevertheless, dense grading is the primary means by which strength and stiffness are maximized in most natural gravel pavements. A high degree of © 1998 G.H.McNally
Figure 4.3 Sources of pavement strength and stiffness in natural road gravels. See text for explanation.
grain-to-grain friction and a framework of coarse angular fragments spread and dissipate wheel loads. Maximum density grading and a proportion of clay binder also cause these pavement courses to be relatively impermeable, protecting moisture-sensitive subgrades from downward-percolating water. These pavements are normally unsaturated and can therefore develop high soil suction, or soil tension, due to negative pore pressure. This can be thought of as a form of confinement analogous to vacuum-sealed plastic wrapping, except that in this case the membrane is a very thin film of water tightly held by capillary forces. Its magnitude (which can exceed 1 MPa) is a function of the dryness of the material and the fineness of its micropores; hence maximum strength is achieved in well-graded (but fines-rich) road gravels by heavy compaction and by ‘drying back’ from the optimum moisture content prior to sealing. However, moisture content within a © 1998 G.H.McNally
Table 4.1 Comparison of natural gravel and crushed rock pavement materials
CBR=California bearing ratio.
pavement varies with the climate, seal condition and other factors, so soil suction is looked upon as a bonus and not as part of the design strength. A fuller discussion of the compaction process is given in Chapter 10. The usual surface treatment for natural gravel pavements is a thin sprayed bitumen seal protected by stone chippings (see Chapter 9). The seal generally consists of two coats of bitumen applied several months apart, so that imperfections in the roadbase that progressively become apparent can be patched prior to the final surface dressing. Periodic resealing is desirable with gravel pavements because the bitumen oxidizes and cracks, especially in hot and sunny climates, allowing moisture penetration. To further compensate for the relatively poor quality of these pavement materials, a dry and strong formation is preferred. This provides a hard floor for pavement compaction and prevents loss of suction. Natural gravels are particularly appropriate in low-rainfall and deep-water-table areas, where infiltration through the road shoulders and capillary movement upwards are minimal. Sources of external moisture and some of the methods of controlling them are discussed in Chapter 11. Subgrade strength is improved by compacting in thin layers and by using the best granular material available at the top of the fill. Dry borrow areas in such environments mean that the earthworks materials can be gradually wetted up to, or slightly below, optimum moisture content. © 1998 G.H.McNally
4.3 DURICRUST ROAD GRAVELS The most important group of natural gravels for road-making purposes are the hardened soil materials: ferricrete, calcrete and silcrete, collectively known as duricrusts, pedocretes or pedoderms. These occur as caprocks on flat-topped hills (mesas and buttes), as boulders and cobbles in talus, as cemented sheets along ancient drainage lines (‘valley train’ deposits) and as lag gravels (‘gibbers’) on plains. Typical geomorphic relationships between these deposits and the implications for pavement materials investigations are summarized in Figure 4.4. Their importance lies in a worldwide distribution and because—being themselves the end-products of extreme weathering and redeposition—they occur in terrains where no other hard rock materials are likely to be found. The engineering uses and problems of duricrusts are described in a classic paper by Grant and Aitchison (1970); and by also Gidigasu (1976) on ferricretes, and by Netterberg (1971, 1982) in relation to calcretes. A recent summary of the geotechnical characteristics of ferricretes (laterites) can be found in Charman (1988). • Ferricrete (Figures 4.5 and 4.6) is the sesquioxide-rich (Fe2O 3+Al2O 3) ‘ironstone’ horizon within a laterite profile, or transported gravel derived from this source. It generally consists of boulders and gravelsized concretions within a silty matrix. Varieties include nodular ‘ironstone gravel’ and pisolitic ‘pea gravel’. As a road pavement material, ferricrete compacts to a high density—partly due to the high specific gravity of the haematite concretions—and resists surface rutting when unsealed because of its gravel content. Ferricrete is probably the most extensively used road-building material in the world, but especially in central and west Africa, northern Australia and southern Asia. • Calcrete (Figures 4.7 and 4.8) is calcareous duricrust, which is both more variable and perhaps even more widespread than ferricrete, owing to its relatively rapid accumulation in semi-arid soil profiles. It ranges from a light CaCO3 dusting on soil fissures, through soft nodular (gravelly) horizons, and eventually to dense cemented sheets. Even in small concentrations, lime can impart useful self-cementing properties to sands deficient in clay binder. However, nodular calcretes and weaker (i.e. rippable) sheet calcretes are considered the better unprocessed pavement materials. Areas of calcrete abundance include southern and north Africa, the Middle East and southern Australia. • Silcrete or siliceous duricrust is the least-used of the three main duricrust materials, although it occurs throughout the interior plains of Australia and South Africa. It normally occurs as bouldery hill cappings and talus, or as cobble-sized ‘gibbers’ (desert armour) on the plains, and requires crushing prior to use in road pavements. © 1998 G.H.McNally
Figure 4.4 Duricrust deposits and their geomorphic expression. In Australia silcrete deposits, being oldest, usually occur as caprocks high in the landscape, while ferricretes may occupy intermediate levels. Calcretes are youngest, and tend to be developed along drainage lines and in dunes.
© 1998 G.H.McNally
Figure 4.5 Laterite profile near Casino, New South Wales, showing ferricrete horizon (about 1 m thick) at top and mottled zone beneath. In extracting this material about 0.5 m of topsoil would first be stripped, and the ferricrete ripped, blended and stockpiled in the pit. The pit floor would be located at the top of the mottled zone.
Figure 4.6 Pisolitic ferricrete (‘pea gravel’ or ‘ironstone gravel’) stockpiled for reconstruction of highway pavement near Cloncurry, Queensland. © 1998 G.H.McNally
Figure 4.7 Typical calcrete profile about 2.5 m deep in a gravel pit near Mannum, South Australia. Note the well-cemented hardpan at the top, nodular calcrete beneath and loose powder calcrete at base.
Figure 4.8 Calcrete nodules (10–25 mm diameter) agglomerated into an irregular boulder-sized mass about 1.5 m across, Broken Hill area, New South Wales. (Photo: I.R.Wilson.) © 1998 G.H.McNally
Although originally formed by weathering in situ, many duricrusts have been recemented, reworked and redeposited by alluvial, colluvial and groundwater processes. They tend to be gap-graded (‘armchair graded’, as shown in Figure 4.9) due to the absence of coarse sand, and to break down with working. The particles are porous and hence absorbent because of cavities left after the solution, redeposition and cementation phases. Hence it is believed that fines microporosity, rather than excess clay minerals, causes high liquid limits (LL) and plasticity indices (PI) in these materials. The more indurated layers are unrippable, but paradoxically they are also difficult to blast because of their porosity. Explosive gases tend to vent (depressurize prematurely from blastholes) without fragmenting the rock, creating an airblast nuisance, or to dissipate energy in compressing the underlying soil. Well-cemented sheet and boulder duricrusts are sometimes crushed to produce dense-graded roadbase and aggregate, although the yield of coarse chips may be low and their soundness suspect. Both calcrete and silcrete basecourses present problems of seal debonding—the bitumen can be literally rolled up in some cases. This can be due to the presence either of salt or of incompatibly charged dust particles along the basecourse/seal interface. These materials are also as highly absorbent of bitumen as they are of water, so that up to four applications—two of thinned or ‘cut-back’ bitumen primer followed by two high-viscosity seal coats—may be required to complete the surface dressing. Siliceous duricrusts, both silcrete and chalcedonic calcrete, are potentially reactive with cement paste (see Chapter 8). Despite this, they have occasionally been used as coarse aggregate in low-strength concrete, through lack of any alternative source. In this situation low-alkali cement is specified and close control over the water/cement ratio (the main factor controlling hardened strength) is essential. Ideally the aggregate should be pre-soaked and mixed in a saturated, surface-dry condition, so that water intended for cement hydration is not drawn into the aggregate micropores instead.
4.4 OTHER ROAD GRAVELS A number of other naturally occurring granular soils and weak rock materials are also used for road pavement construction. The geological origins and engineering properties of these diverse materials have never been systematically described, but an idea of their variability can be gained from the grading curves shown in Figure 4.1. The finer end of the range is represented by the prior stream ‘gravel’, which is in fact a sandy loam with a small proportion of granules. The graded macadam is typical of a broken © 1998 G.H.McNally
Figure 4.9 Comparison of typical duricrust gravel gradings, as-ripped and as-compacted in a road pavement. Note that the sand deficiency remains after on-road working, but the proportion of fines increases at the expense of the cobble and gravel fraction.
© 1998 G.H.McNally
rock pavement with only about 10% by weight of sand and silt-clay fines. The grading curves for a duricrust and a dense-graded fine crushed rock basecourse are also shown for comparison. Residual soils Residual soils, mainly those derived from weathering of granite and related quartz-rich lithologies, were once widely used for rural highway pavements in New South Wales. Such soils tend to be well graded below the 2.36 mm sieve size and of low plasticity, but with very small quantities of fine gravel and no coarser particles. A typical road-making residual soil might be developed on top of a deeply weathered coarse granite saprolite, with a high quartz/orthoclase ratio and a low mica content. Highly feldspathic soils may be similarly well graded, but being composed of weaker particles tend to break down during working. As with the duricrusts, contamination even by small quantities of underlying clayey subsoil may make residual soil unsuitable as a basecourse. Alluvium Alluvium varies greatly in grain size but tends to be either too clean (that is, deficient in silt-clay binder) or, conversely, too clay-rich for use as roadbase. Clean sand and gravel are, of course, very suitable for other road-making purposes, such as concrete and sealing aggregates. Sand and gravel may also be blended with gap-graded soils to meet roadbase specifications. In southeastern Australia, abandoned channel deposits (‘prior streams’) of probable Late Pleistocene age contain large resources of continuous graded but silty sand (Figure 4.1), suitable for light-traffic pavement courses. Their high silt content makes them moisture-sensitive and unsuitable above shallow water tables, where they may become saturated due to capillary rise. Older alluvial deposits (Tertiary ‘Deep Leads’) occurring as hill cappings, gully fills or raised river terraces are often adequately graded but weathered, and their cobble and gravel fraction is unsound as a result. This is not necessarily detrimental in a material to be used as unprocessed roadbase, since it facilitates closer packing after clast breakdown, but high plasticity can be a serious drawback. These deposits are often quite deep (5–15 m) but in the past only the leached, low-PI upper portions were worked. Lime stabilization is now commonly employed to reduce plasticity and increase bearing capacity. Alluvial fans Alluvial fans are significant sources of roadbase in some arid and tectonically active areas. They tend to be well graded, with excess fines © 1998 G.H.McNally
carried away in suspension. Cobbles and coarse gravel may be present in quantity, and can be crushed and blended back to improve the overall grading. Many alluvial fans are, however, composed mainly of mudflow debris, and this would generally be too clayey for roadbase. Colluvial deposits Colluvial deposits are sometimes reasonably graded, but with an excess of clay fines and unsound coarse rock fragments, and are therefore rarely suitable for pavement materials. Some ferricrete and silcrete talus can be recemented by younger pedogenic materials (of the same or different composition), but the volume of these deposits tends to be small. Leached slopewash deposits, particularly those derived from granitic soils and fragmented duricrusts, provide minor sources of natural roadbase. Aeolian deposits Aeolian deposits of carbonate sand (aeolianite, calcarenite or dune limestone) can produce useful roadbase, since their calcrete horizons break down during working to produce angular gravel fragments. These improve the grading and hence the compacted density of the sand; facilitate mixing and uniformity of the pavement courses; and resist ravelling on unsealed road surfaces. Coronus or uplifted coralline sand has similar properties to aeolianite, and is the most widely used pavement material in Papua New Guinea and the islands of the western Pacific. Quartz dune sands of the Australian interior are moderately well graded in the medium to fine sand sizes, but lack coarser material except where nodular calcrete occurs in their B-horizon. Aeolian sand-clays of this type are in fact sandy loams with a proportion of binder. These are used as pavement courses in remote areas of Western Australia and western Queensland, but erode rapidly where unsealed. They may also possess weak self-cementing properties because of the presence of mobile ferruginous coatings on sand grains. Volcanic scoria Volcanic scoria and pyroclastic debris have been used as base and sub-base on rural roads in western Victoria and South Australia, although environmental pressure to preserve the more conspicuous scoria cones is limiting further exploitation. The ash is well graded but the particles are porous and weak, and hence suitable only for very lightly trafficked roads. Scoria is a vesicular rock that breaks down under compaction, but is sometimes strong enough for use as lightweight aggregate or as sub-base. The best-quality scoria is used as a skid-resistant aggregate in wearing© 1998 G.H.McNally
course asphalt, and weaker deposits have been blended with volcanic ash and aeolianite to improve their grading. Weak rockfill Weak rockfill, as a macadam-type pavement material, has been used where no better source was available (see also Chapter 12). These stony materials are generally weathered and cleaved—or extremely close-jointed— metamorphic and igneous rocks or indurated shales, obtained by ripping or light blasting. Typically more than 90% of the pit-run material is coarser than 2.36 mm and composed of weak, angular, often platy rock fragments. This material is further broken down on the road by grid or vibrating drum rollers, though care has to be taken to avoid over-rolling (and hence overfilling of void space, since the strength of the pavement in this case depends on mechanical interlock rather than maximum density grading). Sandstones and conglomerates Sandstones and conglomerates, usually in a weathered, leached or otherwise disaggregated state, are used as sources of ripped rock and aggregate in some areas. The end-product is usually a conventional maximum-density compacted roadbase with a proportion of coarse harder rock fragments, rather than an open-graded macadam pavement.
4.5 LOCATION AND SAMPLING Terrain evaluation The location and evaluation of duricrust, residual, alluvial, aeolian and pyroclastic road-making materials depends to a great extent on recognition of the landforms associated with these deposits. Hence image interpretation, or terrain evaluation in its more systematic form, is a much more useful exploration technique for natural gravels than it is for hard rock quarry sites. This is particularly so when major development projects, such as trunk roads and mine sites, are being planned for remote and semiarid areas. In these situations there is generally a close relationship between geology, soils and vegetation, and good-quality airphotos or satellite imagery are available. Land ownership and environmental constraints play a smaller part in the selection of quarry sites and borrow pits than they do in settled areas, so materials searching can be more extensive. Landsat MSS imagery has in the past not lived up to engineering © 1998 G.H.McNally
expectations, owing to poor resolution (80 m wide pixels), lack of spectral contrast between soil units and user-unfriendly processing techniques. The latest interactive programs allow the geologist who does the fieldwork to complete the interpretation on his/her own PC. Promising results are being obtained using Thematic Mapper (TM) imagery with 30 m resolution, and even finer detail is visible on 10 m resolution SPOT images. Airborne remote sensing, using infra-red linescan, thermal imagery and side-looking radar (SLAR), has in the past been used experimentally for locating construction materials over large areas, and is now becoming costeffective for routine applications. The latest systems can be mounted in a light plane and offer pixel resolutions in the range 1–10 m, depending on the swath width required, and up to 20 data channels in the visible and infra-red regions. Airphoto interpretation Airphoto interpretation, nevertheless, remains the basis of terrain evaluation for engineering purposes. It is best performed as a three-stage process, beginning with a preliminary appraisal of available airphotos, maps and the existing geological information in the office. This should highlight possible deposits—or at least landforms likely to be associated with such deposits— while at the same time allowing large non-prospective areas to be discarded. The second stage, the site survey or ‘ground truth’ stage, involves sampling and reconnaissance mapping in the field. The geologist should not attempt to map the entire area (a corridor 5–10 km wide on either side of a proposed road, for example), but should select typical samples of the landscape that coincide with distinctive photographic patterns and are most conveniently located for visiting. Once the geology underlying these patterns is established, the interpretation can be extended throughout the surveyed area in a final compilation stage. Sampling Sampling during broad-scale preliminary investigations of this type is best carried out using mobile excavation plant such as backhoes or truck-mounted augers. With these machines it may be possible to sample and log 10–20 holes per day along 5–20 km of traverse line. Backhoes can excavate to depths of 3–4 m, which is quite adequate for most superficial deposits. They can also penetrate loose nodular (but not bouldery or sheet) duricrusts, and can give a good picture of layering and horizontal variation in material properties. The most useful augers are 0.3–0.6 m diameter disc or short-spiral types, which can quickly penetrate to depths of 5–10 m. Both types can rapidly penetrate slightly cohesive granular soils above the water table, and the more powerful ones can penetrate weak rock. © 1998 G.H.McNally
Before undertaking detailed sampling of naturally occurring construction material deposits, it is necessary to establish (by scout drilling, pilot sampling and index testing) whether the soils present are within or close to specification, and likely to be present in sufficient quantities to justify further investigation. If this is so, the next step is to determine the lateral and vertical variability present within the deposit by grid drilling (30–50 m centres is a typical interval) and systematic sampling. Individual samples should be taken from the principal layers present in each hole, so that the properties of each horizon can be established. Not all samples will be tested, but it is far better to have taken too many than too few! This is also important because, with careful in-pit blending, two substandard soils can be combined to generate a product that meets specification. Conversely, poor mixing— for example, including clay bands or clay floor in the stockpiled product—can degrade a material otherwise just within specification limits. Because many of these natural materials contain a high proportion of coarse particles (weathered rock fragments, duricrust boulders, alluvial cobbles and volcanic bombs), large volumes are required for representative samples. These can be reduced to manageable proportions by removing and weighing oversize particles—those thicker than the pavement layer (say 100 mm)—and carefully quartering the remainder. In some cases the size of the bulk sample may be so large that a backhoe or front-end loader are needed to assist with quartering. Bulldozer trenches (costeans) are another means of exposing gravel faces for logging and bulk sampling.
4.6 TESTING AND EVALUATION Natural roadbase materials are subjected to the same acceptance tests— including particle size distribution (grading), consistency (Atterberg) limits and compacted (Proctor) density—as crushed rock. The main differences lie in the specification limits set and the tolerances permitted. These are determined by climate, expected traffic volume and material availability. Dry climates and low traffic usually permit higher values of plasticity index and liquid limit, in particular, to be accepted. The most important characteristics of many natural pavement materials, to be kept in mind when evaluating their suitability, are as follows: • Both their coarse fraction and their fines should be composed of cemented and porous particles, which will break down when excessively compacted. Hence it is desirable that the laboratory pretreatment of samples be no more severe than that which will be applied on the road. Surprisingly, this is not generally the case—laboratory samples are subjected to intense pounding during Proctor compaction. © 1998 G.H.McNally
• Furthermore, as a consequence of oversize removal during sample pretreatment, laboratory gradings may bear little relation to the material as compacted on the road. In particular, on-road gradings are likely to be much coarser and the proportion of fines less. Conventional test sample preparation methods include removal of +20 mm stones after pounding, oven drying and disaggregation of cemented fines. This not only increases the proportion of particles finer than 425 µm, but also raises the PI of these fines relative to the on-road material. In some halloysitic clay soils, oven drying at 105°C causes irreversible dehydration and granulation. The use of mechanical agitation and dispersants in settling velocity tests to estimate the clay content of the -75 µm fraction likewise tends to overstate this component, since no such deflocculation occurs in the road pavement. Instead, repeated compaction cycles under standard laboratory conditions should be used to simulate, as far as practicable, the coarse particle breakdown due to handling and working on the road.
4.7 UNSEALED PAVEMENT MATERIALS Material characteristics About two-thirds of Australia’s public roads system, as in other developing countries, remains unsealed because of small traffic volumes, generally less than 200 vpd (vehicles per day). These are mostly rural secondary roads, for which the cost of sealing—which means not just the cost of the bitumen and chippings, but also the expense of meeting higher geometrical design standards, using better-quality pavement gravel, and ongoing seal maintenance—cannot yet be justified. Although their pavement materials are more varied than those in sealed roads, it does not follow that these materials are unspecified and untested. Broadly speaking, the characteristics sought in wearing-course materials for unsealed roads, relative to those used in sealed construction, are the following: • Low-cost The material must be low-cost, which in practical terms means that it must be unprocessed and taken from a pit close to the job, even if this means that quality is somewhat compromised. • Wear-resistant Good wear resistance to surface abrasion by tyres, runoff and wind erosion is needed. This dictates a high proportion of gravel, preferably 20–60%, which also improves on-road mixing. Angular and rough-textured, but weak, rock fragments are preferred to rounded river gravels. • Ease of grading Adequate ease of grading and ride quality are © 1998 G.H.McNally
facilitated by a maximum particle size of 26 mm (preferably) or 53 mm, although this is at odds with wear resistance. A related requirement is to minimize tyre wear by avoiding hard and sharp-edged siliceous rock fragments. • Plastic clay binder A proportion of plastic clay binder must be present to resist wear, to increase dry strength and to make the compacted surface as impermeable as possible. However, too much clay will cause the material to soften and become slippery on wetting. Hence it has to be diluted with sand and silt fines, which also fill the voids between the aggregate particles. Too much sand and the road surface will ‘ravel’ or disintegrate under traffic; too much silt and the surface becomes very dusty in dry weather, and sticky when wet. • Deformability Moderate deformability (loss of pavement shape) and lack of shear strength are also tolerable in unsealed gravels. Pavement shape is in any case difficult to maintain, even in good-quality unsealed roadbase, and can be restored by periodic regrading (of the road surface, that is, not of its particle size distribution!). The life of wearing-course material is relatively short, as the name implies, owing to erosion and grader trimming losses, hence it is usual to resheet with a new gravel layer every few years (where a sealed pavement would be designed for about 30 years). This is another reason why sub-specification unsealed materials are acceptable, since anything better would eventually be wasted. Because of these requirements, most of the better-performing unsealed pavement materials have a higher gravel content than those in sealed roads, and this fraction is also coarser. Their fines have somewhat higher liquid limits, plasticity indices and linear shrinkages. The dust ratio (which is defined as the ratio of particles -75 µm to particles -2.36 mm, roughly the fines to sand ratio) should ideally be 0.2–0.6. In many unsealed basecourses, however, the main difference lies in the plasticity allowed rather than in the overall particle size distribution. This is one reason why good unsealed gravels—such as coronus (coral) or ferricrete—can sometimes be later upgraded for sealing by lime stabilization. Staged construction Unsealed roads built to a high geometrical standard are often the first step in staged construction. By this means a cheap pavement on a low embankment is provided initially, where the main requirement is for an all-weather road rather than for high vehicle speeds. When the growth of traffic justifies the expense, perhaps 10–20 years later, a superior-quality base is laid and sealed, with the former unsealed pavement acting as a sub-base. This also © 1998 G.H.McNally
allows the underlying subgrade to compact slowly under traffic and to reach its equilibrium moisture content. Haul road pavement A somewhat different approach is used in heavy-duty haul road pavement design. These roads are unsealed because the maintenance of a ‘blacktop’ would be too expensive, and adequate strength can be obtained from a thick waterbound macadam pavement made up of coarse, angular but free-draining particles (Figure 4.1). The trafficability of these roads under heavy wheel loading at low speeds is maintained by continual watering and grading, and by frequent resheeting. Compaction is provided by the truck wheels themselves and some care is needed in selection of wearing-course stone, since tyre wear can be a significant cost where sharp fragments are abundant. In open-cut coalmines the base is often coarse washery reject, unweathered stone fragments with a top size of about 75 mm and very little -2.56 mm fines, but any source of relatively sound rock will suffice.
4.8 BENEFICIATION Beneficiation or upgrading of in situ marginal roadbase materials is becoming more common than not in Australia, as better-quality deposits of natural gravel diminish and pavement design standards improve. Upgrading can take place in the pit or on the road, and strategies for achieving this, roughly in order of increasing cost, are now outlined: • In-pit blending or on-road mixing (granular stabilization) of substandard soils to create one meeting specification grading limits. • Scalping off oversize in the pit using a grizzly (a robust bar screen) and either discarding or crushing it. • Breaking up oversize on the road, using a grid roller, a cleated vibrating roller or a ‘rockbuster’ (a small tractor-drawn impact crusher). • Single-stage crushing run-of-pit material, or only oversize—sometimes a proportion of the fines is removed as undersize (note that this is only feasible where the soil is very dry and loose). • Stabilization of run-of-pit or processed material using lime and/or cement. Some of these procedures are discussed further in Chapters 5 and 18.
4.9 CASE HISTORY: CALCRETES, SOUTHERN AFRICA The geological occurrence and engineering properties of calcareous duricrusts have been described comprehensively in a series of papers from © 1998 G.H.McNally
South Africa (in particular, Netterberg, 1971, 1982). These deposits are widespread in areas of low rainfall throughout southern Africa, where they are the predominant sources of unprocessed roadbase. They form by cementation and replacement of pre-existing soil particles, the carbonate content ranging from 10% to 90%. It occurs as silty matrix, crack infillings, nodules, concretionary boulders and sheet-like hardpans. There are two basic types: pedogenic and groundwater calcretes. Pedogenic calcretes form by capillary rise and downward infiltration in the unsaturated zone of a soil profile. They are predominantly nodular, variably cemented and often weakly agglomerated into irregular masses, and are widespread in sanddune terrains. Groundwater calcretes develop where lime-bearing phreatic waters discharge and evaporate, usually along ephemeral watercourses. These are limited in areal distribution but more cemented and larger in volume than pedogenic deposits, and are therefore better suited to crushing and screening operations. Compared to ferruginous and siliceous duricrusts, most calcretes are geologically young, sometimes only a few thousand years old, though the older varieties (being more cemented) make the better gravel sources. One consequence of their recent age is their occurrence relatively low in the terrain, in landforms and beneath vegetation that are distinctive on airphotos. Other prospecting aids include probing rods and backhoe pits, since useful deposits tend to be most dense at their top and to be present at depths of 1–2 m. This top crust may be smooth-surfaced and difficult to rip, yet also difficult to blast because of abundant cavities. Conversely, the calcrete may be bouldery and generate oversize that cannot easily be broken down by tracking. Deposits are generally inhomogeneous and shallow, becoming finer and looser with depth; selecting a cutoff depth takes some skill on the part of the bulldozer operator. Particle size distributions for calcrete materials are not especially diagnostic of their properties, since these depend on the degree of in-pit and on-road breakage to which they have been subjected. However, they are almost invariably gap-graded with a deficiency in the coarse sand and fine gravel sizes. Atterberg limits are similarly misleading because of particle microporosity and water absorption; high liquid limits indicate this characteristic rather than clay content. The clay itself may be palygorskite or illite. Perhaps surprisingly, many calcretes respond well to lime stabilization due to their clay or diatom (i.e. silica) content. Natural self-cementation can also increase the strength of some calcretes threefold in laboratory wetting and drying tests. However, a number of problems have been reported with calcrete pavements: • Because of their deviation from maximum-density grading, sensitivity to sample preparation techniques (especially oversize removal and oven drying) and ambiguous Atterberg results, it can be difficult to distinguish © 1998 G.H.McNally
between adequate and inferior-quality materials. Self-cementing characteristics, in particular, are difficult to predict. • Most calcretes contain some clay and salt, and in large amounts these can cause seal debonding. • Their coarse particles are relatively weak, making most unprocessed calcretes unsuitable for even moderately trafficked (say, 500–1000 vpd) trunk roads. Hence the harder calcretes are being increasingly crushed and screened for prepared roadbase and aggregate. This can result in a high proportion of dust and fine sand-sized waste, and very extensive pits requiring rehabilitation. The best crushed calcrete is comparable with other limestone aggregates, and may exhibit high polishing resistance and low flakiness, but a high proportion of particles are usually unsound to some degree. Siliceous calcrete may be subject to alkalisilica reaction, and all calcrete aggregates may present problems in concrete mixes due to their microporosity and clay content. In short, calcrete is a useful source of marginal-quality aggregate and roadbase in remote areas, but deposits require considerable care in selecting, evaluating and working.
REFERENCES AND FURTHER READING Bullen, F. (1990) Materials problems associated with providing a highway infrastructure for remote areas. Proceedings, 15th Australian Road Research Board Conference, 15 (2), 217–31. Carseldine, H.B. and Parkinson, B.D. (1986) Experience with silcrete materials in road construction in northwest Queensland. Proceedings, 13th Australian Road Research Board Conference, 13 (5), 146–61. Charman, J.H. (1988) Laterite in Road Pavements. CIRIA/TRRL Special Report 47. Construction Industry Research and Information Association, and Transport and Road Research Laboratory, London. Cocks, G.C. and Hamory, G. (1988) Road construction using lateritic gravel in Western Australia. Proceedings, 2nd International Conference on Geomechanics in Tropical Soils, Singapore, December, pp. 369–84. Gidigasu, M.D. (1976) Laterite Soil Engineering. Elsevier, Amsterdam. Grant, K. and Aitchison, G.D. (1970) The engineering significance of silcretes and ferricretes in Australia. Engineering Geology, 4, 93–120. Hight, D.W., Toll, D.G. and Grace, H. (1988) Naturally occurring gravels for road construction. Proceedings, 2nd International Conference on Geomechanics in Tropical Soils, Singapore, December, pp. 405–12. Kilvington, D. and Hamory, G. (1986) The performance of natural gravels as basecourse in a sealed pavement. Proceedings, 13th Australian Road Research Board Conference, 13 (5), 86–101. © 1998 G.H.McNally
Lawrance, C.J. and Toole, T. (1984) The Location, Selection and Use of Calcrete for Bituminous Road Construction in Botswana. TRRL, Crowthorne, Berks, LR 1122. Metcalf, J.B. (1991) Use of naturally-occurring but non-standard materials in low-cost road construction. Geotechnical and Geological Engineering, 9, 155–65. Netterberg, F. (1971) Calcrete in Road Construction. National Institute for Road Research, CSIR South Africa, Bulletin 10. Netterberg, F. (1982) Geotechnical properties and behaviour of calcretes in South and South West Africa, in Geotechnical Properties, Behaviour and Performance of Calcareous Soils, eds K.R.Demars and R.C.Chaney, ASTM Special Technical Publication No. 777, pp. 296–309. Netterberg, F. and Paige-Green, P. (1988) Pavement Materials for Low Volume Roads in Southern Africa: A Review . National Institute for Transport and Road Research, CSIR South Africa, Report RR 630. Toll, D.G. (1991) Towards understanding the behaviour of naturallyoccurring road construction materials. Geotechnical and Geological Engineering, 9, 197–217. Weinert, H.H. (1981) The Natural Road Construction Materials of Southern Africa. Academia, Pretoria and Cape Town.
© 1998 G.H.McNally
Blasting and crushing
Rock size reduction in quarries and mines is referred to as comminution and the processes include blasting, crushing and grinding. Blasting produces rock spalls with a maximum size typically 300–800 mm, which can be fed into a medium-sized primary crusher for reduction down to 100–200 mm. This material is then passed on to secondary and tertiary crushers for further size reduction and particle shaping. Typical nominal product sizes are 20 mm, 14 mm, 10 mm and 7 mm. Most comminution techniques used in quarries are scaled-down versions of those developed for overburden removal and mineral processing. One important difference, however, is that quarry stone is generally stronger and tougher than overburden (and many ores), yet it must be blasted finer. On the other hand, the finest quarry product size is about 7 mm, so further comminution by milling and grinding are not usually required. Further information on blasting can be found in Sen (1995) and in manuals published by the explosives manufacturers. The standard reference book on comminution is that by Lowrison (1974), but much useful material can be found in textbooks on mineral processing, such as those by Kelly and Spottiswood (1982) and Wills (1988). Crushing in quarries is addressed specifically by Mellor (1990), and Australian quarrying practice is well summarized in Armstrong and Dutton (1993).
5.1 QUARRY BLASTING AND EXPLOSIVES Elements of blast design The basic elements of blast design can be thought of as the following: • Choice of explosive, its distribution within the blasthole and the measures used to ‘partition’ the ratio of heave (gas pressure) to strain (shattering) energy. • Blasthole geometry, its diameter, depth, angle of inclination, stemming length and backfill depth. © 1998 G.H.McNally
• Blasthole pattern, including spacing within rows, row spacing (burden distance) and delay configuration. All of these parameters are influenced by the geomechanical properties of the rock, but even more so by the distribution of fractures within the in situ rockmass. The main considerations in quarry blasting are to generate minimum oversize and to satisfy environmental restrictions on dust and ground vibration. Good fragmentation with acceptable vibration is achieved by limiting the weight of explosive fired at any instant, and by carefully distributing this charge within blastholes (see Chapter 20). Oversize blocks are not always unwelcome, however, because they may sell at a premium for use as breakwater armourstone. Quarry blastholes tend to be narrow, heavily charged (high powder factor) and closely spaced relative to mine overburden blasts. Quarry blasts are relatively small (Figure 5.1)—a blasting round might fragment 6000 m3 (say 13000 t) of stone with one or two rows of holes. A large coal overburden round, by comparison, might blast 100000 m3 and be 10 rows deep. Many quarries blast only once a week, usually at a predictable time like midday, while mine blasts occur daily. Drilling and blasting costs are less important in quarrying than in mining, since money spent here can reduce downstream processing costs and prevent complaints from neighbours (who also tend to live closer in the case of quarries!). Explosives The main types of explosives used in quarrying are compared in Table 5.1. Traditional nitroglycerine-based high explosives, such as AN gelignite 60, are little used today. The most commonly used explosive, actually a blasting agent since its constituents are non-explosive, is ANFO (a mixture of 94% ammonium nitrate and 6% fuel oil). This is cheap, energetic and safe to transport, store and load. ANFO was the first of the bulk explosives that could be poured straight into blastholes, thus simplifying loading and improving charge-to-rock energy coupling. It is well suited to closely jointed hard rock, since it generates a higher proportion of its energy as gas pressure (heave energy) than any other explosive. It is less satisfactory in strong and massive rocks where more strain energy is required, and may not detonate at all in small-diameter blastholes. However, the main drawback of ANFO is its watersensitivity; it will not initiate in wet holes and may only partially detonate in damp ones. Increased shattering power (brisance) for ANFO was obtained initially by denser packing—note the increased bulk (volumetric) strength of pressureloaded ANFO in Table 5.1—and later by the addition of aluminium dust (hence ALANFO). From the 1960s watergels or ‘slurries’ began to replace © 1998 G.H.McNally
Figure 5.1 Bench blast, Riverview Quarry, Adelaide. Although this is a major quarry producing aggregates from dolomite and quartzite, a typical blast might include only 20 holes. (Photo: M.Drechsler.)
ANFO in wet holes. Watergels are saturated aqueous solutions with gelling agents and ammonium nitrate (AN) prills (spherical grains) in suspension. By varying the ingredients, their strength can be tailored to the rock, though at a cost penalty relative to ANFO. The latest generation of explosives are emulsions of AN-saturated droplets about 1 µm (0.001 mm) in diameter, dispersed in an oil-wax © 1998 G.H.McNally
Table 5.1 Comparison of quarrying explosives
VOD=velocity of detonation. Energy output is the percentage ratio of strain energy to heave energy (s/h); H indicates proportion of each in hard rock, S in soft rock. b
mixture. Emulsions are waterproof, offer the highest brisance of any of the bulk explosives, and hence are well suited to hard rock quarrying. Because of their very rapid reaction rate, indicated by a velocity of detonation (VOD) up to 5000 m/s, their strain energy component is about three times that of ANFO. Like the watergels, emulsion mixtures can be adjusted to suit the rock, and can be pumped into blastholes. Blends of ANFO with emulsion, or ‘heavy ANFO’, may be more economical in some rockmasses.
5.2 BLAST DESIGN Blast pattern design A typical ANFO-loaded quarry blasthole design is illustrated in Figure 5.2. Holes are drilled using tracked rotary-percussion rigs, generally at diameters of 90–150 mm. Blastholes may be vertical or, more commonly these days, inclined at about 70° from the horizontal. Inclined holes are more difficult to drill straight, but result in finer and more uniform fragmentation. After charging, blastholes are stemmed with crushed stone to depths of at least 2 m. Shorter stemming depths can result in flyrock, airblast and cutoffs (breaks in the detonating cord, which isolate later-firing parts of the pattern and prevent their ignition). Long stemming columns, on the other hand, inhibit airblast but may increase ground vibration by over-confining © 1998 G.H.McNally
Figure 5.2 Typical ANFO-loaded blasthole design and explanation of some blasting terms.
explosive energy; they also cause poor fragmentation around the collar of the blasthole. Some of the terms used in blast pattern design are illustrated in Figures 5.2 and 5.3. In quarry blasting the inter-row distance or burden is typically about 3 m, blasthole spacing within rows is 3–5 m and bench height is 10– 15 m. Drilling and blasting costs diminish as these dimensions increase, but so do the risks of generating oversize and excessive ground vibrations. A free face is any plane that can reflect strain energy, which includes bench faces and open joints. Blasthole patterns are most commonly rectangular, with spacing around 1.3 times burden, but may also be square or even oblique. Initiation sequence and delays The blasthole initiation sequence by delayed firing is even more important in quarrying than in mining, since it largely determines the degree of rockmass fracturing and the ground vibration intensity. Delays are slow fuses inserted into detonating circuits; their purpose is to limit © 1998 G.H.McNally
Figure 5.3 Blasthole patterns and initiation sequences. Row-by-row initiation is more common in quarrying, though the ‘V’ pattern offers better fragmentation.
© 1998 G.H.McNally
the weight of explosive firing at any instant. Blasts may therefore be initiated hole-by-hole, row-by-row or in the ‘V’ pattern shown in Figure 5.3, which improves fragmentation by throwing rock towards the centre of the ‘V’ and thereby maximizes block-to-block impacts. Note that the drilling pattern is identical in both blast designs; only the firing sequence changes. Inter-row delays are usually set at 17–35 ms (milliseconds). Longer delays impair fragmentation and cause cutoffs, while shorter delays may cause ‘choking’ (overconfinement) of rear rows, hence backbreak and flyrock. Backbreak is fracturing that extends into the rockmass beyond the rear row, resulting in bench face instability when the broken rock is removed. Short delays are becoming more common as their timing accuracy improves, although previously they could overlap and conspicuously increase ground vibration amplitude. Another innovation with relevance to quarry blasting is the use of non-electric (Nonel) initiation, which, among other virtues, eliminates the high-frequency airblast associated with detonating cord firing on the ground surface.
5.3 FRAGMENTATION MECHANISMS The fragmentation mechanisms produced by blast detonation depend largely on whether the rock is closely jointed or massive. In the first case gas pressure or heave energy is the dominant factor, and most fragments will be bedding- or joint-bounded. Hence the size distribution of the blasted rock fragments will be largely determined by the original jointing intensity (joint area per cubic metre). In massive rock strain wave energy will be more important, and most fractures will result from radial cracking and gas-pressure-driven joint extension. Some additional comminution is likely to be caused by flexure during rockmass dilation and rock-to-rock collisions.
5.4 GEOLOGICAL ASPECTS OF BLAST DESIGN Intact rock properties Most lithological or intact rock properties (Table 5.2) have a greater effect on crushing than on blasting, but tensile strength and elastic modulus are important in both cases, with one proviso. In blasting we are concerned with dynamic properties and the effects of almost instantaneous loading; rock is both stronger and stiffer under these conditions, so even soft rock can behave in a brittle manner. Crushing involves much slower loading, and hence static geomechanical properties, obtained from laboratory tests, are more relevant. © 1998 G.H.McNally
Table 5.2 Geological factors in blast and crusher design
Rockmass properties Conversely, structural or rockmass properties, especially jointing, are much more significant in blasting than they are in crushing. ‘Joint’ is used here in the engineering sense, meaning any structural discontinuity within a rockmass. This includes true (geological) joints but also bedding, foliation, cleavage and flow layering, as well as fractures induced by previous blasts. Joint aperture (width or openness) is important in that slightly open joints (say +1 mm) can act as free faces, confining the strain energy within single joint-bounded blocks. The charged blocks become excessively fragmented, leaving the surrounding ones unbroken (and hence generating oversize). Open joints can also waste blast energy by premature venting of explosive gases, which also causes airblast. Finally, open joints act as ground water conduits, thereby precluding the use of ANFO below the water table. However, closely spaced tight joints greatly improve fragmentation throughout the rockmass. They transmit most of the strain energy (especially if damp), while at the same time providing a network of fractures for gas pressure to act on. The orientation and attitude (dip) of the principal joint set can affect fragmentation and face stability. Blast comminution is improved when the face is aligned parallel to the main joint direction, and stability will be maintained so long as the joint dip is steeper than the face (that is, these joints do not ‘daylight’). Methods of quarry and pit slope stability investigation, and open-pit blast design, are extensively described in Hoek and Bray (1977). Bench slope stability appears to be much less of a problem in quarries than it is in open-cut mines, since the former are almost always shallower and work stronger rock. Some instability can, however, be expected in bedded and dipping deposits, such as some limestones and quartzites. © 1998 G.H.McNally
The effects of groundwater in tight rockmasses may be negligible, or even beneficial (owing to improved coupling across tight joint faces), but in general its presence will require that ANFO be replaced by watergels at about three times the cost. Furthermore, damp fines may choke crushers, accelerate abrasion of crusher plates, clog screens and overload conveyor belting. In some cases, such as cavernous limestones, fractured basalt flows and jointed quartzites, the quarry rock itself may be an aquifer, and its dewatering may be a major operating expense.
5.5 PRIMARY CRUSHING Crusher classification It is generally not possible to comminute blasted rock satisfactorily in one operation, so crushers are described as primary, secondary or tertiary depending on the size of the feed. The principal types are shown in Figures 5.4 to 5.9. Most are available in either primary or secondary versions, but jaws and gyratories are usually primary crushers, while impactors and cones perform secondary duty. The maximum particle size usually processed is about 800mm for primaries and 200 mm for secondaries. One means of classifying crushers is in terms of reduction ratio, the ratio of maximum feed size to maximum product size. Alternatively, this can be defined as the ratio of 80% of entry width (gape) to 80% of exit width (closed side setting). Compression crushers (jaws and gyratories) have maximum reduction ratios of 8:1 to 10:1 but normally operate at about half this, since high ratios result in excessive fines due to interparticle rubbing and generate platy particles through shearing. Impact crushers perform satisfactorily at much higher reduction ratios, in the range 10:1 to 20:1. Most primary crushers have a feeder, which evens out the flow of broken rock and separates (scalps) undersize using an inclined bar screen. Spalls retained on the screen trickle into the primary crusher, while the undersize bypasses this stage and is directed either straight into the secondary crusher, or to waste if it is weathered. This arrangement increases the throughput or capacity of the primary machine and prevents fines packing in its crushing chamber. Coarse oversize is separated at the blast face prior to loading, or fractured by a hydraulicarm rock breaker when it jams in the primary crusher entry slot. Jaw crushers Jaw crushers (Figure 5.4) break rock by slow compression-release cycles between ribbed plates, one fixed and one moving, on opposite sides of a © 1998 G.H.McNally
wedge-shaped chamber. This narrows downwards, so that after blocks are split on the compression stroke the pieces slip further down on the release stroke. At some point they become jammed again and the cycle is repeated, until eventually the fragments fall out of the base of the crusher. Jaw crushers can be classified into those with a single or double toggle action. Double-toggle machines are able to exert larger compressive loadings, and are therefore used for handling the strongest (UCS up to 500 MPa), most blocky (up to 3 m) and most-abrasive feed. However, in most quarrying applications, single-toggle machines perform satisfactorily and are less costly. They are well suited to small to medium-sized operations, including mobile plant, where intermittent production is normal. A number of jaw arrangements involving different pivot points, curved and planar plates are also offered. Jaws are cheaper in both capital and maintenance
Figure 5.4 Single-toggle jaw crusher, schematic. The left side plate (shaded) is fixed, with the right-hand jaw moving in an elliptical path. © 1998 G.H.McNally
Figure 5.5 Gyratory crusher, schematic. The inner cone moves eccentrically, but the outer plate (mantle) is fixed.
© 1998 G.H.McNally
costs than gyratories handling the same feed size, but their production rate is much less. They are economic for up to 500–1000 tph (tonnes per hour), above which gyratories are favoured. Gyratory crushers A gyratory crusher resembles a pestle in a narrow open-base mortar, or two cones, one inverted within the other (Figures 5.5 and 5.6). The inner pestlelike solid cone, known as the head, moves eccentrically around the fixed outer bowl, alternately closing and opening gaps around the lower rim. It functions as a multitude of jaw crushers, and can therefore be much smaller for the same capacity. Gyratory crushers tend to be chosen where high throughput (up to 5000 tph) is required and where a relatively fine and uniformly blasted feedstock is assured, since they are less tolerant of oversize than jaws. They are more compact than jaw crushers of the same capacity and more efficient in terms of energy consumption per unit of output. Because their construction is lighter, they require less elaborate foundations (but more headroom) than jaw crushers and their feeding arrangements are simpler. They are ‘choke fed’, meaning that the machine works best when
Figure 5.6 Mortar-and-pestle arrangement of a gyratory crusher at Prospect quarry, near Sydney, New South Wales. When operating, this would be buried in blasted rock spalls (‘choke feeding’). © 1998 G.H.McNally
buried in rock fragments, as opposed to the ‘trickle feed’ arrangements needed for jaw crushers. Both types of compression crushers turn out a fairly uniformly sized product, though the gyratory output has somewhat more fines. In hard rock the gyratory action is said to produce more cubic chips, although both types tend to generate a proportion of sheared and unsound particles. Product grading curves for both of these compression machines are similar: the particle size range is narrower than from impact crushing, but wider than from a rolls crusher. Rolls crushers A third primary type, the rolls crusher (Figure 5.7), is limited to weaker (UCS less than 100 MPa) and non-abrasive rock, such as limestone and brick shale. The machine may be equipped with single, double or multiple rollers, and these can be fitted with teeth, cleated or ribbed. Double rolls are most common, with one drum axis fixed and the other spring-loaded to accommodate oversize slabs. Rolls crushers are relatively cheap in relation to their high capacity, economical in power consumption, easily transportable and low in profile
Figure 5.7 Double rolls crusher with interlocking teeth. Both rolls rotate towards the centre, but one is fixed and the other sprung to allow oversize blocks to pass through. © 1998 G.H.McNally
when erected (which simplifies feeding). These characteristics make them a good choice for crushing demolition rubble, especially concrete slabs and brickwork, or weak excavated rock for select fill on construction sites. Rolls crushers are particularly suited to clay-rich feed, and to processing plastic and slabby bedded rocks, which would tend to block jaw or gyratory crushers.
5.6 SECONDARY AND TERTIARY CRUSHING Secondary or reduction crushers have two functions in quarrying. They further comminute primary crusher output to marketable sizes, and may at the same time correct particle shape and soundness (that is, make platy particles more cubic and disintegrate porous or microfractured ones). In some materials primary comminution may be unnecessary, since single-stage crushing is possible with large reduction ratio (10:1 or more) impactors. Tertiary crushers are employed to shape flaky aggregates and to increase the percentage of fines generated. They generally are similar in design to secondaries, but have a closer set and hence very small reduction ratios (only about 2:1). A wide variety of machines are used for secondary and tertiary comminution, including scaled-down jaw crushers (granulators) and shorthead gyratories, but the most common are cone and impact crushers. Cones are the most popular secondary machines in Australia, while impact crushers dominate the tertiary market. The main operational problems experienced are as follows: • Capacity mismatches between primary and secondary crushers, the first producing too much or too little product for the efficient operation of the second stage. • Wear in the primary crusher enlarging outlet settings and producing oversized feed for the later stages. • Excessive fines passing through the secondary crushers, causing increased wear and reducing their capacity. Cone crushers Cone crushers are really small gyratories in which the oscillating inner cone and fixed outer cone are roughly parallel, and the inner cone is pivoted from below rather than suspended from above. Cone crushers have large capacities in relation to their small size, and can handle hard and abrasive feed. Compared to impact crushers they tend to produce a narrower range of particle sizes, less fines and more flaky particles. The two crushing surfaces are held together by springs, allowing tough oversize particles to pass through without damaging the machine. © 1998 G.H.McNally
Impact crushers Impact crushers (Figures 5.8 and 5.9) break rock by the action of rapidly rotating hammers or beaters attached to a central shaft, which may be horizontally or vertically mounted. The feed particles cascade into the crushing chamber and shatter on impact with the whirling beaters, or are deflected by them to strike hardened breaker plates lining the chamber. The beaters may be hinged swing hammers or, more commonly, fixed blow bars
Figure 5.8 Impact crusher, schematic. Rock pieces falling from above are struck by fast-moving blow bars or swing hammers, and either shatter immediately or are flung against the armoured lining (breaker plates). © 1998 G.H.McNally
Figure 5.9 Small portable impact crusher being used for comminution of demolition rubble. Note hopper and elevating feeder conveyor, and product stockpile at rear. The right-hand conveyor feeds to a screening unit.
rotating at 250–3000 rpm. Impact crushers are relatively light and cheap for their capacity, and do not require elaborate foundations. Their main disadvantage is the cost of frictional and chipping wear to beaters and breaker plates, and the downtime required for their replacement. In general terms, impact crushers are limited to rock with UCS values below about 150 MPa and granular quartz (‘free silica’) contents below 5– 7%, though some machines can handle stronger feed. The beating action is advantageous with wet and sticky clay-rich river gravels, though clean gravels are too hard and abrasive for this type of comminution. Product particle shape is particularly good, since high-speed impact shatters unsound fragments and tends to generate near-cubic chips and abundant fines. Impact crushers as a group are divided between large single-stage and smaller reduction machines. The larger impact breakers are characterized by very high reduction ratios (up to 40:1, but 10:1 to 20:1 is more usual) and relatively low velocities (250–500 rpm). They can accept large blocks as feed and some impactors offer capacities up to 1500 tph—comparable with primary gyratories in both respects, though not in the quality of rock that can be crushed. Smaller secondary impactors operate at higher rotational speeds (500–2500 rpm) but with finer feedstock (-200 mm) and generate more fines. © 1998 G.H.McNally
Vertical shaft impact (VSI) crushers have no hammers at all, but depend on high-speed collisions between rock fragments (rock-on-rock breakage). A ring of breaker plates is protected from wear by a cushion of fallen stone, against which other particles are thrown horizontally at high speed. These are dedicated tertiary machines with reduction ratios of only 2:1, used for shaping hard but flaky particles with a maximum size of about 40 mm. They are also unlike other impact crushers in producing few fines and being unaffected by abrasive feed. At some sites it is necessary to manufacture fine aggregate (sand) from crushed rock, either because the natural material is insufficient or because it fails to satisfy grading, soundness or roundness requirements. Sand plants for this purpose are in effect quaternary crushers, rod or ball mills that grind -25 mm feed from tertiary machines. Alternatively, fine crushed rock can be recirculated through tertiary cones until sufficient sand is generated (closedcircuit crushing). 5.7 GEOLOGICAL INPUT FOR CRUSHER SPECIFICATION Crushing mechanisms There are four basic ways to crush rock—by compression, impact, attrition and shear (Figure 5.10). Most crushers employ a combination of these mechanisms: • Indirect tensile failure, due to slow compression, predominates in jaw and gyratory crushers where the feed is strong and brittle, as is generally the case with aggregate-quality rock. Tensile breakage tends to produce a small quantity of similarly sized particles with few fines, which is one reason why secondary crushing is required. • Dynamic (impulsive) loading, due to high-speed rock-on-steel or interparticle collision, is the basis of impact crushing. In these conditions even soft rock behaves in a brittle manner, clean tensile fractures can form, and the resulting particles are equidimensional and unstrained. Disintegration of unsound particles adds a proportion of fines and hence the product is well graded. • Attrition, or interparticle rubbing, is a much more important reduction mechanism in milling than it is in crushing. It is associated with particle rounding in choked crushers, but is otherwise insignificant. • Shearing is also a minor crushing mechanism, associated mainly with plastically deforming shales and with the tearing action of toothed rolls crushers. It generates platy, strained particles. The general requirements for aggregate are that the rock chips should be clean, tough, durable and roughly cubical. The requirements for roadbase are similar but less restrictive, since a proportion of fines is not only © 1998 G.H.McNally
Figure 5.10 Crushing mechanisms. See text for explanation.
tolerated but necessary. These specifications can be met by most unweathered and unaltered igneous and metamorphic rocks, and by a few well-cemented sedimentary rocks. Such lithologies typically have uniaxial compressive strength (UCS) values in the range 50–500 MPa, densities around 2.7 t/m3, porosities of less than 1% and elastic moduli around 500 times their UCS. Measures of rock crushability One method of classifying rock suitable for aggregate is in terms of modulus ratio (E/UCS), as shown in Figure 5.11. In this diagram compressive strength is plotted against elastic modulus, and the group of © 1998 G.H.McNally
Figure 5.11 Classificiation of rock materials in terms of modulus ratios (E/UCS), with steel and high-strength concrete for comparison. © 1998 G.H.McNally
aggregate-quality rocks are shown to be stronger and stiffer than the roadbase sources, although there is some overlap. Some very brittle cherts and limestones, with modulus ratios around 1000, are also indicated; these can be blasted and crushed easily, but break down under repeated impacts in road surfacing. In crusher specifications, rock strength is usually quoted in terms of its uniaxial compressive strength (UCS), even though the main breakage mechanism is believed to be indirect tensile failure caused by compressional or impact loading. Tensile strength averages about 7% of UCS, but varies from 2% (for very brittle rock) to 20% (for ductile shales). The usual ruleof-thumb adopted for primary crusher design is to assume that 99% of the feed particles will have a strength less than their mean UCS plus three standard deviations (SD). Given that the SD for UCS values is commonly about 30% of the mean, this can mean designing for twice the average rock strength measured. A more useful measure of rock ‘crushability’ than strength is the work expended in breaking a unit weight of the material, otherwise known as the specific energy of fracture. This is most widely expressed in terms of the Bond work index (BWI), in kilowatt hours per tonne (kWh/t). The procedure for determining BWI, known as the ‘double pendulum’ test, measures the impact energy required to fracture a rock lump struck on opposite sides by swinging hammers. Toughness can be thought of as the rock’s resistance to crack penetration, or simply as the opposite of brittleness. Brittle rocks are easily crushed, even though their surface can be hard, and fail at very low strains (typically less than 0.5%). Tough aggregates require more energy in comminution and considerably reduce crusher capacity, but are necessary for road surfacing, high-strength concrete and railway ballast. Toughness is related to strength and elasticity, so that a toughness index (resilient modulus) equal to UCS2/2E has been defined. One measure of toughness is the area under the stress-strain curve recorded during the UCS test, which is proportional to the strain energy stored in the specimen prior to failure. The other parameter important in crusher selection and design is the rock abrasivity. It is quantified in terms of milligrams of metal wear per kilogram of rock fragments in paddle abrasion (stirring) tests. Abrasivity is a function of compressive strength (the main cause of chipping or impact wear) and granular quartz content (the source of most frictional wear on crusher plates, roller teeth and gyratory mantles). These two types of wear require different countermeasures. Impact wear or chipping resistance dictates hard-surfaced but brittle tungsten alloys, while abrasive wear is best minimized by the use of tough, work-hardening manganese steel components. The influence of abrasive minerals—primarily granular quartz, but including all framework silicates—is most apparent when
© 1998 G.H.McNally
comparing wear rates between limestone crushers (low) and those handling quartzose rocks (high). A number of other geological factors influence crusher design, but are less easily quantified. These include: maximum expected particle size and shape (estimated from joint and bedding spacing); proportion of clay fines liberated during comminution or present in the feed material; moisture content of the feed; and whether or not hard inclusions (such as siderite nodules) are present within the rockmass.
REFERENCES AND FURTHER READING Armstrong, A.T. and Dutton, A.H. (1993) Handbook on Quarrying, 5th edn. South Australia Department of Mines and Energy, Adelaide. Ball, M.J. (1988) A review of blast design considerations in quarrying and opencast mining, Parts I and II. Quarry Management, June, pp. 35–9, and July, pp. 23–7. Ball, M.J. (1990) Emulsion explosives. Mine and Quarry, June, pp. 14–16. Dalgleish, I. (1989) Cost-effective drilling and blasting. Quarry Management, January, pp. 19–27. Hagan, T. (1980) Effects of some structural properties of rock on the design and results of blasting. Proceedings, 3rd Australian-New Zealand Geomechanics Conference, Wellington, NZ. Hoek, E. and Bray, J.W. (1977) Rock Slope Engineering, 2nd edn. Institution of Mining and Metallurgy, London. Kelly, E.G. and Spottiswood, D.J. (1982) Introduction to Mineral Processing. John Wiley, New York. Lowrison, G.C. (1974) Crushing and Grinding. Butterworths, London. McKenzie, C. (1993) Quarry blast diagnosis—How can it help? Quarry Management, July, pp. 17–23. Mellor, S.H. (1990) An Introduction to Crushing and Screening. Institute of Quarrying, UK. Rorke, A.J. (1988) A scientific approach to blast design—the influence of rock characteristics. Quarry Management, October, pp. 33–43. Sen, G.C. (1995) Blasting Technology. University of New South Wales Press, Sydney. Wang, H., Latham, J.P. and Poole, A.B. (1991) Prediction of block size distribution for quarrying. Quarterly Journal of Engineering Geology, 24, 91–9. Wills, B.A. (1988) Mineral Processing Technology, 4th edn. Pergamon, Oxford. Wylde, L.J. (ed.) (1978) Workshop on Aggregate and Road Base Production with Mobile Equipment. Australian Road Research Board Report ARR 98.
© 1998 G.H.McNally
Sizing and processing
The downstream treatment of crusher products includes separation into size fractions, cleaning and blending to meet differing specifications. In this chapter emphasis is placed on processing of alluvial sand and gravel, but the screening requirements for crushed hard rock are similar. Gravel differs from crushed stone chiefly in having smoother and more rounded particle faces, and in being derived from harder and more durable rock types. Sand and gravel production processes can be grouped into extraction (digging, loading and transporting), preparation (clay matrix disaggregation, washing, scrubbing and cobble crushing), sizing (gravel screening and sand classification) and beneficiation (removal of deleterious particles, desliming and dewatering). The present tendency is towards more elaborate plants, with more diverse products obtained from less-promising feedstocks. Other recent developments are the use of friable, weakly cemented sandstone and conglomerate as sources, and the wider use of dredged marine sands. Sand and gravel processing are well covered in the British technical literature, reflecting a former dependence (which is declining) on fluvioglacial outwash deposits rather than hard rock quarrying for aggregates. Three recent and comprehensive references are those by Mellor (1990), Littler (1990) and Smith and Collis (1993). An older, but still relevant, summary of aggregate processing techniques based on American practice is that by Rockwood (1948).
6.1 EXTRACTION The first consideration in selecting mining equipment for alluvial pits is whether they are to be worked wet or dry, i.e. above or below the water table. In most cases it is not economic to dewater the excavation, and hence different types of excavators must be used in dry and wet situations. Dry pits Excavation in dry pits is generally carried out using conventional earthmoving plant such as bulldozers, scrapers, front-end loaders (FELs) and © 1998 G.H.McNally
trucks. Face shovels and hydraulic excavators, smaller versions of the overburden removal equipment at opencast mines, are used in some alluvial quarries. Cemented or densely packed gravels, particularly those with a stiff clay matrix, can be loosened by bulldozer ripping or—much less commonly—by blasting. The main geotechnical problems in dry pits are face collapse due to oversteepening in gravels and piping in sands, and the presence of occasional large boulders and of layers cemented by ferricrete, calcrete or silcrete. Selective working is much more feasible in dry pits than in wet ones. Wet pits In wet pits sand is generally mined by suction-cutter dredging, using a barge-mounted pump (Figure 6.1). Usually the pond floor is simply agitated to cause the sand to go into suspension, but where the material is bound by clay matrix a more vigorous action is required and this is provided by renewable knives or water jets mounted on the cutter head. The sand slurry, typically 10–20% solids by weight, is pumped through a floating pipeline to shore for processing and stockpiling. The pumps used are centrifugal (impeller) types for the most part, but jet pumps (operating on the siphon principle) and air-lift (reverse-circulation) pumps are used in special circumstances. Centrifugal pumps can draw sand from depths down to about 25 m, while jet and air-lift pumps actually improve in efficiency with depth. Gravel extraction underwater is more difficult, with correspondingly lower productivity. Fine gravel dredging can be carried out by suction-cutter barges equipped with powerful pumps, but operational penalties include increased impeller and pipeline wear relative to sand. Much more power is consumed because of the higher fluid velocities required to keep the gravel in suspension, and because a greater volume of water has to be moved for a given amount of solids. Small draglines are generally preferred for gravel extraction in wet pits, despite their working depth limitation (5–10 m) and inability to dig tough clayey materials. For coarser or more compact gravels, a variety of bucketwheel and ladder dredges, floating grabs and clamshells are used. The geotechnical information needed for assessing whether a material can be economically dredged or not includes the following: • Particle size distribution, with particular emphasis on the percentage of clay fines and of oversize cobbles. Both size extremes can easily be underestimated from drilling samples. The quartz content and angularity of the sand fraction should also be noted, since coarse ‘sharp’ sand is especially abrasive in pumps and pipes. • Consistency (stiffness) of the matrix, its silt/clay ratio and its dispersivity. This is important for estimating cutter resistance, washing characteristics, © 1998 G.H.McNally
Figure 6.1 Suction-cutter barge working an offstream mineral sands deposit, Tomago, New South Wales. Note the lifting frame for manoeuvring the submerged suction pipe, the floating pipeline and the sand delta created by discharge from the treatment plant.
settling time in tailings ponds, and turbidity if released into downstream river waters. • Obstructions such as cemented or densely packed gravel bands, tree trunks, boulders and bedrock pinnacles; and the presence of deleterious layers such as clay lenses or peat bodies. • Aquifer characteristics of the alluvium (such as static water level, transmissivity, storage coefficient and water quality) if pool lowering is planned.
6.2 WASHING, SCRUBBING AND CRUSHING Alluvial sands and gravels are prepared for size separation by oversize removal and fines reduction, in other words ‘topping and tailing’ the grading curve. More consolidated materials require lump breaking, matrix disaggregation and scrubbing. Washing Washing, as the term is used here, means stripping off relatively small quantities of silt weakly adhering to gravel-sized particles. The quantity of water and the degree of agitation needed are relatively small. At its simplest, © 1998 G.H.McNally
washing is performed by water jets directed onto the material as it passes across a vibrating deck or through a rotating cylindrical screen. The water sprays not only clean the aggregate, but also increase the screen capacity and reduce its rate of wear. Scrubbing Scrubbing is a more energetic process, required when a gravel deposit is so fines-rich that it must be broken down by agitation and thoroughly flushed. These fines are not only more abundant, they are also more clay-rich, creating a considerable disposal problem. As a result, scrubbing is more expensive than washing and would only be used when less-clayey deposits were unavailable. In mechanical terms the main distinction between scrubbing and washing lies in the energy involved. Drum washers operate at about half the rotational speed of drum scrubbers, but are otherwise similar in design. They are inclined revolving steel cylinders lined with projecting shelves to lift, turn and drop clayey gravel in a continuous water shower. The disaggregating action is due to stone-on-stone impact, complemented by jostling of particles immersed in the lower half of the drum. The operating principles of drum washers and scrubbers are illustrated in Figure 6.2. In another type of scrubber, known as a logwasher, the agitation is performed by rotating paddles in a sloping trough similar to a heavy-duty spiral classifier (Figure 6.3). The paddles are attached to two thick, parallel, contra-rotating axles or ‘logs’. Logwashers are well suited to disaggregating dense sands and weak sandstones, and helical screws can be substituted for the logs. Crushing Crushing is considerably less significant in gravel pits than it is in hard rock quarries, since oversize here usually means coarser than about 100 mm and may constitute only 5–10% of the material. In some pits these cobbles are simply discarded, but they may also be sold as landscaping or beaching stone. The usual arrangement is a small single-stage gyratory or cone crusher reducing from 100 mm down to 20 mm. Impact crushers, though cheaper, are not widely used because of the severe wear caused by hard siliceous cobbles.
6.3 COARSE AGGREGATE SCREENING Purpose of screening Screening provides the means by which run-of-crusher materials down to a size of about 3 mm are separated into saleable products. In addition to this © 1998 G.H.McNally
Figure 6.2 Drum scrubber and coarse-aperture cylindrical screen (trommel), mainly used for disaggregating and cleaning clayey gravels.
© 1998 G.H.McNally
Figure 6.3 Spiral sand classifier, schematic. The sand slurry is agitated by the helical screw, which also elevates and drains the coarse sand product. Note the different solids contents of the feed, product and waste (overflow).
© 1998 G.H.McNally
primary sizing task, screens are used for scalping oversize, waste removal and dewatering. • Scalping of blasted rock is carried out over bar screens in order to separate coarse spalls, which will be passed through the primary crusher, from undersize, which can be routed straight into the secondaries. The bar spacing (100–200 mm) equals the exit width of the primary, thereby effectively increasing its capacity, since only a third or so of the blasted rock need pass through. Scalping also reduces the risk of blockage due to fines packing, and may improve product shape. • Waste removal by screening usually means the separation of topsoil and weathered rock as undersize. Sounder spalls are then passed on for primary and secondary crushing (this is sometimes referred to as prescreening). Oversize trash such as timber, reinforcing bars and clay balls may also be skimmed off in this way. • Dewatering of sand (clean gravels have negligible moisture adhesion) may be carried out over fine vibrating screens, which reduce the moisture content from over 20% to less than 10%. Since sand is sold by weight, this is still a considerable proportion, and further moisture reduction by cycloning or air drying is often required to avoid contract penalties, particularly where long road hauls to markets are involved. Nonetheless, sand drying below about 5% moisture content is usually impracticable. A wide variety of screens are used in aggregate processing, but the most common type is the vibrating multi-deck set (Figure 6.4). The vibratory motion is induced mechanically, by electromagnetic induction or by resonance. Both frequency (10–50 Hz) and amplitude can be varied. Deck inclination is generally in the range 12–20°, but can alter along the screen length. Decks usually consist of two to four screens, typically 40 mm down to 3 mm aperture. The screens themselves may be of round, square, hexagonal or slotted punched steel plate; woven wire or welded steel rods; and hard rubber or polyurethane mesh. The latter materials are rapidly gaining in market share, despite higher cost, owing to their low noise output and—surprisingly— excellent wear resistance. Particles are sized according to their intermediate dimension, since the long axis can align itself perpendicular to the screen opening. The vibratory motion and inclination of the screen causes the crushed stone to segregate and stratify, with finer particles sinking to the bottom and either passing through the holes or gradually migrating down the screen. Screen performance, meaning throughput rate plus completeness of size separation, is affected both by mechanical factors and by the characteristics of the feed material. © 1998 G.H.McNally
Figure 6.4 Screen decks and product bins in a limestone quarry, Kuala Lumpur. Normally these are hidden behind cladding to prevent dust and noise escaping. The two multi-deck vibrating screens enable six products to be generated.
Screen capacity Screen capacity, or rate of throughput, is directly proportional to the hole width (about 10% larger than the nominal product diameter), which means that coarser screens have the greater capacity. Other factors affecting capacity include the following: • Percentage of open area on the screen (the ratio of aperture space to total screen area). This is proportional to aperture width, but is also dependent on the screen material. Punched plate screen, for example, has less open area for the same aperture than welded mesh. • Screen width (width of the deck, not aperture of mesh), with wider screens having greater capacity. • Screen inclination, which for most screens has an optimum around 15°. Below this, the screen’s capacity is reduced; steeper, and feed material moves too quickly down the screen and undersize is retained. Furthermore, capacity also varies with the position on the screen, reaching a peak about one-third along its length, as shown in Figure 6.5. By this point about 75% of the undersize has passed through the screen, and the remaining length merely improves the precision of the size separation or ‘cut’. In other words, capacity is largely unaffected by screen length beyond this critical distance, but efficiency is improved; © 1998 G.H.McNally
Figure 6.5 Single-deck vibratory screening, illustrating the difference between screen capacity (rate of throughput) and efficiency (degree of size separation). Note, in the lower diagram, how screen capacity increases with aperture.
© 1998 G.H.McNally
long vibrating screens present more opportunities for undersize particles to slip through. Screen efficiency Screen efficiency is a measure of how complete size separation is achieved between oversize (particles retained) and undersize (material passing) for a given screen. Coarse particles are most efficiently sorted by low-frequency, high-amplitude vibrations, while passage of finer sizes is facilitated by high frequencies and short strokes. Screen efficiency must generally be traded off against capacity, as it is uneconomic to allow the low feed-rate and long screen residence time necessary for complete size separation. The nature of the feed material is probably the most important factor determining screen performance. Screen efficiency will be reduced by the following factors: • A high proportion of particles close to the nominal aperture size (say 70– 110% of its width), which tend to jam in the slots and reduce capacity. This is known as pegging, and prismatic fragments (‘carrots’) are particularly prone to jam in this way. Furthermore, misshapen fragments adversely affect grading, since flaky particles tend to be retained one deck higher than their volume justifies, while prismatic particles slip through their nominal aperture size. In other words, flaky aggregates appear to be coarser, while prismatic aggregates appear to be finer than their true sizing. • Accumulations of damp clay and silt grains around mesh openings, which eventually block off or blind the screen. These fines will also adhere to the larger particles, producing a dirty aggregate. Where very fine sizes are prevalent in the feed, it should be screened either perfectly dry or wet. Wet screening is technically superior, but incurs drying costs plus clean water supply and mud disposal problems. Apart from the vibratory multi-deck inclined screens described above, two other types are important. Grizzlies are robust inclined frames with widely spaced parallel bars, used for scalping. Rotating cylindrical screens called trommels (see Figure 6.2) are used for small-scale wet screening of gravels. By varying the screen aperture along the length of the drum, several sizes can be delivered in one operation, with oversize tumbling off the lower end.
6.4 FINE AGGREGATE CLASSIFICATION Separation via classification As screen capacity and efficiency diminish in the fine aggregate sizes, and mesh wear accelerates, screening is replaced by size separation through © 1998 G.H.McNally
particle settling velocity, or classification. This is based on Stokes’ law, whereby settling velocity is proportional to volume for spherical particles of the same specific gravity (SG)—generally assumed to be quartz, SG 2.65. Complications arise because non-spherical, and particularly rough-textured and flaky, particles settle more slowly. Their movement is further retarded by the presence of suspended clay platelets in the water, making it effectively a dense medium. Hindered settling of this kind, rather than the free settling assumed by Stokes’ law, is therefore the normal situation with sand slurries. Furthermore, clay platelets attach themselves to the early-sinking coarse sand particles, resulting in a dirty product. This can be counteracted by gentle upwelling or elutriating currents, which keep the clay in suspension but allow clean sand to fall to the base of the settling column. Sizing by classification is cruder than the cut obtained by screening; separation efficiencies are only 30–80%, compared with 90–95% when screening coarse aggregates. Fortunately, only two products are normally obtained from classifiers: a relatively clean, coarse sand for concrete mixes (the high-value product), and a silty fine sand suitable for mortar or filling and other low-value applications. Much greater sizing precision is required for glass and foundry sands. Classifiers come in even more varied designs than screens, but have two features in common—some means of agitating a sand slurry, and of separating a suspended overflow of fine sand and silt from a settling underflow or bottom load of coarser grains. Usually these are the only products, but several size fractions in the range 60 µm-2 mm can be obtained where the devices are arranged in series, such that the overflow from the first classifier becomes the feed for the second and so on. Hydraulic classifiers Hydraulic classifiers include fluidized-bed classifiers, elutriators and classification tanks. Fluidized-bed classifiers (hydrosizers) make use of hindered settlement, by which upward-flowing water in a sorting column opposes particles sinking under gravity (Figure 6.6). The upward velocity is adjusted until only sand coarser than a certain diameter will settle, with the rest being carried away in the overflow. The accumulated coarse sand is periodically drawn out at the conical or pyramidal base. Possibly the most common type of hydraulic classifier is the elutriator (Figure 6.7). This also depends on hindered settlement, but has no moving parts and no introduced clean water. Instead, the descending sand slurry is deflected upwards such that it splits into two streams, a coarser underflow that is drawn off at the base of the vessel and a fine overflow that spills over at the top. Sand can also be sized by horizontal fractionation in a classification tank (Figure 6.8). © 1998 G.H.McNally
Figure 6.6 The principle of hindered settlement, as demonstrated in a fluidized-bed classifier. The ‘teeter zone’ is where fine particles are prevented from sinking further under gravity by upwelling water currents.
Here the sand slurry enters a long, narrow trough with some velocity and particles follow the current in a ballistic trajectory, with the coarsest grains settling at the feed end and the finest close to the muddy water discharge lip. A series of spigots, typically 8–10 along the base, allow closely graded fractions to be drawn off; these may subsequently be reblended if the specification demands. © 1998 G.H.McNally
Figure 6.7 Hydraulic classification by vertical separation in an elutriator. In this case the water currents are provided by the downward motion of the slurry and directed by baffles in the cylindrical vessel.
Mechanical classifiers Mechanical classifiers work on the principle of free settling in a box-like tank. Sand slurry is poured into a pool at the lower end of the trough and the coarsest fraction quickly settles. Coarse sand is removed from the tank by lifting, pushing or scraping it up an inclined trough, while muddy water is discharged over a weir at the opposite end. The most common type of mechanical classifier uses a helical spiral to agitate and lift the coarse product (see Figure 6.3), and the upward movement allows it to be partially dewatered and deslimed. Figure 6.9 shows a small mechanical classification plant. © 1998 G.H.McNally
Figure 6.8 Horizontal size separation in a classification tank. Here a variety of sand products can be drawn off at different points along the length of a narrow, deep, ‘V’section trough.
Figure 6.9 Portable sand classification plant, Glenlee, New South Wales. Coarse lumps are shed on the bar screen (at right) and finer clay balls by the vibrating screen (top left). The dry scalped feed is then dropped into a long, narrow, water-filled trough, where it is agitated by a helical screw. Clean coarse sand is lifted out of the trough by the bucketwheel and the fine sand residue is drained away. © 1998 G.H.McNally
6.5 DEWATERING, DESLIMING AND BENEFICIATION Dewatering Dewatering is necessary to improve the saleability of washed sand and to allow washwater to be recirculated. Classification, washing and scrubbing all generate heavy suspensions of clay- and silt-sized grains (1– 60 µm) in the circulating water. These must be precipitated before the water can be recirculated within the washing plant or discharged into rivers. Hydrocyclones (Figure 6.10) are widely used for dewatering because they have no moving parts, and hence are simple to operate and cheap to build. Their main shortcoming is that internal scouring by sharp sand limits their working life. Waste water from classifiers is introduced under pressure into the conical hydrocyclone chamber, where its centrifugal movement creates a vortex in the centre. Heavier grains are forced outwards and downwards towards the apex of the cone, while the suspended fines are drawn upwards and out of the chamber. Hydrocyclones can be used for sizing as well as for dewatering, but since the former depends on fluid velocity—and this is fairly
Figure 6.10 Dewatering hydrocyclone (conical object at the top of the tower), Calga, New South Wales. The lower (high pressure) of the inclined twin pipes carries the feed slurry and the upper pipe drains off silt-laden water to tailings dams. Two product stockpiles are visible. © 1998 G.H.McNally
unpredictable in vortices—the grain size of the underflow product tends to be inconsistent. Although hydrocyclones are less efficient than hydraulic classifiers in fractionating within the sand size (but superior to mechanical classifiers), they are very effective in removing silt and clay in the muddy overflow. Desliming The process just described is known, rather inelegantly, as desliming. The muddy water is discharged into tailings dams, which may be either old pits or shallow lagoons constructed for the purpose. The settling time for silt is only a few hours, but finer clay may require weeks or months. The simplest solution is to decant the upper water as soon as it clears, then allow the rest to evaporate. This can require large areas of level land and a dry climate, and in any case wastes water. Drying can be accelerated by scooping up and turning over the tailings once the surface water has drained off or evaporated. Relatively coarse non-cycloned tailings can sometimes be sold after drying as bricklaying sand, or may be reserved for pit restoration. Where land is scarce or the climate too wet for evaporation, finer clay suspensions may have to be chemically flocculated in thickening tanks. These products have been experimentally used as brick-making and ceramic clays. However, it has been found that tailings pond deposits are inhomogeneous and may have only 30–40% solids content, despite a firmlooking and dry surface crust, even after years in place. Further dewatering, possibly by electro-osmosis or filter drainage, is necessary before the tailings can be put to commercial use. Beneficiation Low-grade sand and gravels can be upgraded, or beneficiated, by removing deleterious matter using gravity separation techniques. These are generally of low specific gravity relative to quality aggregates, which are mostly SG 2.65–2.70. They include wood fragments, shells, coal chips, lignite and weak or unsound rock (SG 2.00–2.35) such as chalk, porous sandstone, pumice and shale. Beneficiation techniques have not been much used by the sand and gravel industry up to the present, but could become more common in the future as prime deposits are further depleted. Their main potential appears to lie in removing shell fragments from marine sands, unsound particles from crusher grit, and clay from ground limestone. Like much of the comminution and sizing technology used in quarrying, beneficiation procedures have been adapted and scaled down from those used in extractive metallurgy. The two principal methods of gravity separation are heavy media separation and jigging. © 1998 G.H.McNally
REFERENCES AND FURTHER READING Kelly, E.G. and Spottiswood, D.J. (1982) Introduction to Mineral Processing, Chs 9 and 10. John Wiley, New York. Littler, A. (1990) Sand and Gravel Production, Chs 1–3. Institute of Quarrying, UK. Mellor, S.H. (1990) An Introduction to Crushing and Screening, Ch. 2. Institute of Quarrying, UK. Raspass, F.W. (1980) Developments in fine aggregate processing. Quarry Management and Products, 7 (August), 217–28. Rockwood, N.C. (1948) Production and manufacture of fine and coarse aggregates, in ASTM Symposium on Mineral Aggregates, Detroit, June. ASTM Special Technical Publication No. 83 , pp. 88–116. Sand and Gravel Association of Great Britain (SAGA) (1967) Pit and Quarry Textbook. MacDonald, London. Smith, M.R. and Collis, L. (1993) Aggregates: Sand, Gravel and Crushed Rock Aggregates for Construction Purposes, 2nd edn, Chs 4 and 5. Geological Society of London, Engineering Group Special Publication No. 9. Trahair, J.W. (1981) Sand extraction and processing in South Australia. Quarry Management and Products, 8 (September), 603–13. Wills, B.A. (1988) Mineral Processing Technology, 4th edn. Pergamon, Oxford.
© 1998 G.H.McNally
Aggregate and roadbase testing This chapter discusses the methods of testing and specification applied to crushed rock aggregates, including roadbase. It is worth emphasizing that not all end-uses require the same toughness, durability and wear resistance. The most demanding applications are as road surfacing aggregate and railway ballast; somewhat lesser-quality stone is acceptable for most concrete mixes, lower-course asphalt and unbound basecourse. Relatively poor aggregate may be adequate for road subbase, backfill concrete and sub-ballast courses. In this book ‘aggregate’ refers to any crushed rock product, plus some naturally fragmented materials such as river gravel and sand. Coarse aggregate is that which is larger than about 5 mm, and fine aggregate comprises particles from 5mm down to 75 µm (0.075 mm). Particles finer than 75 µm are referred to as filler, binder or dust. Roadbase, as the term is used here, is any unbound pavement material; it can be either a natural granular mixture (see Chapter 4) or processed fine crushed rock. The better sort of roadbase is known as basecourse or simply as base, and the lesserquality one (lower course) is sub-base. The purpose of aggregate testing, as with all engineering materials, is, first, to provide a basis for comparison with satisfactory or failed materials used in the past. In practice the highest recommendation that can be given to a quarry product is that it has consistently performed well over a long period. Specification limits, especially for roadbase, are set up with these successful materials in mind rather than from any theoretical considerations. The other main purpose of testing is to provide a basis for accepting or rejecting a material, or in other words to ensure compliance with a specification. The tests prescribed for compliance vary from country to country, state to state, and even between construction organizations—but generally involve at least: • Particle size distribution and shape • Crushing resistance • Durability (susceptibility to in-service weathering) © 1998 G.H.McNally
More specialized tests to determine such things as chemical reactivity, skid resistance and bitumen adhesion are sometimes also required. The tests stipulated, and the limits imposed, vary somewhat because of local practice and material availability. The desirable characteristics of an aggregate testing procedure might therefore be the following: • It is widely used and accepted as a valid test, and carried out under more or less standard conditions with similar equipment. • It is a reasonable simulation of in-service conditions (for example, accelerated weathering by wetting and drying cycles). • The procedures give repeatable results (that is, the same operator can achieve nearly the same result each time on identical samples), and these are reproducible (meaning that a different operator in a different laboratory can produce a similar result). • The test is economical to perform (that is, it can be performed by an operator of average skill, using simple apparatus and easily obtained samples). In this chapter the aim is to compare aggregate tests grouped into broad procedural categories (Table 7.1 gives a listing), emphasizing their applications and shortcomings. To describe these tests in detail would be tedious and detract from the main purpose, and in any case is best done in the relevant national standards. These include those of the British Standards Institution (BSI), the American Society for Testing and Materials (ASTM) and the Standards Association of Australia (SAA). Note that these are really suggested methods for good practice rather than true standards, and that it is quite common for major users of rock products— such as state highways departments—to set their own test procedures and specification limits. Good summaries of the most common test procedures and their limitations are given in Lay (1990) and Smith and Collis (1993). 7.1 AGGREGATE SAMPLING Sampling categories Aggregate sampling is nowadays much involved with statistical analysis, but the remarks here will be confined to the practicalities of sample-taking. Interested readers are referred to the chapter by Harris and Sym in Pike (1990) for a discussion on the application of statistical methods to the sampling and testing of aggregates. Aggregate samples can be thought of as falling into three broad categories: • Continuous samples such as rock spalls or drillcore are taken across the full width or depth of a deposit, usually during the exploration stage. Core drilling at the largest possible diameter (generally HQ, 61 mm, in © 1998 G.H.McNally
Table 7.1 Principal aggregate tests
© 1998 G.H.McNally
Australia) is used to recover the maximum weight of sample per metre intersected. Sometimes drillholes are duplicated to obtain sufficient material for a variety of tests, since two adjacent slim holes are cheaper than one large-diameter hole. • Type samples are meant to represent the full range of variability within a product size fraction, or to represent a batch being supplied for a major contract. To encompass this variability, samples have to be very large, say 100–400 kg, and must be reduced by quartering at the sampling site. This should produce manageable, but still representative, quantities of sample—generally 50–100 kg, the weight increasing with nominal particle diameter. • Typical samples are much smaller and less rigorously collected, but more common. They are intended to demonstrate the material properties within a particular bed, layer, rock type or stockpile in the quarry. Their reliability is very much dependent on the expertise of the sampler and the geological complexity of the deposit. Sampling from stockpiles Sampling from stockpiles requires particular care because, although the procedures are straightforward, the results may be used to penalize a contractor or even to reject aggregate batches outright. Since the contractor will already have processed the material and probably delivered it on site, he may well dispute the sampling method or the test procedures. For a start, therefore, stockpiles need to be laid out systematically for sampling and volume measurement. They are typically long parallel ridges of trapezoidal cross-section, about 100–200 m long by 3–4 m high, as illustrated in Figure 7.1. Sample increments are taken at the base, midslope and top, and at regular intervals along the length of the stockpile, as shown in Figure 7.1. Conical stockpiles should be sampled in a spiral fashion, allowing for segregation whereby the coarser particles tend to roll to the base of the pile. Sample increments should also be taken at least 200 mm below the surface, since this is where fines washed downwards by rain accumulate and where the moisture content is representative of the bulk of the stockpile (Figure 7.2). In sand stockpiles the moisture content at this depth may be 5–10% higher than at the surface, a significant difference when calculating water/cement ratios for concrete mixes.
7.2 INTACT ROCK PROPERTIES The geomechanical properties of intact parent rock are less important in aggregate evaluation than might at first be supposed. This is because aggregate is a particulate material, so its behaviour as a mass is more © 1998 G.H.McNally
Figure 7.1 Typical aggregate stockpile and steps required to obtain a representative 50 kg specimen.
Figure 7.2 Problems of segregation, inhomogeneous moisture and fines distribution in aggregate stockpiles.
relevant than the properties of individual fragments. Nonetheless, rock mechanics index tests are useful at the exploration stage because they provide a good basis for comparison between proposed quarry sites. They are also well suited to small drillcore samples, whereas standard aggregate tests require larger quantities of rock. Intact strength The intact strength of aggregate source rock is conventionally measured by the uniaxial compressive strength (UCS) test, performed on © 1998 G.H.McNally
cylindrical samples about 50 mm in diameter by 120 mm long. This is called the ‘crushing strength’ in some of the literature, but should not be confused with the aggregate crushing value (ACV), a test carried out on stone chips. In general, rock with UCS values less than 50 MPa is useless as aggregate and may be suitable only as low-grade roadbase. Values of 50–100 MPa indicate more indurated sedimentary rock or weathered igneous lithologies; it may be suitable for crushed roadbase or aggregate in low-strength concrete. UCS values of 100–200 MPa include most sources of good-quality crushed roadbase and concrete aggregate, but even higher values are desirable for very-high-strength concrete and bestquality ballast. Extremely strong rocks (above 200 MPa) are usually difficult to crush, generating few fines and resulting in a harsh or ‘boney’ product. The point load strength index (PLSI) test is a convenient and widely used method for estimating the strength variation in drillcore. As a means of predicting UCS it has limitations, since the multiplier—usually quoted as 24—may range from about 12 for weak rock to 30 for very strong but brittle material. Elastic modulus The elastic modulus (E) of intact rock proposed as a source of aggregate is most useful as a factor in two derived parameters, modulus ratio (E/UCS) and toughness or resilience (UCS2/2E). Normally it is obtained as part of a UCS test, by attaching strain gauges to the specimen. High values of both UCS and E indicate that the rock resists crack penetration and is difficult to crush (i.e. stores strain energy and therefore reduces crusher throughput). Hardness Strictly speaking, hardness, as defined by Moh’s scale of scratch resistance (M), is a property of minerals rather than of intact rock, which is usually a composite of many minerals. It is, however, related to abradability, the resistance of an aggregate to tyre wear and polishing, and explains the quite different wear characteristics of limestone (mainly calcite, M=3) and granite (mainly quartz, M=7, and feldspar, M=6). Density, porosity and absorption Particle density, porosity and water absorption are interrelated properties, since the specific gravities (SGs) of most rock-forming silicates are in the range 2.6–2.7. Dry particle densities below 2.5 t/m3 indicate significant porosity in silicate rocks. This in turn implies low strength, reduced durability, high binder absorption and high abrasion wear rates in © 1998 G.H.McNally
aggregates from such sources. Note that particle density, often called particle SG, should not to be confused with the bulk density (from about 1.4 t/m3 loose, up to 2.4 t/m3 densely compacted) of crushed aggregate mixtures. It is also necessary to note whether the particle density determinations relate to oven-dry, air-dried (AD) or saturated/surface-dry (SSD) conditions. Water absorption (WA) of aggregate particles after 24 hours soaking is usually measured in preference to porosity, which requires more elaborate equipment. WA is generally less than porosity, often only half, since it depends not only on the pore space available but also on the diameter of the pores and their dryness. Nevertheless it is a useful indicator of nondurability in some rock types.
7.3 SIZING AND GRADING Sizing of aggregates Aggregate sizing is performed dry, using a series of standard sieves whose apertures generally range from about 40mm down to 75 µm (0.075 mm), each being roughly half the mesh width of the preceding one. The nominal size of each fraction is the smallest aperture at which 100% passes. The proportion retained on each sieve is weighed and plotted as a cumulative percentage passing versus particle diameter diagram such as Figure 7.3. It is assumed that the particles are equidimensional—hence sieve aperture equals grain diameter—and that their specific gravity (SG) is uniform. Elongate or prismatic particles cause the coarser fractions to be underestimated, while platy or flaky ones cause it to be overestimated. In other words, prismatic particles are retained one deck lower than their volume requires, while platy particles are held one deck too high. Particle sizing below 75 µm is impracticable using sieves, and instead is based on settling velocity in a water column dosed with dispersant. However, although the percentage of -75 µm fines in aggregate samples is of interest, the silt/clay proportion can more easily be estimated from Atterberg limits. The dust of crushing, predominantly non-plastic and silt-sized, adheres to damp aggregate chips—hence it is frequently underestimated by dry sieving—and must be released by washing. Grading of aggregates Grading, as the term is used in this book, is synonymous with particle size distribution (PSD), the end-result of the sieving process. The PSD of an aggregate, roadbase or subgrade soil has important implications for its geomechanical properties such as bearing capacity, shearing resistance, voids ratio (hence permeability) and compaction behaviour. Three types of © 1998 G.H.McNally
PSD are important for such applications as concrete and asphaltic mix design, pavement material evaluation and road surfacing: dense-graded, open-graded and gap-graded aggregate mixes (Figure 7.3). • Dense-graded mixes (also termed well graded, continuous graded, straight line graded) are characterized by an even blend of size fractions from coarse gravel to silt, such that the finer grains can—with the help of vibration, watering and compaction—fit between the coarser ones. This closer packing is evident in a higher mix density and reduced void space following compaction, which in turn means increased shear strength and layer stiffness. Dense-graded aggregate mixtures are used as unbound roadbase and in asphaltic concrete. In roadbase they may be composed of either fine crushed rock or natural gravel-sand-fines mixtures. Their strength and stiffness derive partly from interparticle friction and partly from the confinement offered by a low-voids compacted mass. • Open-graded aggregate blends (also termed no fines, harshly graded) contain an even mixture of coarse particle sizes, but little or no voidfilling fines. They are characterized by a steep PSD curve, and depend on friction between interlocking angular, coarse and rough-textured
Figure 7.3 Particle size distribution curves for different aggregate mixtures used for concrete, unbound roadbase and asphalt. © 1998 G.H.McNally
fragments for their strength and layer stiffness. This internal friction is greatest where the number of point-to-point and face-to-face contacts is maximized. Because of this, stronger and more abrasion-resistant aggregate particles are preferred than is the case with dense-graded roadbase. The other significant property of open-graded mixes is that they are more or less free-draining and not subject to capillary rise—an important consideration in shallow-water-table or frost-prone sites. The main disadvantage is that they are ‘harsh’ materials, meaning that they are difficult to spread and compact to their highest density—which is low relative to dense-graded mixes anyway. The classic open-graded aggregate mixture is railway ballast, but the same principle is used in the design of permeable asphalts, no-fines concretes, free-draining sub-bases and macadam pavements. A special case of open grading is uniform grading, in which only a single size fraction is represented. Two examples of this are the monosized cover aggregate used on sprayed seals (chip seals), and dune sand, used as fine aggregate in some concrete mixes. Uniform grading is indicated by near-vertical PSD curves, with negligible coarse tops and fine tails. • Gap-graded mixtures (also termed skip graded or ‘armchair’ graded) have an intermediate size fraction missing, generally coarse sand or fine gravel (say, 1–5 mm). This reduces their compacted density, leaves a proportion of voids unfilled, and makes them prone to segregation. Gap grading is common in natural road gravels, particularly in those derived from duricrusts, and is sometimes corrected by granular stabilization. Some concrete mixes are gap-graded, either by necessity—because only coarse aggregate and uniform sand are available—or because the use of rounded dune sand improves their workability.
Grading curves Particle size distributions in aggregate mixtures are represented pictorially by grading curves, also known as Fuller or Talbot curves, such as those shown in Figure 7.3. Because of the wide particle size range represented on these curves, sometimes 1 µm (0.001 mm) to 100 mm, the horizontal scale is logarithmic. Usually the coarsest sieve sizes are plotted on the right, but this may be reversed. Cumulative percentages finer than a particular grain size are shown in linear scale on the vertical axis. The PSD may be drawn as straight-line segments between sieve aperture sizes, or as smooth curves, or as grading envelopes enclosing the range of sizes acceptable in a particular product. These curves are mathematically described by the equation: P=100(d/D)n © 1998 G.H.McNally
where P is the percentage of particles finer than the sieve aperture d, D is the maximum particle size and n is Talbot’s factor. The shape of a PSD curve is defined by the Talbot exponent (n), with values in the range 0.4–0.5 for dense-graded roadbases, 1.5 or more for open-graded mixes, and around 0.3 for well-graded sands with an excess of fines. Dense-graded mixtures plot in Figure 7.3 as slightly concave curves spanning a wide range of particle sizes. Open gradings are shown by steep sigmoidal curves at the coarse (right-hand) end, while uniform (single-sized) sands, though not shown here, are even steeper (n=3–5). Gap-graded mixtures show up as stepped curves, with the flat segment indicating the deficient size fraction. ‘Poorly graded’ mixtures are any that depart significantly from the maximum density curve; hence they may be gap-graded, open-graded or uniformly graded. This is therefore a term that should be either discarded or only used when qualified.
7.4 PARTICLE SHAPE In an ideal aggregate mixture all particles should be equidimensional and angular, but not spherical (unless good workability has a higher priority than shear strength). In practice, a proportion of misshapen particles—flaky or elongate—is always present, but their percentage is severely limited in most specifications. The reasons for this stipulation, summarized in Figure 7.4, are as follows: • Some flaky particles are more easily stripped from bitumen seals, because they are held by only a narrow face in contact with the binder. • Elongated particles are more prone to flexural breakage, causing mixtures to become finer than their nominal grading. • Concrete mixes rich in misshapen fragments are difficult to pump and to compact. • These flakes may bridge across open voids in the mix, weakening it, or, if filled, will increase the cement demand. The causes of flakiness may be inherent (foliation or flow banding in the parent rock) or induced (by single-stage crushing, by reduction ratios above 3:1 or 4:1, and by excessive fines in the feedstock). Induced flakiness appears to be the more common, since foliated rocks are rarely crushed for aggregate, and flaky particles are common even where the feed stone has no obvious planar fabric. Hard, brittle rocks also appear to be more likely to generate misshapen fragments by splintering than tougher lithologies. The degree of departure from cubic shape is measured by the flakiness index, the weight percentage of particles in a sample that have a minimum © 1998 G.H.McNally
Figure 7.4 Consequences of flaky and elongate particles on aggregate behaviour in chip seals, concrete and asphalt.
dimension less than 0.6 times the mean, or by the elongation index, the proportion of prismatic particles longer than 1.8 times the mean. The main problem with these tests lies in selecting a truly representative group of stones to perform the required 200 measurements, and the fact that flaky or prismatic particles may be more prevalent in some size fractions than in others. There is some dispute as to whether jaws, gyratory or cone crushers give rise to the more flaky products, but it is accepted that impact crushers generate the most-equant particles. Hence poorly shaped products may be improved by tertiary crushing in an impactor, which © 1998 G.H.McNally
shatters particles by high-velocity blows rather than by squeezing (see Chapter 5).
7.5 SURFACE PROPERTIES ‘Surface properties’ of aggregates include all those factors influencing the bond between chips and bituminous binder in asphalt, and that between cement paste and aggregate in concrete. The skid resistance and tenacity of bituminous road surfacing materials is also dependent on these characteristics of sealing aggregates. The relevant aggregate properties comprise particle roughness, dustiness, moisture content and surface chemistry. Aggregate surface texture Aggregate surface texture is a function of mineral grain size and rock fabric. Fine-grained igneous rocks tend to have smooth or glassy fracture surfaces, medium- and coarse-grained ones are rougher textured, while some are visibly porous or even vesicular. The rougher the texture, the better the bond strength; one indication of this is the extent to which concrete test cylinder failure surfaces pass through aggregate particles (good bonding) or around them (weak bonding). Another piece of evidence is the fact that some relatively weak (UCS45 and their parent rocks include some finely vesicular basalts, harder scorias and slags, and some coarse but well-cemented orthoquartzites (‘gritstones’). Surprisingly, a few altered igneous rock types perform well, the secondary minerals being soft and the primary minerals harder. Erosion of the soft matrix minerals under traffic exposes rough crystals of the harder species, maintaining the rough microtexture while the chip diminishes in size.
7.6 SOUNDNESS, DURABILITY AND ABRADABILITY These are three properties that describe the tendency for aggregate to break down within its usual service life, say 10–100 years. This breakdown generally involves a reduction in chip size and an increase in the proportion of clay fines, plus weakening of the remaining coarse particles. The processes involved are similar to those of physical weathering. Chemical weathering (decomposition) is believed to contribute little, since the mineral species liberated are the same as those present in the parent rock prior to quarrying. What has changed as result of crushing, however, is the surface area of the source rock now exposed to the effects of atmospheric oxygen, stress relief, fluctuating moisture content and thermal cycling. Consider a typical blasted rock spall of volume 1m3 in a quarry muckpile: crushing this to nominal 10mm cubes increases its area a millionfold. Clays and fibrous secondary minerals previously locked up within the intact rock can now draw in airborne moisture, swell and further split the particles. The combination of cracking and water infusion can cause slaking, whereby moisture is sucked into newly created microfractures by capillary tension and compresses the air within, to the point where the rock chips literally explode. These are the reasons why some altered igneous rocks, which appear fresh and hard when first exposed, can deteriorate in stockpiles or road pavements within months. The effects of diminishing particle size on the rate of breakdown are illustrated in Figure 7.5. Note that the effects of © 1998 G.H.McNally
degradation by salt crystallization increase dramatically at sizes finer than 20 mm, and that the surface area per unit weight curve almost exactly parallels the degradation curve. • Soundness is the vaguest of the three ‘weatherability’ parameters used in engineering. Originally it may have referred to the fact that rock that is liable to break down in service is porous; when struck by a hammer it emits a dull thud, whereas better-quality rock will ‘ring’. As the term is presently understood, it means the extent to which aggregate chips or rock cubes will disintegrate in salt crystallization (‘sulphate soundness’) tests. • Abradability is more specific: it is the tendency of aggregate particles to wear away by abrasion (tyre-on-stone wear) or attrition (stone-on-stone rubbing). • Durability is another general term that can cover any form of in-service degradation, although it is best restricted to moisture-dependent, nonwearing processes. Abradability tests Abradability tests simulate on-road wear by ball milling, interparticle attrition and dropped weight impacts, in either the wet or dry state. The
Figure 7.5 Relationship between soundness (as measured by sulphate test loss) and particle diameter for single-sized chips from the same source. Note the close connection between surface area and weatherability, assuming all chips to be cubic. © 1998 G.H.McNally
samples used are closely sized coarse aggregate fractions, and the weight percentage of ‘fines’ (-2.36 mm or -1.18 mm) produced under standard conditions is taken as the measure of wear potential. The best known and oldest of the abradability tests is the Los Angeles abrasion (LAA) test, a dry milling procedure using steel balls. Its values are widely quoted and just as widely criticized, mainly on the grounds that steel ball impacts are unduly severe in simulating road conditions and that the test fails to allow for the weakening effects of water. Typical allowable losses as fines from good-quality aggregates are 25-40% in the LAA test. The Washington degradation test (WDT) more closely mimics on-road conditions, since water is added but there are no steel balls and the attriting action—20 minutes agitation in a sieve shaker—is more gentle. The WDT scale is also a more complex one, which gives a measure of both the amount of fines generated and their activity (i.e. clay content plus clay mineralogy). Durability tests Durability tests, or accelerated weathering tests, examine the wetting and drying behaviour of aggregates, with or without the addition of chemicals to hasten breakdown. The best known of these is the sulphate soundness test (SST), a method that combines salt wedging—by crystallization of Na 2SO 4 or MgSO 4—with alternate soaking and desiccation. Like the LAA test, it has been criticized for being unrealistically severe. Another way of assessing durability is to compare the saturated and oven-dry strengths, assuming that porous rocks are prone to disintegrate as moisture moves into and out of the interparticle voids. In Australia the most favoured aggregate durability test is the wet/dry strength variation in the ten per cent fines (TPF) test. The TPF test itself is primarily a means of assessing the crushing resistance of roadbase mixtures, and is described later in this chapter. The wet/dry strength variation is determined by performing the test on identical saturated surface-dry (SSD) and oven-dry specimens. Large differences between the ram loads required to generate 10% of fines indicate water-sensitive and therefore non-durable aggregate; similar low wet/dry strength ratios are characteristic of UCS results from weak and porous rock like sandstone.
7.7 STRENGTH AND STIFFNESS OF PARTICULATE MIXES As pointed out earlier, the properties of rock in a particulate mass—such as an aggregate mixture—differ greatly from those of the intact parent rock. Particle mixtures are weaker in compression, more deformable and have negligible tensile strength. This is not a problem in concrete because the © 1998 G.H.McNally
imposed load is carried by the hardened cement paste, but it may become so with unbound roadbase, since in this case the coarse aggregate framework supports and redistributes most of the stresses due to moving vehicles. Strength Strength in road pavement courses is defined by the point at which compressive strains become very large, due to some aggregate chips fracturing and rearranging themselves into a denser packing. However, general failure of a pavement section from a single loading is rare, because the stresses imposed by traffic are less than 10% of the ultimate (failure) stress for most granular materials. The problem therefore lies not in assessing the effects of one grossly overloaded truck, but from the passage of (say) 10 million heavy vehicles over 20 years. This is because each loading cycle imposes both recoverable (elastic or resilient) strains and irrecoverable (permanent or residual) strains on the compacted roadbase, as illustrated in Chapter 11. These permanent strains can accumulate to the point where general fatigue failure of the pavement occurs, as indicated by wheelpath rutting or other severe surface deformations. Stiffness Strength and deformability are thus closely related in roadbase materials, the stiffness modulus (or simply ‘stiffness’) being 50–100 times the peak strength. The term ‘stiffness’ is generally used in preference to ‘elastic modulus’ for particulate mixtures because their stress-strain behaviour is non-linear (i.e. not truly elastic). At the low stresses typical of wheel loadings the stress-strain curve is flatter (i.e. stiffness is less) than it is when approaching peak stress. Hence roadbase becomes both stiffer and more nearly elastic in its behaviour due to closer packing at high confining pressures. It also responds more stiffly to dynamic loading than to static or slowly applied loads. This is the reason why slow-moving trucks cause more furrowing in climbing lanes than in fast lanes, and why airport taxiways should be thicker than runways. Consider, for example, a hard limestone crushed to produce a well-graded highway basecourse. The parent rock in the intact state might have a UCS of 100 MPa, an elastic modulus of 40 GPa and a density of 2.7 t/m3 at 4% porosity. As a crushed and recompacted roadbase mixture its dry compressive strength might be only 5 MPa, its stiffness 300 MPa, its bulk density 2.1 t/m3 and its porosity 25%. Although the strength and stiffness of the aggregate mixture is much less than that of the intact rock, it is nevertheless quite adequate to handle the low level of trafficimposed stress, typically about 0.8 MPa (static) per truck wheel. In addition, both the © 1998 G.H.McNally
strength and stiffness of this roadbase are increased by confinement within a pavement.
7.8 TESTING OF PARTICULATE MIXES Triaxial testing Triaxial testing differs from the other methods used with particulate materials in that it can simulate confinement, repetitive traffic loadings, and variable moisture and compacted density. The test results—the shape and steepness of the Mohr failure envelope, stiffness and Poisson’s ratio—are directly usable as input for numerical models. Tests can be performed using a Texas triaxial cell or equivalent apparatus. The procedure is multistage, carried out on a single 100 mm× 150 mm cylindrical specimen at five successive lateral pressures in the range 0–200 kPa. The resulting failure envelope is compared with a set of standard curves, illustrated in Figure 7.6. Classes 1 and 2 are suitable as basecourses, class 3 as sub-base, and the flatter curves represent clay-rich materials unsuitable for pavement courses but of varying quality as subgrades. The repeated load triaxial test is a development of the standard Texas method, which simulates the effects of moving traffic by cyclic loading of the test cylinder. Ten minutes of vertical load pulsing at 30 Hz can represent 10– 20 years of truck traffic. The specimen is first ‘conditioned’ by about 1000 pulse repetitions, to mimic the bedding-down effects of traffic before the resilient modulus is measured. This is the material stiffness as indicated by the unloading portion of the stress-strain curve, which is thought to be more consistent than the loading half-cycle. Crushing resistance tests Routine methods of aggregate and roadbase assessment include several crushing resistance tests (not to be confused with UCS). These measure the weight percentage of fines generated by a standard compactive effort. A monosized coarse aggregate specimen contained within a cylindrical steel mould is loaded by the ram of a compression testing machine or struck repeatedly by a sliding weight (Figure 7.7). The proportion of -2.36 mm fines produced is considered to be inversely proportional to the sample’s strength and durability. In the aggregate crushing value (ACV) test, the compressive force is gradually raised to 400 kN and the weight percentage of fines liberated is measured. A high value indicates a weak, potentially non-durable material. This test is a useful alternative to the LAA test, because the crushing action is non-violent and hence better replicates on-road conditions. However, with © 1998 G.H.McNally
Figure 7.6 Texas triaxial test results (Mohr envelopes) for granular materials. The steep curves indicate high internal friction and rapid strength increase with confinement, hence suitability as unbound basecourse in flexible pavements.
some softer rocks used for crushed roadbase the voids tend to clog and prevent further ram penetration, putting an upper limit on the ACV. Another problem with the test is that flaky aggregates can increase the ACV by up to 60%, so particle shape must therefore be allowed for in the assessment. The aggregate impact value (AIV) test produces results that are numerically similar to ACV, but the loading is applied by a 14 kg dropped weight or sliding hammer. Hence the apparatus is portable and more suited to field laboratory use, though AIV is less widely used than either the ACV or TPF tests. © 1998 G.H.McNally
Figure 7.7 Test methods for comparing aggregate strength, based on the proportion of fines generated under standard loading conditions. © 1998 G.H.McNally
The ten per cent fines (TPF) test was devised to remedy the problem of void clogging in the ACV test, by limiting the amount of fines produced and recording the ram load (kN) to achieve this instead. Clearly, some judgement is required to generate exactly 10% fines; in practice, two tests are usually performed, with the aim of liberating about 7% and 13% fines. The ram load required for 10% fines is then estimated by proportioning between these values. The TPF test is also carried out on wet and dry aggregate samples, the wet/dry strength ratio being taken as a measure of durability (high wet/dry ratios indicating a sound material). The TPF is distantly related to the California bearing ratio (CBR) test, which was originally devised as a penetration resistance test for fine crushed rock roadbase, although it is now almost exclusively used for subgrade strength estimation. However, the CBR ram is much smaller than that in a compression machine, the apparatus is much less robust, and penetration is only 2.5 mm (compared to 15–25 mm for the TPF ram, the depth increasing as the aggregate becomes stronger).
7.9 PROPERTIES OF FINES The presence of ‘fines’ in aggregate mixtures—meaning, in this context, particles finer than 75 µm—may be necessary, tolerated, or severely limited, depending on the proposed use. Fines are necessary as binders in otherwise cohesionless roadbase or as void fillers in asphalt; they are tolerable up to a few per cent in concrete aggregate; but they can be a nuisance in sealing aggregate. Densegraded roadbase specifications include up to 10% of low-plasticity fines, predominantly silt. Most concrete mixes stipulate a maximum of 2–4% fines, though much larger percentages of fly ash (PFA) filler are often acceptable. Asphaltic mixes include up to 12% of -75 µm filler as a percentage of total aggregate weight, although 3–7% is more common. Its function here is not only to fill the finer voids, but also to stiffen the bitumen binder. Sealing aggregates, on the other hand, are required to be ‘dry and dust-free’. They are normally precoated to improve the bitumen-to-stone bond and thereby reduce any tendency to strip. The type of fines and their occurrence, as well as their amount, are important as well. Evenly distributed coarse inert silt ‘rock flour’ or crusher dust is much more acceptable than active clay minerals. Limonite coatings, fine mica flakes, organic matter and adhering mud are also objectionable to varying degrees, depending on the end-use. The desirable properties of mineral filler, as opposed to deleterious clay, are not stated in specifications, but appear to be the following: • There should be a predominance of coarse silt-sized particles, say 20–75 µm, which should be dry, and made up of quartz or carbonate grains (but not mica flakes). © 1998 G.H.McNally
• Particles should preferably be rounded, like fly ash, cement or ball-milled limestone dust. Surface charge should be minimal. • The filler grains should not be attached to aggregate particles, but added dry in weighted quantities during batching to ensure even distribution through the mixture. In assessing the significance of fines in aggregate mixes, it is usually sufficient to know the weight proportion of -425 µm material (the fraction used for consistency limit tests), that of -75 µm material, and the consistency limits themselves. The latter are better known as Atterberg limits (liquid limit, LL; plastic limit, PL; and plasticity index, PI=LL— PL). Silt-dominant mixtures are indicated by LL